# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2017

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1_sq
_database_code_depnum_ccdc_archive 'CCDC 991332'
_audit_update_record             
;
2017-10-04 deposited with the CCDC.
2017-10-09 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C32 H113 Er Ge2 Mo22 N8 O100'
_chemical_formula_weight         4633.42

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           7
_space_group_name_H-M_alt        'P n'
_space_group_name_Hall           'P -2yac'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'x+1/2, -y, z+1/2'

_cell_length_a                   13.1184(6)
_cell_length_b                   12.6369(5)
_cell_length_c                   32.3036(12)
_cell_angle_alpha                90
_cell_angle_beta                 96.168(4)
_cell_angle_gamma                90
_cell_volume                     5324.2(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    5780
_cell_measurement_theta_min      2.8269
_cell_measurement_theta_max      29.1761

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.890
_exptl_crystal_F_000             4434
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.450
_exptl_crystal_size_mid          0.350
_exptl_crystal_size_min          0.320
_exptl_absorpt_coefficient_mu    3.956
_shelx_estimated_absorpt_T_min   0.269
_shelx_estimated_absorpt_T_max   0.364
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.93987
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   ?

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Enhance (Mo) X-ray Source'
_diffrn_measurement_device_type  'Xcalibur, Ruby, Gemini ultra'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            20044
_diffrn_reflns_av_unetI/netI     0.0829
_diffrn_reflns_av_R_equivalents  0.0535
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_theta_min         3.006
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measured_fraction_theta_full 0.970
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_Laue_measured_fraction_full 0.970
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_point_group_measured_fraction_full 0.970
_reflns_number_total             12711
_reflns_number_gt                11203
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.999
_reflns_Friedel_fraction_max     0.996
_reflns_Friedel_fraction_full    0.970

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_cell_refinement       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction        
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXTL

_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0447P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.295(14)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         12711
_refine_ls_number_parameters     1184
_refine_ls_number_restraints     92
_refine_ls_R_factor_all          0.0530
_refine_ls_R_factor_gt           0.0452
_refine_ls_wR_factor_ref         0.1082
_refine_ls_wR_factor_gt          0.1032
_refine_ls_goodness_of_fit_ref   1.013
_refine_ls_restrained_S_all      13.932
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.4331(17) -0.1131(19) 0.3940(7) 0.042(6) Uani 1 1 d . U . . .
H1A H 0.3820 -0.0947 0.4124 0.050 Uiso 1 1 calc R U . . .
H1B H 0.4017 -0.1609 0.3728 0.050 Uiso 1 1 calc R U . . .
C2 C 0.469(2) -0.014(2) 0.3735(9) 0.061(8) Uani 1 1 d . . . . .
H2A H 0.5176 -0.0329 0.3540 0.074 Uiso 1 1 calc R U . . .
H2B H 0.4113 0.0210 0.3581 0.074 Uiso 1 1 calc R U . . .
C3 C 0.5746(18) -0.0893(18) 0.4465(8) 0.048(7) Uani 1 1 d . . . . .
H3A H 0.6373 -0.1235 0.4583 0.058 Uiso 1 1 calc R U . . .
H3B H 0.5341 -0.0729 0.4691 0.058 Uiso 1 1 calc R U . . .
C4 C 0.601(2) 0.013(2) 0.4248(9) 0.054(7) Uani 1 1 d . . . . .
H4A H 0.6349 0.0613 0.4454 0.064 Uiso 1 1 calc R U . . .
H4B H 0.6491 -0.0023 0.4048 0.064 Uiso 1 1 calc R U . . .
C5 C 0.5559(18) 0.202(3) 0.3079(8) 0.078(11) Uani 1 1 d D . . . .
H5A H 0.4831 0.2091 0.2994 0.093 Uiso 1 1 calc R U . . .
H5B H 0.5656 0.1572 0.3325 0.093 Uiso 1 1 calc R U . . .
C6 C 0.604(2) 0.302(2) 0.3154(11) 0.114(14) Uiso 1 1 d D . . . .
H6A H 0.5801 0.3464 0.2916 0.137 Uiso 1 1 calc DR U . . .
H6B H 0.5746 0.3324 0.3391 0.137 Uiso 1 1 calc DR U . . .
C7 C 0.7217(17) 0.1689(18) 0.2795(7) 0.039(6) Uani 1 1 d . . . . .
H7A H 0.7540 0.1487 0.2550 0.047 Uiso 1 1 calc R U . . .
H7B H 0.7486 0.1236 0.3023 0.047 Uiso 1 1 calc R U . . .
C8 C 0.745(2) 0.2770(19) 0.2897(8) 0.052(7) Uani 1 1 d . . . . .
H8A H 0.8194 0.2838 0.2947 0.063 Uiso 1 1 calc R U . . .
H8B H 0.7230 0.3201 0.2656 0.063 Uiso 1 1 calc R U . . .
C9 C 0.354(2) 0.657(2) 0.6586(8) 0.050(7) Uani 1 1 d . . . . .
H9A H 0.2840 0.6660 0.6463 0.060 Uiso 1 1 calc R U . . .
H9B H 0.3917 0.6178 0.6394 0.060 Uiso 1 1 calc R U . . .
C10 C 0.4035(14) 0.7633(17) 0.6680(7) 0.031(5) Uani 1 1 d . . . . .
H10A H 0.4059 0.8025 0.6423 0.037 Uiso 1 1 calc R U . . .
H10B H 0.3629 0.8036 0.6858 0.037 Uiso 1 1 calc R U . . .
C11 C 0.456(2) 0.5826(19) 0.7191(10) 0.061(8) Uani 1 1 d . . . . .
H11A H 0.4942 0.5392 0.7014 0.073 Uiso 1 1 calc R U . . .
H11B H 0.4503 0.5444 0.7448 0.073 Uiso 1 1 calc R U . . .
C12 C 0.5095(19) 0.682(2) 0.7282(7) 0.050(7) Uani 1 1 d . . . . .
H12A H 0.5797 0.6680 0.7395 0.060 Uiso 1 1 calc R U . . .
H12B H 0.4765 0.7210 0.7490 0.060 Uiso 1 1 calc R U . . .
C13 C 0.796(3) 0.247(2) 0.4638(10) 0.076(10) Uani 1 1 d . . . . .
H13A H 0.7956 0.1912 0.4433 0.091 Uiso 1 1 calc R U . . .
H13B H 0.8268 0.2193 0.4903 0.091 Uiso 1 1 calc R U . . .
C14 C 0.861(2) 0.340(2) 0.4507(11) 0.076(9) Uani 1 1 d . . . . .
H14A H 0.9310 0.3180 0.4491 0.092 Uiso 1 1 calc R U . . .
H14B H 0.8609 0.3974 0.4708 0.092 Uiso 1 1 calc R U . . .
C15 C 0.649(3) 0.307(4) 0.4274(14) 0.125(15) Uani 1 1 d . U . . .
H15A H 0.5779 0.3254 0.4288 0.150 Uiso 1 1 calc R U . . .
H15B H 0.6526 0.2485 0.4080 0.150 Uiso 1 1 calc R U . . .
C16 C 0.710(3) 0.402(3) 0.4143(13) 0.107(13) Uani 1 1 d . U . . .
H16A H 0.6739 0.4321 0.3893 0.129 Uiso 1 1 calc R U . . .
H16B H 0.7120 0.4549 0.4361 0.129 Uiso 1 1 calc R U . . .
C17 C 0.357(4) 0.486(4) 0.2799(16) 0.130(16) Uani 1 1 d . U . . .
H17A H 0.3216 0.4236 0.2879 0.156 Uiso 1 1 calc R U . . .
H17B H 0.3917 0.4675 0.2558 0.156 Uiso 1 1 calc R U . . .
C18 C 0.286(3) 0.561(3) 0.2677(14) 0.120(15) Uani 1 1 d . U . . .
H18A H 0.2419 0.5733 0.2895 0.144 Uiso 1 1 calc R U . . .
H18B H 0.2440 0.5384 0.2427 0.144 Uiso 1 1 calc R U . . .
C19 C 0.433(3) 0.680(3) 0.2935(12) 0.094(11) Uani 1 1 d . U . . .
H19A H 0.4798 0.7340 0.2856 0.113 Uiso 1 1 calc R U . . .
H19B H 0.4035 0.7052 0.3181 0.113 Uiso 1 1 calc R U . . .
C20 C 0.485(3) 0.590(3) 0.3028(14) 0.107(13) Uani 1 1 d . U . . .
H20A H 0.5222 0.5718 0.2794 0.128 Uiso 1 1 calc R U . . .
H20B H 0.5351 0.6033 0.3265 0.128 Uiso 1 1 calc R U . . .
N1 N 0.5160(14) -0.1629(14) 0.4167(5) 0.039(5) Uani 1 1 d . . . . .
H1C H 0.5577 -0.1886 0.3991 0.047 Uiso 1 1 calc R U . . .
H1D H 0.4932 -0.2170 0.4307 0.047 Uiso 1 1 calc R U . . .
N2 N 0.6134(15) 0.1547(14) 0.2716(6) 0.044(5) Uani 1 1 d . U . . .
H2C H 0.5994 0.0860 0.2689 0.053 Uiso 1 1 calc R U . . .
H2D H 0.5908 0.1865 0.2478 0.053 Uiso 1 1 calc R U . . .
N3 N 0.3575(14) 0.6021(15) 0.6989(7) 0.045(5) Uani 1 1 d . . . . .
H3C H 0.3228 0.6404 0.7158 0.054 Uiso 1 1 calc R U . . .
H3D H 0.3252 0.5404 0.6948 0.054 Uiso 1 1 calc R U . . .
N4 N 0.698(2) 0.2797(17) 0.4675(7) 0.070(8) Uani 1 1 d . . . . .
H4C H 0.6986 0.3356 0.4843 0.084 Uiso 1 1 calc R U . . .
H4D H 0.6632 0.2280 0.4784 0.084 Uiso 1 1 calc R U . . .
N5 N 0.4304(17) 0.5095(16) 0.3112(8) 0.067(7) Uani 1 1 d . . . . .
H5C H 0.4008 0.5228 0.3342 0.081 Uiso 1 1 calc R U . . .
H5D H 0.4712 0.4536 0.3162 0.081 Uiso 1 1 calc DR U . . .
O1 O 0.0882(10) 0.9407(9) 0.4673(4) 0.022(3) Uani 1 1 d . . . . .
O2 O -0.1136(10) 1.0234(10) 0.4355(4) 0.027(3) Uani 1 1 d . . . . .
O3 O -0.2237(9) 0.9779(10) 0.5004(4) 0.021(3) Uani 1 1 d . . . . .
O4 O -0.1424(9) 0.9441(9) 0.5797(4) 0.016(3) Uani 1 1 d . . . . .
O5 O 0.0601(9) 0.9863(10) 0.6106(4) 0.023(3) Uani 1 1 d . . . . .
O6 O 0.1132(10) 0.7702(10) 0.6902(4) 0.022(3) Uani 1 1 d . U . . .
O7 O -0.0704(10) 0.6337(9) 0.5662(4) 0.023(3) Uani 1 1 d . . . . .
O8 O -0.2290(9) 0.7480(10) 0.6010(4) 0.022(3) Uani 1 1 d . . . . .
O9 O -0.2675(10) 0.7128(10) 0.6874(4) 0.024(3) Uani 1 1 d . . . . .
O10 O -0.3269(10) 0.9065(10) 0.7086(4) 0.024(3) Uani 1 1 d D . . . .
O11 O -0.3041(10) 0.4989(10) 0.6662(4) 0.032(3) Uani 1 1 d . . . . .
O12 O -0.3931(10) 0.6626(10) 0.6211(4) 0.028(3) Uani 1 1 d . . . . .
O13 O -0.1216(9) 0.6079(10) 0.6591(4) 0.023(3) Uani 1 1 d . . . . .
O14 O 0.0699(9) 0.6136(10) 0.6330(4) 0.024(3) Uani 1 1 d . . . . .
O15 O 0.0501(10) 0.5708(11) 0.7140(4) 0.031(3) Uani 1 1 d . . . . .
O16 O -0.0274(9) 0.7923(9) 0.6284(4) 0.017(3) Uani 1 1 d . . . . .
O17 O 0.2228(10) 0.9433(12) 0.6716(5) 0.037(4) Uani 1 1 d . . . . .
O18 O 0.1573(9) 0.7995(10) 0.6115(4) 0.026(3) Uani 1 1 d . . . . .
O19 O -0.3512(9) 0.8961(10) 0.5540(4) 0.020(3) Uani 1 1 d . . . . .
O20 O -0.1834(9) 0.9036(9) 0.6628(4) 0.017(3) Uiso 1 1 d . . . . .
O21 O 0.0195(10) 0.8103(11) 0.5421(4) 0.028(3) Uani 1 1 d . . . . .
O22 O -0.1758(10) 0.7624(10) 0.5136(4) 0.029(3) Uani 1 1 d . . . . .
O23 O -0.2195(13) 0.5537(13) 0.5057(5) 0.047(4) Uani 1 1 d . . . . .
O24 O -0.1861(10) 0.8081(10) 0.4300(4) 0.023(3) Uani 1 1 d . U . . .
O25 O 0.1583(10) 0.6104(10) 0.4402(4) 0.026(3) Uani 1 1 d . . . . .
O26 O 0.2243(10) 0.7509(9) 0.3435(4) 0.024(3) Uani 1 1 d . . . . .
O27 O 0.1759(9) 0.9466(10) 0.3570(4) 0.024(3) Uani 1 1 d . . . . .
O28 O 0.0592(10) 1.0768(10) 0.4000(4) 0.025(3) Uani 1 1 d . . . . .
O29 O -0.1259(11) 1.1712(10) 0.3752(4) 0.030(3) Uani 1 1 d . . . . .
O30 O -0.0340(10) 1.0373(10) 0.3235(4) 0.030(3) Uani 1 1 d . . . . .
O31 O -0.3312(11) 0.6604(11) 0.4240(5) 0.037(4) Uani 1 1 d . . . . .
O32 O -0.1486(9) 0.7534(9) 0.3475(4) 0.015(3) Uani 1 1 d . U . . .
O33 O -0.1697(9) 0.9134(9) 0.2803(4) 0.020(3) Uiso 1 1 d . . . . .
O34 O 0.0248(9) 0.8271(9) 0.3101(4) 0.017(3) Uani 1 1 d . . . . .
O35 O 0.1096(11) 0.9818(10) 0.2777(4) 0.032(4) Uani 1 1 d D . . . .
O36 O 0.0749(10) 0.5994(10) 0.2947(4) 0.029(3) Uani 1 1 d . . . . .
O37 O 0.1607(10) 0.7763(10) 0.2652(4) 0.026(3) Uani 1 1 d . . . . .
O38 O 0.3084(10) 0.9176(11) 0.3013(5) 0.036(4) Uani 1 1 d D . . . .
O39 O -0.0054(9) 0.8943(10) 0.3904(4) 0.020(3) Uani 1 1 d . . . . .
O40 O 0.1358(11) 0.6326(11) 0.5549(5) 0.039(4) Uani 1 1 d . . . . .
O41 O -0.0232(11) 0.8534(12) 0.2359(4) 0.036(4) Uani 1 1 d D . . . .
O42 O 0.0431(11) 0.6533(11) 0.2119(4) 0.034(4) Uani 1 1 d . . . . .
O43 O -0.3276(9) 0.8018(9) 0.3624(4) 0.018(3) Uani 1 1 d . U . . .
O44 O -0.2717(10) 0.6046(10) 0.3473(4) 0.027(3) Uani 1 1 d . . . . .
O45 O -0.0903(11) 0.5390(10) 0.3244(4) 0.030(3) Uani 1 1 d . . . . .
O46 O -0.1322(10) 0.6079(10) 0.4156(4) 0.027(3) Uani 1 1 d . . . . .
O47 O 0.0189(10) 0.4823(10) 0.3973(4) 0.028(3) Uani 1 1 d . . . . .
O48 O 0.0433(9) 0.6775(9) 0.3764(4) 0.017(3) Uani 1 1 d . . . . .
O49 O 0.3400(9) 0.6602(11) 0.4079(4) 0.030(3) Uani 1 1 d . . . . .
O50 O 0.1927(9) 0.8122(9) 0.4191(4) 0.019(3) Uani 1 1 d . . . . .
O51 O -0.1042(10) 0.6828(11) 0.2676(4) 0.030(3) Uani 1 1 d . . . . .
O52 O -0.2647(11) 0.5369(11) 0.2669(5) 0.038(4) Uani 1 1 d . . . . .
O53 O -0.3718(9) 0.9415(10) 0.2987(5) 0.031(3) Uani 1 1 d . . . . .
O54 O -0.1973(9) 0.9694(9) 0.3558(4) 0.019(3) Uani 1 1 d . . . . .
O55 O 0.0045(11) 0.5240(12) 0.4809(5) 0.040(4) Uani 1 1 d . . . . .
O56 O 0.2491(10) 1.0212(11) 0.4354(5) 0.033(4) Uani 1 1 d . . . . .
O57 O -0.0144(10) 1.0296(9) 0.5284(4) 0.024(3) Uani 1 1 d . U . . .
O58 O -0.3560(10) 0.6862(11) 0.5420(4) 0.028(3) Uani 1 1 d . . . . .
O59 O -0.3886(10) 0.8705(10) 0.6310(4) 0.025(3) Uani 1 1 d . . . . .
O60 O -0.1717(10) 1.1311(9) 0.5600(4) 0.024(3) Uani 1 1 d . U . . .
O61 O 0.1842(9) 0.5486(10) 0.3632(4) 0.030(3) Uani 1 1 d . . . . .
O62 O 0.0652(11) 0.3904(11) 0.3255(5) 0.038(4) Uani 1 1 d . . . . .
O63 O -0.0691(11) 1.0634(11) 0.2388(4) 0.034(4) Uani 1 1 d . . . . .
O64 O -0.0017(11) 0.7354(10) 0.4610(5) 0.032(4) Uani 1 1 d . . . . .
O65 O -0.2891(10) 0.7451(11) 0.2852(4) 0.029(3) Uani 1 1 d . . . . .
O66 O -0.3713(10) 1.1023(11) 0.5260(4) 0.032(3) Uani 1 1 d . . . . .
O67 O -0.2219(11) 0.7778(11) 0.7692(4) 0.033(4) Uani 1 1 d . . . . .
O68 O -0.1206(10) 0.9494(10) 0.7366(4) 0.026(3) Uani 1 1 d D . . . .
O69 O 0.0208(9) 0.9595(9) 0.6869(4) 0.021(3) Uani 1 1 d . . . . .
O70 O -0.0454(11) 1.1495(11) 0.7225(4) 0.033(3) Uani 1 1 d . . . . .
O71 O -0.2467(10) 0.5473(9) 0.5907(4) 0.027(3) Uani 1 1 d . . . . .
O72 O -0.0740(9) 0.7555(10) 0.7135(4) 0.020(3) Uani 1 1 d . . . . .
O73 O 0.0243(12) 1.1900(10) 0.5814(5) 0.039(4) Uani 1 1 d . . . . .
O74 O -0.0838(10) 1.0978(10) 0.6396(4) 0.025(3) Uani 1 1 d . . . . .
O75 O -0.2366(10) 1.0854(10) 0.6886(4) 0.026(3) Uani 1 1 d . . . . .
O76 O -0.4418(10) 1.0632(12) 0.6639(4) 0.036(4) Uani 1 1 d D . . . .
O77 O -0.5243(10) 0.7819(12) 0.5688(4) 0.036(4) Uani 1 1 d . . . . .
O78 O -0.3089(10) 1.0489(10) 0.6073(4) 0.027(3) Uani 1 1 d . . . . .
O79 O 0.5200(14) 0.0612(13) 0.4055(5) 0.058(5) Uani 1 1 d . . . . .
O80 O 0.7050(14) 0.3170(13) 0.3224(6) 0.057(5) Uani 1 1 d . . . . .
O81 O 0.5093(12) 0.7494(14) 0.6890(5) 0.052(4) Uani 1 1 d . . . . .
O82 O 0.8111(18) 0.3789(17) 0.4066(8) 0.089(8) Uani 1 1 d . . . . .
O83 O 0.3495(19) 0.665(3) 0.2591(9) 0.127(11) Uani 1 1 d . . . . .
Ge1 Ge -0.14617(15) 0.84826(15) 0.61745(6) 0.0158(4) Uani 1 1 d . . . . .
Ge2 Ge -0.02019(14) 0.78963(15) 0.35714(6) 0.0159(4) Uani 1 1 d . . . . .
Mo1 Mo -0.39731(13) 0.78274(14) 0.58281(5) 0.0246(4) Uani 1 1 d . . . . .
Mo2 Mo -0.23417(12) 0.70183(13) 0.40045(5) 0.0210(4) Uani 1 1 d . . . . .
Mo3 Mo -0.27268(13) 0.86765(13) 0.31941(5) 0.0236(4) Uani 1 1 d . . . . .
Mo4 Mo -0.19710(13) 0.80702(13) 0.71984(5) 0.0210(4) Uani 1 1 d . . . . .
Mo5 Mo -0.27214(13) 1.02368(13) 0.54454(5) 0.0226(4) Uani 1 1 d . . . . .
Mo6 Mo 0.18928(12) 0.88594(13) 0.30820(5) 0.0218(4) Uani 1 1 d . . . . .
Mo7 Mo -0.26306(13) 0.60083(13) 0.63990(5) 0.0232(4) Uani 1 1 d . . . . .
Mo8 Mo -0.33556(13) 1.00007(14) 0.65644(5) 0.0236(4) Uani 1 1 d . . . . .
Mo9 Mo 0.13977(13) 0.95543(14) 0.42018(5) 0.0229(4) Uani 1 1 d . . . . .
Mo10 Mo 0.11199(13) 0.88903(14) 0.65185(6) 0.0262(4) Uani 1 1 d . . . . .
Mo11 Mo 0.05308(14) 0.71075(14) 0.57711(5) 0.0257(4) Uani 1 1 d . . . . .
Mo12 Mo 0.01611(13) 0.60863(13) 0.44100(5) 0.0226(4) Uani 1 1 d . . . . .
Mo13 Mo -0.03692(13) 1.07429(13) 0.57739(5) 0.0225(4) Uani 1 1 d . . . . .
Mo14 Mo -0.09160(14) 1.04932(13) 0.68994(5) 0.0243(4) Uani 1 1 d . . . . .
Mo15 Mo -0.08591(13) 1.04541(12) 0.38454(5) 0.0221(4) Uani 1 1 d . . . . .
Mo16 Mo 0.21679(13) 0.68258(14) 0.39176(6) 0.0258(4) Uani 1 1 d . . . . .
Mo17 Mo -0.20581(13) 0.61932(14) 0.30267(6) 0.0261(4) Uani 1 1 d . . . . .
Mo18 Mo 0.04790(14) 0.51130(13) 0.34519(6) 0.0268(4) Uani 1 1 d . . . . .
Mo19 Mo -0.04566(13) 0.97035(13) 0.27518(5) 0.0221(4) Uani 1 1 d . . . . .
Mo20 Mo 0.01326(13) 0.65847(13) 0.67658(5) 0.0236(4) Uani 1 1 d . . . . .
Mo21 Mo 0.03088(13) 0.70561(14) 0.25871(5) 0.0250(4) Uani 1 1 d . . . . .
Mo22 Mo -0.21101(14) 0.65333(13) 0.54128(5) 0.0244(4) Uani 1 1 d . . . . .
Er1 Er -0.07583(7) 0.88706(7) 0.48284(3) 0.0241(2) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N1 1.39(3) . ?
C1 C2 1.52(3) . ?
C2 O79 1.50(3) . ?
C3 N1 1.49(3) . ?
C3 C4 1.53(3) . ?
C4 O79 1.32(3) . ?
C5 C6 1.43(2) . ?
C5 N2 1.58(3) . ?
C6 O80 1.34(3) . ?
C7 N2 1.43(3) . ?
C7 C8 1.43(3) . ?
C8 O80 1.33(3) . ?
C9 N3 1.47(3) . ?
C9 C10 1.50(3) . ?
C10 O81 1.49(2) . ?
C11 N3 1.40(3) . ?
C11 C12 1.46(3) . ?
C12 O81 1.52(3) . ?
C13 N4 1.37(4) . ?
C13 C14 1.53(4) . ?
C14 O82 1.58(4) . ?
C15 N4 1.42(5) . ?
C15 C16 1.53(5) . ?
C16 O82 1.41(4) . ?
C17 N5 1.35(5) . ?
C17 C18 1.36(5) . ?
C18 O83 1.60(4) . ?
C19 C20 1.35(4) . ?
C19 O83 1.49(4) . ?
C20 N5 1.29(4) . ?
O1 Mo9 1.742(12) . ?
O1 Er1 2.361(12) . ?
O2 Mo15 1.745(13) . ?
O2 Er1 2.322(14) . ?
O3 Mo5 1.723(11) . ?
O3 Er1 2.375(11) . ?
O4 Ge1 1.724(11) . ?
O4 Mo13 2.156(12) . ?
O4 Mo5 2.187(12) . ?
O5 Mo10 1.887(13) . ?
O5 Mo13 1.926(13) . ?
O6 Mo10 1.945(12) . ?
O6 Mo20 1.945(13) . ?
O7 Mo11 1.890(13) . ?
O7 Mo22 1.948(13) . ?
O8 Ge1 1.716(12) . ?
O8 Mo1 2.266(12) . ?
O8 Mo22 2.304(12) . ?
O8 Mo7 2.314(13) . ?
O9 Mo4 1.777(12) . ?
O9 Mo7 2.093(12) . ?
O10 Mo8 2.052(13) . ?
O10 Mo4 2.117(12) . ?
O11 Mo7 1.665(13) . ?
O12 Mo7 1.915(14) . ?
O12 Mo1 1.956(13) . ?
O13 Mo7 1.894(13) . ?
O13 Mo20 1.908(13) . ?
O14 Mo20 1.756(13) . ?
O14 Mo11 2.174(13) . ?
O15 Mo20 1.674(13) . ?
O16 Ge1 1.712(12) . ?
O16 Mo10 2.261(12) . ?
O16 Mo11 2.303(11) . ?
O16 Mo20 2.321(12) . ?
O17 Mo10 1.671(14) . ?
O18 Mo10 1.870(12) . ?
O18 Mo11 2.009(13) . ?
O19 Mo1 1.845(12) . ?
O19 Mo5 1.959(12) . ?
O20 Ge1 1.740(11) . ?
O20 Mo4 2.234(12) . ?
O20 Mo14 2.321(12) . ?
O20 Mo8 2.328(12) . ?
O21 Mo11 1.716(13) . ?
O21 Er1 2.379(14) . ?
O22 Mo22 1.733(13) . ?
O22 Er1 2.338(13) . ?
O23 Mo22 1.700(16) . ?
O24 Mo2 1.727(13) . ?
O24 Er1 2.339(13) . ?
O25 Mo12 1.869(13) . ?
O25 Mo16 2.032(12) . ?
O26 Mo16 1.795(13) . ?
O26 Mo6 2.076(12) . ?
O27 Mo6 1.779(12) . ?
O27 Mo9 2.147(12) . ?
O28 Mo9 1.935(14) . ?
O28 Mo15 1.956(14) . ?
O29 Mo15 1.691(13) . ?
O30 Mo19 1.768(13) . ?
O30 Mo15 2.156(13) . ?
O31 Mo2 1.638(13) . ?
O32 Ge2 1.742(12) . ?
O32 Mo2 2.240(11) . ?
O32 Mo3 2.289(12) . ?
O32 Mo17 2.302(12) . ?
O33 Mo19 1.803(12) . ?
O33 Mo3 2.030(11) . ?
O34 Ge2 1.754(11) . ?
O34 Mo21 2.268(12) . ?
O34 Mo19 2.276(12) . ?
O34 Mo6 2.289(11) . ?
O35 Mo6 1.819(15) . ?
O35 Mo19 2.035(14) . ?
O36 Mo21 1.828(14) . ?
O36 Mo18 2.036(13) . ?
O37 Mo21 1.915(13) . ?
O37 Mo6 1.969(13) . ?
O38 Mo6 1.651(13) . ?
O39 Ge2 1.702(12) . ?
O39 Mo9 2.180(13) . ?
O39 Mo15 2.180(12) . ?
O40 Mo11 1.685(12) . ?
O41 Mo19 1.990(15) . ?
O41 Mo21 2.102(14) . ?
O42 Mo21 1.674(13) . ?
O43 Mo3 1.832(11) . ?
O43 Mo2 2.070(12) . ?
O44 Mo17 1.767(12) . ?
O44 Mo2 2.127(13) . ?
O45 Mo17 1.895(14) . ?
O45 Mo18 1.897(14) . ?
O46 Mo2 1.816(13) . ?
O46 Mo12 2.028(14) . ?
O47 Mo18 1.804(13) . ?
O47 Mo12 2.133(13) . ?
O48 Ge2 1.725(12) . ?
O48 Mo16 2.278(12) . ?
O48 Mo12 2.323(11) . ?
O48 Mo18 2.334(12) . ?
O49 Mo16 1.669(13) . ?
O50 Mo16 1.904(11) . ?
O50 Mo9 1.940(11) . ?
O51 Mo21 1.848(13) . ?
O51 Mo17 2.007(13) . ?
O52 Mo17 1.681(14) . ?
O53 Mo3 1.680(13) . ?
O54 Mo15 1.904(12) . ?
O54 Mo3 1.940(12) . ?
O55 Mo12 1.694(13) . ?
O56 Mo9 1.685(13) . ?
O57 Mo13 1.734(13) . ?
O57 Er1 2.410(13) . ?
O58 Mo1 1.918(12) . ?
O58 Mo22 1.949(13) . ?
O59 Mo1 1.905(13) . ?
O59 Mo8 1.928(13) . ?
O60 Mo5 1.920(13) . ?
O60 Mo13 1.935(13) . ?
O61 Mo18 1.880(12) . ?
O61 Mo16 1.953(13) . ?
O62 Mo18 1.679(13) . ?
O63 Mo19 1.668(13) . ?
O64 Mo12 1.753(13) . ?
O64 Er1 2.294(12) . ?
O65 Mo3 1.902(13) . ?
O65 Mo17 1.976(14) . ?
O66 Mo5 1.694(13) . ?
O67 Mo4 1.701(13) . ?
O68 Mo14 2.035(13) . ?
O68 Mo4 2.102(12) . ?
O69 Mo14 1.871(12) . ?
O69 Mo10 1.950(11) . ?
O70 Mo14 1.715(14) . ?
O71 Mo7 1.762(12) . ?
O71 Mo22 2.172(13) . ?
O72 Mo4 1.773(12) . ?
O72 Mo20 2.129(12) . ?
O73 Mo13 1.666(12) . ?
O74 Mo14 1.751(13) . ?
O74 Mo13 2.185(12) . ?
O75 Mo8 1.908(13) . ?
O75 Mo14 1.952(13) . ?
O76 Mo8 1.646(12) . ?
O77 Mo1 1.679(14) . ?
O78 Mo8 1.771(13) . ?
O78 Mo5 2.159(13) . ?
Mo5 Mo13 3.218(2) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N1 C1 C2 110(2) . . ?
O79 C2 C1 111(2) . . ?
N1 C3 C4 111(2) . . ?
O79 C4 C3 113(2) . . ?
C6 C5 N2 103(2) . . ?
O80 C6 C5 124(2) . . ?
N2 C7 C8 110.4(19) . . ?
O80 C8 C7 116.7(19) . . ?
N3 C9 C10 106(2) . . ?
O81 C10 C9 110.2(17) . . ?
N3 C11 C12 110(2) . . ?
C11 C12 O81 111(2) . . ?
N4 C13 C14 110(2) . . ?
C13 C14 O82 107(3) . . ?
N4 C15 C16 104(3) . . ?
O82 C16 C15 115(3) . . ?
N5 C17 C18 119(4) . . ?
C17 C18 O83 105(4) . . ?
C20 C19 O83 112(3) . . ?
N5 C20 C19 116(4) . . ?
C1 N1 C3 112.2(18) . . ?
C7 N2 C5 111.6(18) . . ?
C11 N3 C9 115.6(19) . . ?
C13 N4 C15 109(3) . . ?
C20 N5 C17 112(3) . . ?
Mo9 O1 Er1 131.7(7) . . ?
Mo15 O2 Er1 133.5(7) . . ?
Mo5 O3 Er1 138.0(7) . . ?
Ge1 O4 Mo13 128.9(7) . . ?
Ge1 O4 Mo5 127.6(6) . . ?
Mo13 O4 Mo5 95.6(4) . . ?
Mo10 O5 Mo13 159.4(7) . . ?
Mo10 O6 Mo20 117.2(7) . . ?
Mo11 O7 Mo22 140.0(7) . . ?
Ge1 O8 Mo1 120.3(6) . . ?
Ge1 O8 Mo22 121.6(6) . . ?
Mo1 O8 Mo22 93.9(5) . . ?
Ge1 O8 Mo7 125.3(7) . . ?
Mo1 O8 Mo7 93.3(4) . . ?
Mo22 O8 Mo7 94.6(4) . . ?
Mo4 O9 Mo7 146.2(7) . . ?
Mo8 O10 Mo4 117.1(5) . . ?
Mo7 O12 Mo1 118.7(6) . . ?
Mo7 O13 Mo20 163.1(7) . . ?
Mo20 O14 Mo11 118.0(6) . . ?
Ge1 O16 Mo10 122.1(6) . . ?
Ge1 O16 Mo11 120.9(6) . . ?
Mo10 O16 Mo11 93.8(4) . . ?
Ge1 O16 Mo20 125.3(6) . . ?
Mo10 O16 Mo20 92.9(5) . . ?
Mo11 O16 Mo20 93.8(4) . . ?
Mo10 O18 Mo11 118.3(6) . . ?
Mo1 O19 Mo5 157.8(7) . . ?
Ge1 O20 Mo4 122.0(6) . . ?
Ge1 O20 Mo14 117.1(6) . . ?
Mo4 O20 Mo14 101.9(5) . . ?
Ge1 O20 Mo8 116.9(6) . . ?
Mo4 O20 Mo8 102.4(4) . . ?
Mo14 O20 Mo8 91.3(4) . . ?
Mo11 O21 Er1 154.8(8) . . ?
Mo22 O22 Er1 161.5(8) . . ?
Mo2 O24 Er1 153.6(7) . . ?
Mo12 O25 Mo16 118.4(7) . . ?
Mo16 O26 Mo6 147.4(7) . . ?
Mo6 O27 Mo9 156.6(7) . . ?
Mo9 O28 Mo15 114.0(6) . . ?
Mo19 O30 Mo15 145.5(7) . . ?
Ge2 O32 Mo2 119.7(6) . . ?
Ge2 O32 Mo3 122.5(6) . . ?
Mo2 O32 Mo3 95.4(4) . . ?
Ge2 O32 Mo17 123.3(5) . . ?
Mo2 O32 Mo17 96.3(4) . . ?
Mo3 O32 Mo17 92.6(4) . . ?
Mo19 O33 Mo3 146.9(7) . . ?
Ge2 O34 Mo21 119.5(6) . . ?
Ge2 O34 Mo19 119.2(6) . . ?
Mo21 O34 Mo19 102.7(5) . . ?
Ge2 O34 Mo6 121.1(6) . . ?
Mo21 O34 Mo6 95.3(4) . . ?
Mo19 O34 Mo6 93.6(4) . . ?
Mo6 O35 Mo19 119.2(6) . . ?
Mo21 O36 Mo18 147.2(8) . . ?
Mo21 O37 Mo6 120.3(6) . . ?
Ge2 O39 Mo9 126.1(6) . . ?
Ge2 O39 Mo15 127.2(7) . . ?
Mo9 O39 Mo15 96.9(5) . . ?
Mo19 O41 Mo21 120.3(7) . . ?
Mo3 O43 Mo2 118.1(6) . . ?
Mo17 O44 Mo2 120.5(6) . . ?
Mo17 O45 Mo18 157.8(8) . . ?
Mo2 O46 Mo12 138.9(7) . . ?
Mo18 O47 Mo12 119.1(6) . . ?
Ge2 O48 Mo16 119.2(6) . . ?
Ge2 O48 Mo12 121.1(6) . . ?
Mo16 O48 Mo12 93.5(4) . . ?
Ge2 O48 Mo18 128.1(6) . . ?
Mo16 O48 Mo18 92.7(4) . . ?
Mo12 O48 Mo18 93.7(4) . . ?
Mo16 O50 Mo9 152.7(7) . . ?
Mo21 O51 Mo17 148.9(8) . . ?
Mo15 O54 Mo3 160.7(7) . . ?
Mo13 O57 Er1 136.3(6) . . ?
Mo1 O58 Mo22 119.5(7) . . ?
Mo1 O59 Mo8 146.1(7) . . ?
Mo5 O60 Mo13 113.2(6) . . ?
Mo18 O61 Mo16 121.1(7) . . ?
Mo12 O64 Er1 162.7(8) . . ?
Mo3 O65 Mo17 117.7(7) . . ?
Mo14 O68 Mo4 117.5(6) . . ?
Mo14 O69 Mo10 147.5(7) . . ?
Mo7 O71 Mo22 118.9(6) . . ?
Mo4 O72 Mo20 145.8(7) . . ?
Mo14 O74 Mo13 149.0(7) . . ?
Mo8 O75 Mo14 119.0(6) . . ?
Mo8 O78 Mo5 151.1(7) . . ?
C4 O79 C2 108(2) . . ?
C8 O80 C6 107(2) . . ?
C10 O81 C12 111.3(16) . . ?
C16 O82 C14 102(3) . . ?
C19 O83 C18 109(3) . . ?
O16 Ge1 O8 106.9(6) . . ?
O16 Ge1 O4 110.0(5) . . ?
O8 Ge1 O4 111.4(6) . . ?
O16 Ge1 O20 108.9(6) . . ?
O8 Ge1 O20 109.3(6) . . ?
O4 Ge1 O20 110.2(5) . . ?
O39 Ge2 O48 113.1(6) . . ?
O39 Ge2 O32 111.1(5) . . ?
O48 Ge2 O32 105.6(6) . . ?
O39 Ge2 O34 108.1(6) . . ?
O48 Ge2 O34 109.9(5) . . ?
O32 Ge2 O34 109.0(6) . . ?
O77 Mo1 O19 103.8(6) . . ?
O77 Mo1 O59 101.2(6) . . ?
O19 Mo1 O59 88.0(5) . . ?
O77 Mo1 O58 99.0(6) . . ?
O19 Mo1 O58 90.9(5) . . ?
O59 Mo1 O58 159.4(6) . . ?
O77 Mo1 O12 97.2(6) . . ?
O19 Mo1 O12 159.0(6) . . ?
O59 Mo1 O12 86.5(6) . . ?
O58 Mo1 O12 87.2(6) . . ?
O77 Mo1 O8 168.5(6) . . ?
O19 Mo1 O8 85.3(5) . . ?
O59 Mo1 O8 86.0(5) . . ?
O58 Mo1 O8 73.5(5) . . ?
O12 Mo1 O8 74.0(5) . . ?
O31 Mo2 O24 104.3(6) . . ?
O31 Mo2 O46 104.6(7) . . ?
O24 Mo2 O46 98.3(6) . . ?
O31 Mo2 O43 91.8(6) . . ?
O24 Mo2 O43 90.7(6) . . ?
O46 Mo2 O43 158.6(5) . . ?
O31 Mo2 O44 93.9(6) . . ?
O24 Mo2 O44 159.2(5) . . ?
O46 Mo2 O44 86.6(6) . . ?
O43 Mo2 O44 78.6(5) . . ?
O31 Mo2 O32 157.8(7) . . ?
O24 Mo2 O32 90.8(5) . . ?
O46 Mo2 O32 88.9(5) . . ?
O43 Mo2 O32 71.5(4) . . ?
O44 Mo2 O32 69.1(4) . . ?
O53 Mo3 O43 101.8(6) . . ?
O53 Mo3 O65 100.7(7) . . ?
O43 Mo3 O65 92.4(6) . . ?
O53 Mo3 O54 101.3(6) . . ?
O43 Mo3 O54 93.3(5) . . ?
O65 Mo3 O54 155.6(6) . . ?
O53 Mo3 O33 97.5(6) . . ?
O43 Mo3 O33 160.6(5) . . ?
O65 Mo3 O33 84.9(5) . . ?
O54 Mo3 O33 81.9(5) . . ?
O53 Mo3 O32 174.4(5) . . ?
O43 Mo3 O32 74.5(5) . . ?
O65 Mo3 O32 75.4(5) . . ?
O54 Mo3 O32 83.3(5) . . ?
O33 Mo3 O32 86.3(4) . . ?
O67 Mo4 O72 107.2(6) . . ?
O67 Mo4 O9 105.5(6) . . ?
O72 Mo4 O9 96.2(6) . . ?
O67 Mo4 O68 94.5(6) . . ?
O72 Mo4 O68 85.9(5) . . ?
O9 Mo4 O68 158.2(6) . . ?
O67 Mo4 O10 93.3(6) . . ?
O72 Mo4 O10 157.6(5) . . ?
O9 Mo4 O10 86.6(6) . . ?
O68 Mo4 O10 83.6(5) . . ?
O67 Mo4 O20 158.7(5) . . ?
O72 Mo4 O20 87.2(5) . . ?
O9 Mo4 O20 87.9(5) . . ?
O68 Mo4 O20 70.6(5) . . ?
O10 Mo4 O20 70.6(4) . . ?
O66 Mo5 O3 104.0(6) . . ?
O66 Mo5 O60 99.0(6) . . ?
O3 Mo5 O60 98.6(6) . . ?
O66 Mo5 O19 98.0(6) . . ?
O3 Mo5 O19 95.8(6) . . ?
O60 Mo5 O19 154.3(5) . . ?
O66 Mo5 O78 90.2(6) . . ?
O3 Mo5 O78 165.3(5) . . ?
O60 Mo5 O78 82.4(5) . . ?
O19 Mo5 O78 78.4(5) . . ?
O66 Mo5 O4 168.0(6) . . ?
O3 Mo5 O4 86.5(5) . . ?
O60 Mo5 O4 73.5(5) . . ?
O19 Mo5 O4 86.3(5) . . ?
O78 Mo5 O4 79.6(5) . . ?
O66 Mo5 Mo13 132.3(5) . . ?
O3 Mo5 Mo13 85.1(4) . . ?
O60 Mo5 Mo13 33.6(4) . . ?
O19 Mo5 Mo13 128.1(4) . . ?
O78 Mo5 Mo13 87.9(4) . . ?
O4 Mo5 Mo13 41.8(3) . . ?
O38 Mo6 O27 101.6(6) . . ?
O38 Mo6 O35 105.2(7) . . ?
O27 Mo6 O35 95.0(6) . . ?
O38 Mo6 O37 100.7(6) . . ?
O27 Mo6 O37 154.1(6) . . ?
O35 Mo6 O37 91.8(6) . . ?
O38 Mo6 O26 96.7(6) . . ?
O27 Mo6 O26 84.6(6) . . ?
O35 Mo6 O26 157.7(5) . . ?
O37 Mo6 O26 79.8(5) . . ?
O38 Mo6 O34 172.1(6) . . ?
O27 Mo6 O34 86.2(5) . . ?
O35 Mo6 O34 75.1(5) . . ?
O37 Mo6 O34 71.5(5) . . ?
O26 Mo6 O34 82.6(5) . . ?
O11 Mo7 O71 104.0(6) . . ?
O11 Mo7 O13 103.2(6) . . ?
O71 Mo7 O13 95.9(6) . . ?
O11 Mo7 O12 98.7(6) . . ?
O71 Mo7 O12 93.5(6) . . ?
O13 Mo7 O12 153.2(6) . . ?
O11 Mo7 O9 96.4(6) . . ?
O71 Mo7 O9 159.5(5) . . ?
O13 Mo7 O9 80.3(5) . . ?
O12 Mo7 O9 82.1(6) . . ?
O11 Mo7 O8 172.3(6) . . ?
O71 Mo7 O8 76.6(5) . . ?
O13 Mo7 O8 84.3(5) . . ?
O12 Mo7 O8 73.6(5) . . ?
O9 Mo7 O8 82.9(5) . . ?
O76 Mo8 O78 102.3(7) . . ?
O76 Mo8 O75 100.6(6) . . ?
O78 Mo8 O75 95.9(6) . . ?
O76 Mo8 O59 101.6(7) . . ?
O78 Mo8 O59 90.6(6) . . ?
O75 Mo8 O59 154.9(6) . . ?
O76 Mo8 O10 97.6(6) . . ?
O78 Mo8 O10 159.6(5) . . ?
O75 Mo8 O10 84.5(6) . . ?
O59 Mo8 O10 81.2(5) . . ?
O76 Mo8 O20 166.4(6) . . ?
O78 Mo8 O20 90.7(5) . . ?
O75 Mo8 O20 73.8(5) . . ?
O59 Mo8 O20 81.9(5) . . ?
O10 Mo8 O20 69.8(4) . . ?
O56 Mo9 O1 101.3(6) . . ?
O56 Mo9 O28 97.2(6) . . ?
O1 Mo9 O28 97.4(5) . . ?
O56 Mo9 O50 99.8(6) . . ?
O1 Mo9 O50 95.1(5) . . ?
O28 Mo9 O50 156.5(5) . . ?
O56 Mo9 O27 92.0(6) . . ?
O1 Mo9 O27 166.4(6) . . ?
O28 Mo9 O27 83.7(5) . . ?
O50 Mo9 O27 79.6(5) . . ?
O56 Mo9 O39 168.3(6) . . ?
O1 Mo9 O39 86.9(5) . . ?
O28 Mo9 O39 73.3(5) . . ?
O50 Mo9 O39 87.6(5) . . ?
O27 Mo9 O39 80.4(5) . . ?
O17 Mo10 O18 100.7(6) . . ?
O17 Mo10 O5 103.6(6) . . ?
O18 Mo10 O5 91.1(6) . . ?
O17 Mo10 O6 97.3(7) . . ?
O18 Mo10 O6 89.7(6) . . ?
O5 Mo10 O6 158.6(6) . . ?
O17 Mo10 O69 98.9(6) . . ?
O18 Mo10 O69 160.4(5) . . ?
O5 Mo10 O69 85.2(5) . . ?
O6 Mo10 O69 86.9(5) . . ?
O17 Mo10 O16 171.4(6) . . ?
O18 Mo10 O16 75.3(5) . . ?
O5 Mo10 O16 84.2(5) . . ?
O6 Mo10 O16 75.3(5) . . ?
O69 Mo10 O16 85.2(5) . . ?
O40 Mo11 O21 106.3(7) . . ?
O40 Mo11 O7 101.3(7) . . ?
O21 Mo11 O7 95.8(6) . . ?
O40 Mo11 O18 97.6(7) . . ?
O21 Mo11 O18 93.8(6) . . ?
O7 Mo11 O18 155.4(5) . . ?
O40 Mo11 O14 90.6(6) . . ?
O21 Mo11 O14 163.0(5) . . ?
O7 Mo11 O14 82.7(5) . . ?
O18 Mo11 O14 81.6(5) . . ?
O40 Mo11 O16 159.4(6) . . ?
O21 Mo11 O16 92.3(5) . . ?
O7 Mo11 O16 85.1(5) . . ?
O18 Mo11 O16 71.9(5) . . ?
O14 Mo11 O16 70.7(4) . . ?
O55 Mo12 O64 105.7(7) . . ?
O55 Mo12 O25 100.9(6) . . ?
O64 Mo12 O25 99.6(6) . . ?
O55 Mo12 O46 98.3(6) . . ?
O64 Mo12 O46 89.6(6) . . ?
O25 Mo12 O46 155.6(5) . . ?
O55 Mo12 O47 92.3(7) . . ?
O64 Mo12 O47 160.2(6) . . ?
O25 Mo12 O47 85.0(5) . . ?
O46 Mo12 O47 79.2(5) . . ?
O55 Mo12 O48 162.7(6) . . ?
O64 Mo12 O48 91.6(5) . . ?
O25 Mo12 O48 74.6(5) . . ?
O46 Mo12 O48 82.6(5) . . ?
O47 Mo12 O48 70.8(4) . . ?
O73 Mo13 O57 103.2(7) . . ?
O73 Mo13 O5 100.3(7) . . ?
O57 Mo13 O5 98.8(6) . . ?
O73 Mo13 O60 96.6(7) . . ?
O57 Mo13 O60 95.5(6) . . ?
O5 Mo13 O60 154.7(5) . . ?
O73 Mo13 O4 166.6(6) . . ?
O57 Mo13 O4 87.4(5) . . ?
O5 Mo13 O4 85.9(5) . . ?
O60 Mo13 O4 73.9(5) . . ?
O73 Mo13 O74 89.5(6) . . ?
O57 Mo13 O74 167.3(5) . . ?
O5 Mo13 O74 78.5(5) . . ?
O60 Mo13 O74 83.0(5) . . ?
O4 Mo13 O74 80.0(5) . . ?
O73 Mo13 Mo5 129.6(6) . . ?
O57 Mo13 Mo5 83.4(5) . . ?
O5 Mo13 Mo5 128.4(4) . . ?
O60 Mo13 Mo5 33.3(4) . . ?
O4 Mo13 Mo5 42.6(3) . . ?
O74 Mo13 Mo5 88.6(4) . . ?
O70 Mo14 O74 105.1(6) . . ?
O70 Mo14 O69 104.6(6) . . ?
O74 Mo14 O69 92.3(6) . . ?
O70 Mo14 O75 96.9(6) . . ?
O74 Mo14 O75 93.0(6) . . ?
O69 Mo14 O75 155.7(5) . . ?
O70 Mo14 O68 94.9(6) . . ?
O74 Mo14 O68 160.1(6) . . ?
O69 Mo14 O68 82.7(5) . . ?
O75 Mo14 O68 84.3(6) . . ?
O70 Mo14 O20 162.3(5) . . ?
O74 Mo14 O20 90.4(5) . . ?
O69 Mo14 O20 83.0(5) . . ?
O75 Mo14 O20 73.3(5) . . ?
O68 Mo14 O20 69.9(5) . . ?
O29 Mo15 O2 103.1(6) . . ?
O29 Mo15 O54 100.4(6) . . ?
O2 Mo15 O54 98.8(5) . . ?
O29 Mo15 O28 97.5(6) . . ?
O2 Mo15 O28 94.9(6) . . ?
O54 Mo15 O28 154.3(5) . . ?
O29 Mo15 O30 90.2(6) . . ?
O2 Mo15 O30 166.6(6) . . ?
O54 Mo15 O30 80.3(5) . . ?
O28 Mo15 O30 81.3(5) . . ?
O29 Mo15 O39 167.6(5) . . ?
O2 Mo15 O39 85.8(5) . . ?
O54 Mo15 O39 86.6(5) . . ?
O28 Mo15 O39 72.9(5) . . ?
O30 Mo15 O39 80.8(5) . . ?
O49 Mo16 O26 102.2(6) . . ?
O49 Mo16 O50 101.8(6) . . ?
O26 Mo16 O50 91.0(5) . . ?
O49 Mo16 O61 99.0(6) . . ?
O26 Mo16 O61 92.1(6) . . ?
O50 Mo16 O61 157.8(5) . . ?
O49 Mo16 O25 96.7(6) . . ?
O26 Mo16 O25 161.1(6) . . ?
O50 Mo16 O25 86.2(5) . . ?
O61 Mo16 O25 83.9(6) . . ?
O49 Mo16 O48 167.2(6) . . ?
O26 Mo16 O48 88.4(5) . . ?
O50 Mo16 O48 85.0(5) . . ?
O61 Mo16 O48 73.2(5) . . ?
O25 Mo16 O48 72.8(5) . . ?
O52 Mo17 O44 105.5(6) . . ?
O52 Mo17 O45 102.3(7) . . ?
O44 Mo17 O45 94.7(6) . . ?
O52 Mo17 O65 95.9(7) . . ?
O44 Mo17 O65 90.8(6) . . ?
O45 Mo17 O65 158.8(6) . . ?
O52 Mo17 O51 98.2(6) . . ?
O44 Mo17 O51 156.2(6) . . ?
O45 Mo17 O51 82.6(6) . . ?
O65 Mo17 O51 84.1(5) . . ?
O52 Mo17 O32 169.6(6) . . ?
O44 Mo17 O32 73.7(5) . . ?
O45 Mo17 O32 88.1(5) . . ?
O65 Mo17 O32 73.8(5) . . ?
O51 Mo17 O32 82.5(5) . . ?
O62 Mo18 O47 102.7(7) . . ?
O62 Mo18 O61 100.5(6) . . ?
O47 Mo18 O61 92.9(6) . . ?
O62 Mo18 O45 101.3(7) . . ?
O47 Mo18 O45 94.5(6) . . ?
O61 Mo18 O45 154.8(6) . . ?
O62 Mo18 O36 98.8(6) . . ?
O47 Mo18 O36 158.5(6) . . ?
O61 Mo18 O36 82.5(6) . . ?
O45 Mo18 O36 81.8(5) . . ?
O62 Mo18 O48 173.3(6) . . ?
O47 Mo18 O48 76.2(5) . . ?
O61 Mo18 O48 73.1(5) . . ?
O45 Mo18 O48 85.3(5) . . ?
O36 Mo18 O48 82.4(5) . . ?
O63 Mo19 O30 106.1(7) . . ?
O63 Mo19 O33 104.2(6) . . ?
O30 Mo19 O33 96.0(6) . . ?
O63 Mo19 O41 95.9(6) . . ?
O30 Mo19 O41 156.0(6) . . ?
O33 Mo19 O41 87.6(6) . . ?
O63 Mo19 O35 94.9(6) . . ?
O30 Mo19 O35 86.5(6) . . ?
O33 Mo19 O35 159.1(5) . . ?
O41 Mo19 O35 82.1(5) . . ?
O63 Mo19 O34 160.8(6) . . ?
O30 Mo19 O34 87.2(6) . . ?
O33 Mo19 O34 87.7(5) . . ?
O41 Mo19 O34 69.2(5) . . ?
O35 Mo19 O34 71.7(5) . . ?
O15 Mo20 O14 104.6(6) . . ?
O15 Mo20 O13 100.3(6) . . ?
O14 Mo20 O13 96.5(6) . . ?
O15 Mo20 O6 100.5(6) . . ?
O14 Mo20 O6 94.7(5) . . ?
O13 Mo20 O6 153.0(5) . . ?
O15 Mo20 O72 96.1(5) . . ?
O14 Mo20 O72 159.3(5) . . ?
O13 Mo20 O72 79.7(5) . . ?
O6 Mo20 O72 81.1(5) . . ?
O15 Mo20 O16 174.3(6) . . ?
O14 Mo20 O16 77.5(5) . . ?
O13 Mo20 O16 84.6(5) . . ?
O6 Mo20 O16 73.9(5) . . ?
O72 Mo20 O16 81.8(4) . . ?
O42 Mo21 O36 103.3(6) . . ?
O42 Mo21 O51 105.4(7) . . ?
O36 Mo21 O51 91.7(6) . . ?
O42 Mo21 O37 96.5(6) . . ?
O36 Mo21 O37 93.3(6) . . ?
O51 Mo21 O37 155.9(6) . . ?
O42 Mo21 O41 95.5(6) . . ?
O36 Mo21 O41 161.1(6) . . ?
O51 Mo21 O41 84.2(6) . . ?
O37 Mo21 O41 83.5(6) . . ?
O42 Mo21 O34 160.5(5) . . ?
O36 Mo21 O34 93.7(5) . . ?
O51 Mo21 O34 83.3(5) . . ?
O37 Mo21 O34 72.8(5) . . ?
O41 Mo21 O34 67.6(5) . . ?
O23 Mo22 O22 104.1(7) . . ?
O23 Mo22 O7 100.1(7) . . ?
O22 Mo22 O7 91.2(6) . . ?
O23 Mo22 O58 99.9(7) . . ?
O22 Mo22 O58 98.7(6) . . ?
O7 Mo22 O58 154.8(5) . . ?
O23 Mo22 O71 92.0(6) . . ?
O22 Mo22 O71 163.7(6) . . ?
O7 Mo22 O71 83.6(5) . . ?
O58 Mo22 O71 80.5(5) . . ?
O23 Mo22 O8 161.0(6) . . ?
O22 Mo22 O8 94.3(5) . . ?
O7 Mo22 O8 84.2(5) . . ?
O58 Mo22 O8 72.1(5) . . ?
O71 Mo22 O8 69.8(4) . . ?
O64 Er1 O2 119.0(5) . . ?
O64 Er1 O22 81.0(5) . . ?
O2 Er1 O22 133.7(5) . . ?
O64 Er1 O24 70.7(5) . . ?
O2 Er1 O24 76.4(5) . . ?
O22 Er1 O24 72.0(4) . . ?
O64 Er1 O1 75.4(5) . . ?
O2 Er1 O1 77.4(4) . . ?
O22 Er1 O1 148.1(5) . . ?
O24 Er1 O1 118.3(4) . . ?
O64 Er1 O3 149.5(5) . . ?
O2 Er1 O3 71.1(4) . . ?
O22 Er1 O3 73.4(5) . . ?
O24 Er1 O3 85.6(4) . . ?
O1 Er1 O3 134.3(4) . . ?
O64 Er1 O21 72.7(5) . . ?
O2 Er1 O21 152.8(5) . . ?
O22 Er1 O21 69.7(5) . . ?
O24 Er1 O21 130.1(4) . . ?
O1 Er1 O21 82.9(4) . . ?
O3 Er1 O21 112.2(4) . . ?
O64 Er1 O57 133.4(5) . . ?
O2 Er1 O57 83.2(4) . . ?
O22 Er1 O57 114.2(4) . . ?
O24 Er1 O57 154.8(5) . . ?
O1 Er1 O57 70.3(4) . . ?
O3 Er1 O57 73.8(4) . . ?
O21 Er1 O57 72.6(4) . . ?

_refine_diff_density_max         1.102
_refine_diff_density_min         -1.225
_refine_diff_density_rms         0.184

_shelxl_version_number           2014-3


_vrf_CHEMW03_1_sq                
;
CHEMW03_ALERT_2_A

RESPONSE: Use of Platon SQUEEZE to remove disordered solvent. The accessible
solvent void in the crystal structure indicates that some more water molecules
and morpholine should exist in the structure, but cannot be found from the
weak residual electron peaks. Based on the TG analyses and elemental analysis,
14 water molecules and 8 morpholine were included in the sum formula.
;
_vrf_PLAT201_1_sq                
;
PLAT201_ALERT_2_B Isotropic non-H Atoms in Main Residue(s) ...... 2

RESPONSE: The structure contains a high degree of disorder.
;
_vrf_PLAT342_1_sq                
;
PLAT342_ALERT_3_B Low Bond Precision on C-C Bonds .............. 0.044 Ang.

RESPONSE: The low bond distance precision is likely due to the low data to
parameter ratio. There is a large amount of disorder in the structure. This is
common in high nuclearity polyoxometalate cluster . (such as Angew. Chem. Int.
Ed, 2010, 49, 6984; Angew. Chem. Int. Ed, 2008, 47, 6881, J. Am. Chem. Soc,
2004, 126, 13880.)
;
_vrf_PLAT430_1_sq                
;
PLAT430_ALERT_2_B Short Inter D...A Contact O10...O35 ......2.84 Ang.

RESPONSE: The structure contains a high degree of disorder.
;

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2_sq
_database_code_depnum_ccdc_archive 'CCDC 991333'
_audit_update_record             
;
2017-10-04 deposited with the CCDC.
2017-10-09 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C32 H111 Gd Ge2 Mo22 N8 O99'
_chemical_formula_weight         4605.39

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           7
_space_group_name_H-M_alt        'P n'
_space_group_name_Hall           'P -2yac'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'x+1/2, -y, z+1/2'

_cell_length_a                   13.2175(3)
_cell_length_b                   12.7258(4)
_cell_length_c                   32.5224(10)
_cell_angle_alpha                90
_cell_angle_beta                 96.203(3)
_cell_angle_gamma                90
_cell_volume                     5438.3(3)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    10923
_cell_measurement_theta_min      3.0902
_cell_measurement_theta_max      29.2020

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.812
_exptl_crystal_F_000             4406
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.420
_exptl_crystal_size_mid          0.340
_exptl_crystal_size_min          0.300
_exptl_absorpt_coefficient_mu    3.710
_shelx_estimated_absorpt_T_min   0.305
_shelx_estimated_absorpt_T_max   0.402
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.64910
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   ?

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Enhance (Mo) X-ray Source'
_diffrn_measurement_device_type  'Xcalibur, Ruby, Gemini ultra'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            19948
_diffrn_reflns_av_unetI/netI     0.0415
_diffrn_reflns_av_R_equivalents  0.0268
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_theta_min         3.101
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measured_fraction_theta_full 0.969
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_Laue_measured_fraction_full 0.969
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_point_group_measured_fraction_full 0.969
_reflns_number_total             13447
_reflns_number_gt                12960
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.999
_reflns_Friedel_fraction_max     0.994
_reflns_Friedel_fraction_full    0.969

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_cell_refinement       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction        
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXTL

_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0749P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.387(12)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         13447
_refine_ls_number_parameters     1302
_refine_ls_number_restraints     102
_refine_ls_R_factor_all          0.0409
_refine_ls_R_factor_gt           0.0391
_refine_ls_wR_factor_ref         0.1023
_refine_ls_wR_factor_gt          0.1007
_refine_ls_goodness_of_fit_ref   1.024
_refine_ls_restrained_S_all      9.883
_refine_ls_shift/su_max          0.016
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.9599(7) 0.8656(7) 0.0595(3) 0.024(2) Uani 1 1 d . . . . .
O2 O 0.8166(8) 0.8880(7) -0.0060(3) 0.025(2) Uani 1 1 d . . . . .
O3 O 0.7772(8) 0.7334(7) -0.0636(3) 0.023(2) Uani 1 1 d . . . . .
O4 O 0.6613(7) 0.7425(7) 0.2832(3) 0.022(2) Uani 1 1 d . . . . .
O5 O 0.7242(7) 0.7161(8) 0.3611(3) 0.025(2) Uani 1 1 d D . . . .
O6 O 1.1546(7) 0.7901(7) -0.0611(3) 0.022(2) Uani 1 1 d . . . . .
O7 O 1.1158(6) 0.7518(7) 0.0252(3) 0.0155(19) Uani 1 1 d . . . . .
O8 O 1.0301(7) 0.5577(7) 0.0464(3) 0.0151(19) Uani 1 1 d . U . . .
O9 O 0.8277(7) 0.5154(7) 0.0147(3) 0.022(2) Uani 1 1 d . . . . .
O10 O 1.2140(7) 0.5991(7) -0.0836(3) 0.022(2) Uani 1 1 d D . . . .
O11 O 0.9011(7) 0.4687(8) 0.0964(3) 0.023(2) Uani 1 1 d . . . . .
O12 O 1.1095(7) 0.5202(7) 0.1252(3) 0.021(2) Uani 1 1 d . . . . .
O13 O 0.7977(7) 0.5571(7) 0.1587(3) 0.020(2) Uani 1 1 d . . . . .
O14 O 0.9993(7) 0.4712(7) 0.1917(3) 0.021(2) Uani 1 1 d . . . . .
O15 O 1.0738(7) 0.6919(7) 0.1969(3) 0.021(2) Uani 1 1 d . . . . .
O16 O 0.8262(7) 0.4214(7) 0.2254(3) 0.020(2) Uani 1 1 d . . . . .
O17 O 1.0826(7) 0.5275(8) 0.2709(3) 0.024(2) Uani 1 1 d . . . . .
O18 O 1.2128(7) 0.6952(7) 0.2645(3) 0.020(2) Uani 1 1 d . . . . .
O19 O 1.0334(6) 0.7433(7) 0.2790(3) 0.0153(19) Uani 1 1 d . . . . .
O20 O 0.8605(7) 0.6676(7) 0.3159(3) 0.018(2) Uani 1 1 d . . . . .
O21 O 0.8349(8) 0.9306(8) -0.0871(3) 0.032(3) Uani 1 1 d . . . . .
O22 O 0.9617(7) 0.7522(8) -0.0882(3) 0.021(2) Uani 1 1 d . . . . .
O23 O 1.2794(7) 0.8398(7) 0.0048(3) 0.021(2) Uani 1 1 d . . . . .
O24 O 1.2390(7) 0.6041(7) 0.0719(3) 0.019(2) Uani 1 1 d . . . . .
O25 O 1.1957(7) 0.4543(7) 0.0175(3) 0.021(2) Uani 1 1 d . . . . .
O26 O 1.0589(7) 0.3704(7) 0.0647(3) 0.019(2) Uani 1 1 d . . . . .
O27 O 1.0647(7) 0.7382(8) 0.1118(3) 0.025(2) Uani 1 1 d . . . . .
O28 O 1.1084(9) 0.9454(8) 0.1203(3) 0.035(3) Uani 1 1 d . . . . .
O29 O 0.9149(7) 0.7115(7) -0.0016(3) 0.019(2) Uani 1 1 d . . . . .
O30 O 0.6635(7) 0.5622(9) -0.0447(4) 0.033(3) Uani 1 1 d . . . . .
O31 O 0.5768(8) 0.5784(9) 0.3261(3) 0.035(3) Uani 1 1 d D . . . .
O32 O 0.7066(7) 0.5497(8) 0.2687(3) 0.025(2) Uani 1 1 d . . . . .
O33 O 0.7743(7) 0.5124(7) 0.3490(3) 0.023(2) Uani 1 1 d D . . . .
O34 O 1.0553(7) 0.5832(8) 0.3457(3) 0.021(2) Uani 1 1 d . . . . .
O35 O 1.2543(7) 0.5560(8) 0.3274(3) 0.030(2) Uani 1 1 d . . . . .
O36 O 1.1572(7) 0.8940(8) 0.2800(3) 0.025(2) Uani 1 1 d . . . . .
O37 O 1.0148(7) 0.8906(7) 0.2119(3) 0.024(2) Uani 1 1 d . . . . .
O38 O 0.7275(7) 0.8864(7) 0.1876(3) 0.024(2) Uani 1 1 d . . . . .
O39 O 0.8925(6) 0.6039(6) 0.2354(3) 0.0142(19) Uani 1 1 d . . . . .
O40 O 1.2747(7) 0.6326(7) -0.0052(3) 0.021(2) Uani 1 1 d . . . . .
O41 O 1.0703(7) 0.5986(7) -0.0366(3) 0.018(2) Uani 1 1 d . . . . .
O42 O 0.8653(7) 0.5444(7) -0.0610(3) 0.023(2) Uani 1 1 d . . . . .
O43 O 1.0099(7) 0.5558(7) -0.1112(3) 0.022(2) Uani 1 1 d D . . . .
O44 O 1.0071(7) 0.8952(7) -0.0322(3) 0.021(2) Uani 1 1 d . . . . .
O45 O 1.1894(8) 1.0027(7) -0.0396(3) 0.031(2) Uani 1 1 d . . . . .
O46 O 1.1317(8) 0.9549(7) 0.0358(3) 0.026(2) Uani 1 1 d . . . . .
O47 O 1.2420(8) 0.8144(8) 0.0837(3) 0.025(2) Uani 1 1 d . . . . .
O48 O 0.7320(7) 0.7045(8) 0.0147(3) 0.025(2) Uani 1 1 d . . . . .
O49 O 0.8801(9) 0.9745(9) 0.1474(4) 0.038(3) Uani 1 1 d . . . . .
O50 O 0.8676(7) 1.0139(7) 0.2306(3) 0.025(2) Uani 1 1 d . . . . .
O51 O 1.2191(8) 0.8421(8) 0.2034(3) 0.029(2) Uani 1 1 d . . . . .
O52 O 0.9748(7) 0.9566(7) 0.3023(3) 0.025(2) Uani 1 1 d . . . . .
O53 O 0.8393(7) 0.8187(7) 0.2496(3) 0.021(2) Uani 1 1 d . . . . .
O54 O 0.6936(7) 0.6851(7) 0.2071(3) 0.019(2) Uani 1 1 d . . . . .
O55 O 1.0096(7) 0.3258(8) 0.2517(3) 0.027(2) Uani 1 1 d . . . . .
O56 O 0.8110(7) 0.8929(7) 0.3313(3) 0.024(2) Uani 1 1 d . . . . .
O57 O 0.8433(8) 0.8407(8) 0.4146(3) 0.029(2) Uani 1 1 d . . . . .
O58 O 0.9095(8) 0.6426(8) 0.3918(3) 0.027(2) Uani 1 1 d D . . . .
O59 O 0.8866(7) 0.7657(7) 0.1650(3) 0.022(2) Uani 1 1 d . . . . .
O60 O 0.8662(8) 0.6910(8) 0.0840(3) 0.028(2) Uani 1 1 d . . . . .
O61 O 1.4096(7) 0.7197(8) 0.0569(3) 0.027(2) Uani 1 1 d . . . . .
O62 O 1.2572(7) 0.3975(8) 0.0989(3) 0.026(2) Uani 1 1 d . . . . .
O63 O 0.8623(8) 0.3108(7) 0.0419(3) 0.030(2) Uani 1 1 d . . . . .
O64 O 0.9721(7) 0.4068(7) -0.0144(3) 0.022(2) Uani 1 1 d . . . . .
O65 O 1.3287(7) 0.4398(8) -0.0398(3) 0.029(2) Uani 1 1 d D . . . .
O66 O 1.1248(7) 0.4201(7) -0.0640(3) 0.022(2) Uani 1 1 d . . . . .
O67 O 0.9313(8) 0.3586(8) -0.0969(3) 0.031(2) Uani 1 1 d . . . . .
O68 O 0.6361(8) 0.4750(8) 0.1914(3) 0.033(3) Uani 1 1 d . . . . .
O69 O 0.5461(8) 0.8362(9) 0.2191(4) 0.034(3) Uani 1 1 d . . . . .
O70 O 0.6982(7) 0.9477(8) 0.2632(3) 0.028(2) Uani 1 1 d . . . . .
O71 O 0.8193(9) 1.1040(8) 0.3033(3) 0.033(3) Uani 1 1 d . . . . .
O72 O 1.1477(8) 0.9555(9) 0.3605(4) 0.036(3) Uani 1 1 d . . . . .
O73 O 1.1725(7) 0.7506(8) 0.3413(3) 0.022(2) Uani 1 1 d . . . . .
O74 O 0.9895(7) 0.8121(7) 0.3588(3) 0.022(2) Uani 1 1 d . . . . .
O75 O 0.9189(7) 0.4580(7) 0.3026(3) 0.020(2) Uani 1 1 d . . . . .
O76 O 0.9523(8) 0.4313(8) 0.3868(3) 0.031(2) Uani 1 1 d . . . . .
O77 O 0.7520(8) 0.8663(8) 0.0720(4) 0.032(3) Uani 1 1 d . . . . .
O78 O 1.1090(8) 0.7272(9) -0.1421(3) 0.030(2) Uani 1 1 d . U . . .
O79 O 0.3773(10) 0.7537(10) 0.9365(4) 0.048(3) Uani 1 1 d . . . . .
O80 O 0.3652(10) 0.6619(11) 0.2091(4) 0.055(4) Uani 1 1 d . . . . .
O81 O 0.1841(12) 0.1813(10) 0.3042(4) 0.056(4) Uani 1 1 d . . . . .
O82 O 0.0700(14) 0.1186(15) 0.2171(6) 0.081(5) Uani 1 1 d . . . . .
O83 O 0.0752(15) 0.7537(17) 0.4729(6) 0.094(6) Uani 1 1 d . . . . .
O84 O 0.5378(12) 0.8253(15) 0.3677(6) 0.089(6) Uani 1 1 d D . . . .
O85 O 0.449(3) 0.415(3) 0.0516(12) 0.183(13) Uani 1 1 d . U . . .
N1 N 0.1869(13) 0.2187(12) 0.1620(5) 0.052(4) Uani 1 1 d . . . . .
H1A H 0.2235 0.2707 0.1529 0.062 Uiso 1 1 calc R U . . .
H1B H 0.1882 0.1643 0.1449 0.062 Uiso 1 1 calc R U . . .
N2 N 0.5347(10) 0.9018(11) 0.9294(5) 0.037(3) Uani 1 1 d . . . . .
H2A H 0.5699 0.8663 0.9121 0.044 Uiso 1 1 calc R U . . .
H2B H 0.5658 0.9630 0.9349 0.044 Uiso 1 1 calc R U . . .
N3 N 0.3660(12) 0.4423(10) 0.2209(5) 0.040(4) Uani 1 1 d . . . . .
H3A H 0.3459 0.3846 0.2332 0.048 Uiso 1 1 calc R U . . .
H3B H 0.4086 0.4229 0.2029 0.048 Uiso 1 1 calc R U . . .
N4 N 0.2720(13) 0.3451(12) 0.3552(4) 0.049(4) Uani 1 1 d . . . . .
H4A H 0.2946 0.3138 0.3789 0.058 Uiso 1 1 calc R U . . .
H4B H 0.2853 0.4135 0.3578 0.058 Uiso 1 1 calc R U . . .
N5 N 0.251(2) 0.805(2) 0.4338(8) 0.114(10) Uani 1 1 d . . . . .
H5A H 0.2327 0.8209 0.4073 0.137 Uiso 1 1 calc R U . . .
H5B H 0.3185 0.8093 0.4382 0.137 Uiso 1 1 calc R U . . .
N6 N 0.4514(14) 0.9908(14) 0.3179(8) 0.077(7) Uani 1 1 d . . . . .
N7 N 0.647(3) 0.479(3) 0.0846(13) 0.181(16) Uani 1 1 d . U . . .
H7A H 0.6644 0.4481 0.1089 0.217 Uiso 1 1 calc R U . . .
H7B H 0.6984 0.5204 0.0794 0.217 Uiso 1 1 calc R U . . .
C1 C 0.3774(14) 0.8176(15) 0.8986(6) 0.045(5) Uani 1 1 d . . . . .
H1C H 0.3081 0.8335 0.8873 0.054 Uiso 1 1 calc R U . . .
H1D H 0.4103 0.7795 0.8779 0.054 Uiso 1 1 calc R U . . .
C2 C 0.4359(18) 0.9199(15) 0.9105(8) 0.061(6) Uani 1 1 d . . . . .
H2C H 0.4396 0.9618 0.8858 0.074 Uiso 1 1 calc R U . . .
H2D H 0.3985 0.9601 0.9292 0.074 Uiso 1 1 calc R U . . .
C3 C 0.4843(11) 0.7400(13) 0.9589(5) 0.033(4) Uani 1 1 d . . . . .
H3C H 0.4806 0.7048 0.9851 0.039 Uiso 1 1 calc R U . . .
H3D H 0.5249 0.6970 0.9423 0.039 Uiso 1 1 calc R U . . .
C4 C 0.5323(13) 0.8448(15) 0.9660(7) 0.048(5) Uani 1 1 d . . . . .
H4C H 0.4948 0.8845 0.9848 0.058 Uiso 1 1 calc R U . . .
H4D H 0.6013 0.8357 0.9790 0.058 Uiso 1 1 calc R U . . .
C5 C 0.2793(14) 0.4922(16) 0.1991(6) 0.048(5) Uani 1 1 d . . . . .
H5C H 0.2298 0.5071 0.2182 0.057 Uiso 1 1 calc R U . . .
H5D H 0.2481 0.4444 0.1782 0.057 Uiso 1 1 calc R U . . .
C6 C 0.3058(13) 0.5896(15) 0.1793(6) 0.043(4) Uani 1 1 d . . . . .
H6C H 0.2440 0.6246 0.1678 0.052 Uiso 1 1 calc R U . . .
H6D H 0.3456 0.5735 0.1568 0.052 Uiso 1 1 calc R U . . .
C7 C 0.4180(13) 0.5082(15) 0.2511(6) 0.044(5) Uani 1 1 d . . . . .
H7C H 0.4755 0.4704 0.2650 0.052 Uiso 1 1 calc R U . . .
H7D H 0.3728 0.5263 0.2716 0.052 Uiso 1 1 calc R U . . .
C8 C 0.4557(12) 0.6083(13) 0.2324(6) 0.038(4) Uani 1 1 d . . . . .
H8A H 0.4867 0.6540 0.2541 0.045 Uiso 1 1 calc R U . . .
H8B H 0.5061 0.5918 0.2139 0.045 Uiso 1 1 calc R U . . .
C9 C 0.1598(15) 0.3288(14) 0.3465(6) 0.047(5) Uani 1 1 d . . . . .
H9A H 0.1265 0.3516 0.3701 0.056 Uiso 1 1 calc R U . . .
H9B H 0.1337 0.3710 0.3228 0.056 Uiso 1 1 calc R U . . .
C10 C 0.3262(14) 0.2997(15) 0.3202(6) 0.046(5) Uani 1 1 d . U . . .
H10A H 0.3088 0.3393 0.2950 0.055 Uiso 1 1 calc R U . . .
H10B H 0.3994 0.3026 0.3273 0.055 Uiso 1 1 calc R U . . .
C11 C 0.1365(19) 0.2180(17) 0.3380(7) 0.064(6) Uani 1 1 d . . . . .
H11A H 0.1591 0.1765 0.3623 0.077 Uiso 1 1 calc R U . . .
H11B H 0.0634 0.2093 0.3322 0.077 Uiso 1 1 calc R U . . .
C13 C 0.172(3) 0.0907(17) 0.2152(9) 0.083(9) Uani 1 1 d . . . . .
H13A H 0.1773 0.0347 0.1953 0.100 Uiso 1 1 calc R U . . .
H13B H 0.2030 0.0672 0.2420 0.100 Uiso 1 1 calc R U . . .
C14 C 0.225(2) 0.190(2) 0.2018(9) 0.086(8) Uani 1 1 d . U . . .
H14A H 0.2153 0.2468 0.2208 0.103 Uiso 1 1 calc R U . . .
H14B H 0.2980 0.1771 0.2027 0.103 Uiso 1 1 calc R U . . .
C15 C 0.090(2) 0.2502(19) 0.1644(8) 0.076(8) Uani 1 1 d . . . . .
H15A H 0.0610 0.2766 0.1377 0.091 Uiso 1 1 calc R U . . .
H15B H 0.0891 0.3061 0.1846 0.091 Uiso 1 1 calc R U . . .
C16 C 0.029(2) 0.155(2) 0.1772(10) 0.090(9) Uani 1 1 d . . . . .
H16A H -0.0416 0.1757 0.1780 0.108 Uiso 1 1 calc R U . . .
H16B H 0.0311 0.0995 0.1571 0.108 Uiso 1 1 calc R U . . .
C17 C 0.1169(19) 0.698(2) 0.4382(9) 0.075(7) Uani 1 1 d . U . . .
H17A H 0.0927 0.6263 0.4373 0.090 Uiso 1 1 calc R U . . .
H17B H 0.0913 0.7319 0.4124 0.090 Uiso 1 1 calc R U . . .
C18 C 0.2197(16) 0.698(2) 0.4415(7) 0.064(6) Uani 1 1 d . . . . .
H18A H 0.2438 0.6503 0.4214 0.077 Uiso 1 1 calc R U . . .
H18B H 0.2473 0.6756 0.4690 0.077 Uiso 1 1 calc R U . . .
C19 C 0.088(2) 0.859(2) 0.4600(9) 0.084(8) Uani 1 1 d . U . . .
H19A H 0.0577 0.9066 0.4786 0.101 Uiso 1 1 calc R U . . .
H19B H 0.0534 0.8690 0.4324 0.101 Uiso 1 1 calc R U . . .
C20 C 0.206(2) 0.884(2) 0.4603(9) 0.080(7) Uani 1 1 d . U . . .
H20A H 0.2151 0.9539 0.4499 0.096 Uiso 1 1 calc R U . . .
H20B H 0.2391 0.8796 0.4884 0.096 Uiso 1 1 calc R U . . .
C21 C 0.399(2) 0.899(2) 0.3275(10) 0.097(9) Uani 1 1 d . U . . .
H21A H 0.3663 0.9123 0.3522 0.116 Uiso 1 1 calc R U . . .
H21B H 0.3460 0.8857 0.3051 0.116 Uiso 1 1 calc R U . . .
C22 C 0.457(2) 0.8091(16) 0.3338(7) 0.065(7) Uani 1 1 d . . . . .
H22A H 0.4868 0.7913 0.3087 0.078 Uiso 1 1 calc R U . . .
H22B H 0.4140 0.7511 0.3405 0.078 Uiso 1 1 calc R U . . .
C23 C 0.528(3) 1.006(3) 0.3574(11) 0.114(11) Uani 1 1 d . U . . .
H23A H 0.5639 1.0723 0.3554 0.137 Uiso 1 1 calc R U . . .
H23B H 0.4908 1.0100 0.3815 0.137 Uiso 1 1 calc R U . . .
C24 C 0.5966(16) 0.9254(17) 0.3620(8) 0.061(6) Uani 1 1 d . U . . .
H24A H 0.6457 0.9376 0.3859 0.074 Uiso 1 1 calc R U . . .
H24B H 0.6329 0.9199 0.3377 0.074 Uiso 1 1 calc R U . . .
C25 C 0.477(3) 0.488(3) 0.0898(12) 0.114(11) Uani 1 1 d . U . . .
H25A H 0.4253 0.5413 0.0909 0.136 Uiso 1 1 calc R U . . .
H25B H 0.4798 0.4464 0.1150 0.136 Uiso 1 1 calc R U . . .
C26 C 0.5698(18) 0.534(2) 0.0872(9) 0.076(7) Uani 1 1 d . U . . .
H26A H 0.5625 0.5803 0.0632 0.092 Uiso 1 1 calc R U . . .
H26B H 0.5839 0.5791 0.1113 0.092 Uiso 1 1 calc R U . . .
C27 C 0.532(2) 0.354(3) 0.0476(11) 0.100(10) Uani 1 1 d . U . . .
H27A H 0.5180 0.3183 0.0211 0.120 Uiso 1 1 calc R U . . .
H27B H 0.5313 0.2994 0.0685 0.120 Uiso 1 1 calc R U . . .
C28 C 0.632(3) 0.390(4) 0.0496(15) 0.157(17) Uani 1 1 d . U . . .
H28A H 0.6457 0.4185 0.0230 0.188 Uiso 1 1 calc R U . . .
H28B H 0.6794 0.3323 0.0564 0.188 Uiso 1 1 calc R U . . .
Ge1 Ge 0.90530(10) 0.70674(10) 0.26912(4) 0.0133(3) Uani 1 1 d . . . . .
Ge2 Ge 1.03297(10) 0.65361(10) 0.00873(4) 0.0125(3) Uani 1 1 d . . . . .
Mo1 Mo 1.08932(9) 0.87553(10) 0.32470(4) 0.0228(3) Uani 1 1 d . . . . .
Mo2 Mo 1.08387(9) 0.69714(9) -0.09338(4) 0.0182(3) Uani 1 1 d . . . . .
Mo3 Mo 1.11917(8) 0.79763(9) 0.22689(4) 0.0180(3) Uani 1 1 d . . . . .
Mo4 Mo 0.69627(9) 0.60881(9) 0.31783(4) 0.0189(3) Uani 1 1 d . . . . .
Mo5 Mo 0.87347(9) 0.84332(9) -0.05006(4) 0.0208(3) Uani 1 1 d . . . . .
Mo6 Mo 1.14894(9) 0.90115(9) -0.01322(4) 0.0199(3) Uani 1 1 d . . . . .
Mo7 Mo 0.74479(9) 0.54197(10) 0.20583(4) 0.0207(3) Uani 1 1 d . . . . .
Mo8 Mo 1.28355(9) 0.71738(10) 0.04258(4) 0.0213(3) Uani 1 1 d . . . . .
Mo9 Mo 0.83651(9) 0.79258(10) 0.04937(4) 0.0224(3) Uani 1 1 d . . . . .
Mo10 Mo 1.10049(9) 0.84735(9) 0.08541(4) 0.0213(3) Uani 1 1 d . . . . .
Mo11 Mo 1.22037(9) 0.50142(10) -0.03129(4) 0.0202(3) Uani 1 1 d . . . . .
Mo12 Mo 1.15966(9) 0.47758(9) 0.08067(4) 0.0180(3) Uani 1 1 d . . . . .
Mo13 Mo 0.93081(9) 0.52583(9) 0.35061(4) 0.0192(3) Uani 1 1 d . . . . .
Mo14 Mo 0.83632(10) 0.98368(9) 0.28225(4) 0.0237(3) Uani 1 1 d . . . . .
Mo15 Mo 0.97591(9) 0.45645(9) -0.06468(4) 0.0205(3) Uani 1 1 d . . . . .
Mo16 Mo 1.15705(9) 0.62936(10) 0.30677(4) 0.0213(3) Uani 1 1 d . . . . .
Mo17 Mo 0.77452(9) 0.61448(10) -0.02465(4) 0.0223(3) Uani 1 1 d . . . . .
Mo18 Mo 0.92528(9) 0.42599(9) 0.04759(4) 0.0184(3) Uani 1 1 d . . . . .
Mo19 Mo 0.85335(9) 0.78866(10) 0.36753(4) 0.0210(3) Uani 1 1 d . . . . .
Mo20 Mo 0.66858(9) 0.81325(10) 0.23519(4) 0.0219(3) Uani 1 1 d . . . . .
Mo21 Mo 0.97057(9) 0.45142(9) 0.24188(4) 0.0202(3) Uani 1 1 d . . . . .
Mo22 Mo 0.86785(9) 0.88987(9) 0.18631(4) 0.0191(3) Uani 1 1 d . . . . .
Gd1 Gd 0.96175(5) 0.61150(5) 0.14345(2) 0.01832(16) Uani 1 1 d . . . . .
C12 C 0.293(2) 0.192(2) 0.3148(9) 0.076(7) Uiso 1 1 d . . . . .
H12A H 0.3129 0.1540 0.3402 0.091 Uiso 1 1 calc R U . . .
H12B H 0.3278 0.1607 0.2931 0.091 Uiso 1 1 calc R U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 Mo9 1.876(10) . ?
O1 Mo10 1.969(10) . ?
O2 Mo5 1.780(10) . ?
O2 Mo9 2.166(10) . ?
O3 Mo5 1.910(10) . ?
O3 Mo17 1.975(10) . ?
O4 Mo20 1.814(10) . ?
O4 Mo4 2.065(10) . ?
O5 Mo19 1.932(10) . ?
O5 Mo4 1.967(10) . ?
O6 Mo2 1.779(9) . ?
O6 Mo6 2.110(10) . ?
O7 Ge2 1.709(9) . ?
O7 Mo8 2.271(8) . ?
O7 Mo10 2.331(9) . ?
O7 Mo6 2.342(9) . ?
O8 Ge2 1.732(8) . ?
O8 Mo18 2.178(9) . ?
O8 Mo12 2.192(8) . ?
O9 Mo17 1.878(10) . ?
O9 Mo18 1.950(9) . ?
O10 Mo11 2.100(10) . ?
O10 Mo2 2.121(9) . ?
O11 Mo18 1.740(9) . ?
O11 Gd1 2.454(10) . ?
O12 Mo12 1.742(10) . ?
O12 Gd1 2.402(10) . ?
O13 Mo7 1.761(9) . ?
O13 Gd1 2.380(9) . ?
O14 Mo21 1.733(10) . ?
O14 Gd1 2.394(9) . ?
O15 Mo3 1.731(9) . ?
O15 Gd1 2.389(10) . ?
O16 Mo7 1.942(10) . ?
O16 Mo21 1.963(9) . ?
O17 Mo21 1.928(10) . ?
O17 Mo16 1.940(10) . ?
O18 Mo16 1.830(9) . ?
O18 Mo3 2.098(9) . ?
O19 Ge1 1.752(8) . ?
O19 Mo3 2.247(9) . ?
O19 Mo16 2.296(9) . ?
O19 Mo1 2.313(9) . ?
O20 Ge1 1.764(9) . ?
O20 Mo13 2.272(9) . ?
O20 Mo19 2.287(9) . ?
O20 Mo4 2.304(9) . ?
O21 Mo5 1.678(10) . ?
O22 Mo2 1.784(9) . ?
O22 Mo5 2.135(10) . ?
O23 Mo6 1.926(10) . ?
O23 Mo8 1.981(9) . ?
O24 Mo8 1.859(9) . ?
O24 Mo12 1.959(9) . ?
O25 Mo11 1.759(9) . ?
O25 Mo12 2.179(9) . ?
O26 Mo18 1.927(9) . ?
O26 Mo12 1.938(9) . ?
O27 Mo10 1.725(10) . ?
O27 Gd1 2.411(9) . ?
O28 Mo10 1.683(10) . ?
O29 Ge2 1.726(9) . ?
O29 Mo17 2.287(9) . ?
O29 Mo9 2.293(9) . ?
O29 Mo5 2.326(9) . ?
O30 Mo17 1.678(10) . ?
O31 Mo4 1.675(10) . ?
O32 Mo4 1.785(10) . ?
O32 Mo7 2.160(10) . ?
O33 Mo4 1.837(10) . ?
O33 Mo13 2.070(10) . ?
O34 Mo13 1.823(9) . ?
O34 Mo16 2.031(9) . ?
O35 Mo16 1.670(10) . ?
O36 Mo1 1.804(10) . ?
O36 Mo3 2.135(11) . ?
O37 Mo3 1.843(10) . ?
O37 Mo22 2.028(10) . ?
O38 Mo22 1.861(10) . ?
O38 Mo20 2.031(10) . ?
O39 Ge1 1.705(8) . ?
O39 Mo21 2.197(8) . ?
O39 Mo7 2.225(8) . ?
O40 Mo8 1.884(10) . ?
O40 Mo11 1.973(9) . ?
O41 Ge2 1.751(9) . ?
O41 Mo2 2.255(10) . ?
O41 Mo15 2.327(9) . ?
O41 Mo11 2.328(9) . ?
O42 Mo15 1.855(9) . ?
O42 Mo17 1.985(10) . ?
O43 Mo15 2.058(10) . ?
O43 Mo2 2.098(9) . ?
O44 Mo6 1.911(10) . ?
O44 Mo5 1.916(9) . ?
O45 Mo6 1.671(10) . ?
O46 Mo6 1.771(10) . ?
O46 Mo10 2.190(10) . ?
O47 Mo10 1.924(10) . ?
O47 Mo8 1.943(9) . ?
O48 Mo17 1.851(10) . ?
O48 Mo9 2.024(10) . ?
O49 Mo22 1.682(11) . ?
O50 Mo14 1.814(10) . ?
O50 Mo22 2.137(10) . ?
O51 Mo3 1.694(10) . ?
O52 Mo14 1.907(10) . ?
O52 Mo1 1.910(10) . ?
O53 Ge1 1.753(9) . ?
O53 Mo20 2.256(9) . ?
O53 Mo22 2.317(10) . ?
O53 Mo14 2.354(9) . ?
O54 Mo20 1.915(9) . ?
O54 Mo7 1.945(9) . ?
O55 Mo21 1.699(10) . ?
O56 Mo19 1.822(10) . ?
O56 Mo14 2.027(10) . ?
O57 Mo19 1.686(10) . ?
O58 Mo13 2.041(10) . ?
O58 Mo19 2.121(10) . ?
O59 Mo22 1.753(9) . ?
O59 Gd1 2.342(9) . ?
O60 Mo9 1.731(10) . ?
O60 Gd1 2.415(10) . ?
O61 Mo8 1.681(9) . ?
O62 Mo12 1.699(9) . ?
O63 Mo18 1.686(10) . ?
O64 Mo15 1.758(10) . ?
O64 Mo18 2.187(10) . ?
O65 Mo11 1.681(9) . ?
O66 Mo11 1.873(10) . ?
O66 Mo15 2.019(9) . ?
O67 Mo15 1.693(10) . ?
O68 Mo7 1.692(10) . ?
O69 Mo20 1.671(10) . ?
O70 Mo14 1.918(10) . ?
O70 Mo20 1.958(10) . ?
O71 Mo14 1.703(10) . ?
O72 Mo1 1.671(11) . ?
O73 Mo16 1.906(10) . ?
O73 Mo1 1.975(10) . ?
O74 Mo19 1.877(9) . ?
O74 Mo1 1.983(9) . ?
O75 Mo13 1.775(10) . ?
O75 Mo21 2.161(9) . ?
O76 Mo13 1.685(10) . ?
O77 Mo9 1.688(10) . ?
O78 Mo2 1.697(10) . ?
O79 C1 1.48(2) . ?
O79 C3 1.529(18) . ?
O80 C6 1.50(2) . ?
O80 C8 1.51(2) . ?
O81 C11 1.40(3) . ?
O81 C12 1.45(3) . ?
O82 C13 1.40(3) . ?
O82 C16 1.43(3) . ?
O83 C19 1.42(3) . ?
O83 C17 1.48(3) . ?
O84 C22 1.46(3) . ?
O84 C24 1.51(3) . ?
O85 C27 1.37(4) . ?
O85 C25 1.56(4) . ?
N1 C15 1.35(3) . ?
N1 C14 1.39(3) . ?
N2 C4 1.40(2) . ?
N2 C2 1.40(2) . ?
N3 C7 1.41(2) . ?
N3 C5 1.43(2) . ?
N4 C9 1.49(2) . ?
N4 C10 1.52(2) . ?
N5 C18 1.46(3) . ?
N5 C20 1.49(4) . ?
N6 C21 1.41(3) . ?
N6 C23 1.56(4) . ?
N7 C26 1.25(4) . ?
N7 C28 1.60(5) . ?
C1 C2 1.54(3) . ?
C3 C4 1.48(2) . ?
C5 C6 1.46(3) . ?
C7 C8 1.52(3) . ?
C9 C11 1.46(3) . ?
C10 C12 1.44(3) . ?
C13 C14 1.53(3) . ?
C15 C16 1.54(3) . ?
C17 C18 1.35(3) . ?
C19 C20 1.59(3) . ?
C21 C22 1.38(3) . ?
C23 C24 1.37(4) . ?
C25 C26 1.37(4) . ?
C27 C28 1.40(5) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo9 O1 Mo10 141.2(5) . . ?
Mo5 O2 Mo9 117.8(5) . . ?
Mo5 O3 Mo17 118.1(5) . . ?
Mo20 O4 Mo4 148.1(5) . . ?
Mo19 O5 Mo4 120.3(5) . . ?
Mo2 O6 Mo6 145.4(5) . . ?
Ge2 O7 Mo8 120.8(4) . . ?
Ge2 O7 Mo10 122.3(5) . . ?
Mo8 O7 Mo10 93.6(3) . . ?
Ge2 O7 Mo6 125.2(5) . . ?
Mo8 O7 Mo6 93.2(3) . . ?
Mo10 O7 Mo6 93.6(3) . . ?
Ge2 O8 Mo18 128.1(5) . . ?
Ge2 O8 Mo12 127.7(5) . . ?
Mo18 O8 Mo12 95.5(3) . . ?
Mo17 O9 Mo18 160.4(6) . . ?
Mo11 O10 Mo2 115.6(4) . . ?
Mo18 O11 Gd1 136.1(5) . . ?
Mo12 O12 Gd1 138.5(5) . . ?
Mo7 O13 Gd1 132.1(5) . . ?
Mo21 O14 Gd1 132.4(5) . . ?
Mo3 O15 Gd1 153.3(5) . . ?
Mo7 O16 Mo21 115.1(4) . . ?
Mo21 O17 Mo16 160.5(6) . . ?
Mo16 O18 Mo3 117.5(4) . . ?
Ge1 O19 Mo3 120.0(4) . . ?
Ge1 O19 Mo16 122.5(5) . . ?
Mo3 O19 Mo16 95.5(3) . . ?
Ge1 O19 Mo1 123.1(5) . . ?
Mo3 O19 Mo1 96.2(3) . . ?
Mo16 O19 Mo1 92.4(3) . . ?
Ge1 O20 Mo13 119.7(5) . . ?
Ge1 O20 Mo19 119.2(4) . . ?
Mo13 O20 Mo19 102.6(4) . . ?
Ge1 O20 Mo4 121.3(5) . . ?
Mo13 O20 Mo4 93.7(3) . . ?
Mo19 O20 Mo4 94.9(3) . . ?
Mo2 O22 Mo5 145.6(5) . . ?
Mo6 O23 Mo8 118.1(4) . . ?
Mo8 O24 Mo12 156.3(5) . . ?
Mo11 O25 Mo12 152.2(5) . . ?
Mo18 O26 Mo12 113.6(5) . . ?
Mo10 O27 Gd1 161.5(6) . . ?
Ge2 O29 Mo17 121.2(5) . . ?
Ge2 O29 Mo9 121.4(5) . . ?
Mo17 O29 Mo9 93.8(3) . . ?
Ge2 O29 Mo5 125.6(5) . . ?
Mo17 O29 Mo5 92.5(3) . . ?
Mo9 O29 Mo5 94.2(3) . . ?
Mo4 O32 Mo7 156.2(6) . . ?
Mo4 O33 Mo13 117.3(5) . . ?
Mo13 O34 Mo16 146.6(5) . . ?
Mo1 O36 Mo3 118.9(5) . . ?
Mo3 O37 Mo22 139.7(5) . . ?
Mo22 O38 Mo20 119.6(5) . . ?
Ge1 O39 Mo21 127.1(5) . . ?
Ge1 O39 Mo7 124.9(4) . . ?
Mo21 O39 Mo7 96.3(3) . . ?
Mo8 O40 Mo11 145.8(5) . . ?
Ge2 O41 Mo2 121.4(4) . . ?
Ge2 O41 Mo15 116.9(5) . . ?
Mo2 O41 Mo15 101.4(4) . . ?
Ge2 O41 Mo11 117.7(5) . . ?
Mo2 O41 Mo11 102.4(4) . . ?
Mo15 O41 Mo11 91.9(3) . . ?
Mo15 O42 Mo17 147.2(6) . . ?
Mo15 O43 Mo2 117.2(4) . . ?
Mo6 O44 Mo5 162.1(5) . . ?
Mo6 O46 Mo10 118.3(5) . . ?
Mo10 O47 Mo8 120.4(5) . . ?
Mo17 O48 Mo9 119.2(5) . . ?
Mo14 O50 Mo22 119.0(5) . . ?
Mo14 O52 Mo1 156.9(6) . . ?
Ge1 O53 Mo20 119.8(5) . . ?
Ge1 O53 Mo22 121.1(5) . . ?
Mo20 O53 Mo22 94.7(4) . . ?
Ge1 O53 Mo14 126.4(5) . . ?
Mo20 O53 Mo14 93.2(3) . . ?
Mo22 O53 Mo14 93.7(3) . . ?
Mo20 O54 Mo7 152.4(5) . . ?
Mo19 O56 Mo14 149.2(6) . . ?
Mo13 O58 Mo19 117.5(5) . . ?
Mo22 O59 Gd1 163.0(6) . . ?
Mo9 O60 Gd1 153.6(6) . . ?
Mo15 O64 Mo18 148.9(5) . . ?
Mo11 O66 Mo15 118.4(5) . . ?
Mo14 O70 Mo20 119.6(5) . . ?
Mo16 O73 Mo1 118.0(5) . . ?
Mo19 O74 Mo1 148.9(5) . . ?
Mo13 O75 Mo21 144.7(5) . . ?
C1 O79 C3 112.1(13) . . ?
C6 O80 C8 112.3(13) . . ?
C11 O81 C12 107.4(17) . . ?
C13 O82 C16 109(2) . . ?
C19 O83 C17 99(2) . . ?
C22 O84 C24 111.7(17) . . ?
C27 O85 C25 107(3) . . ?
C15 N1 C14 106(2) . . ?
C4 N2 C2 110.7(15) . . ?
C7 N3 C5 112.7(14) . . ?
C9 N4 C10 110.1(14) . . ?
C18 N5 C20 113(2) . . ?
C21 N6 C23 102(2) . . ?
C26 N7 C28 114(4) . . ?
O79 C1 C2 107.6(15) . . ?
N2 C2 C1 112.9(16) . . ?
C4 C3 O79 109.2(13) . . ?
N2 C4 C3 112.5(16) . . ?
N3 C5 C6 112.3(15) . . ?
C5 C6 O80 111.9(15) . . ?
N3 C7 C8 112.2(16) . . ?
O80 C8 C7 107.7(13) . . ?
C11 C9 N4 110.7(16) . . ?
C12 C10 N4 106.9(17) . . ?
O81 C11 C9 111.5(17) . . ?
O82 C13 C14 106(2) . . ?
N1 C14 C13 110(2) . . ?
N1 C15 C16 108(2) . . ?
O82 C16 C15 110(2) . . ?
C18 C17 O83 113(2) . . ?
C17 C18 N5 107(2) . . ?
O83 C19 C20 109(2) . . ?
N5 C20 C19 109(2) . . ?
C22 C21 N6 116(3) . . ?
C21 C22 O84 110(2) . . ?
C24 C23 N6 111(3) . . ?
C23 C24 O84 108(2) . . ?
C26 C25 O85 110(3) . . ?
N7 C26 C25 120(3) . . ?
O85 C27 C28 125(4) . . ?
C27 C28 N7 108(4) . . ?
O39 Ge1 O19 110.4(4) . . ?
O39 Ge1 O53 112.4(4) . . ?
O19 Ge1 O53 106.5(4) . . ?
O39 Ge1 O20 108.6(4) . . ?
O19 Ge1 O20 109.0(4) . . ?
O53 Ge1 O20 110.0(4) . . ?
O7 Ge2 O29 106.5(4) . . ?
O7 Ge2 O8 110.8(4) . . ?
O29 Ge2 O8 110.5(4) . . ?
O7 Ge2 O41 109.1(4) . . ?
O29 Ge2 O41 109.7(4) . . ?
O8 Ge2 O41 110.1(4) . . ?
O72 Mo1 O36 104.5(5) . . ?
O72 Mo1 O52 102.9(5) . . ?
O36 Mo1 O52 93.8(4) . . ?
O72 Mo1 O73 95.6(5) . . ?
O36 Mo1 O73 90.8(4) . . ?
O52 Mo1 O73 159.1(4) . . ?
O72 Mo1 O74 98.2(5) . . ?
O36 Mo1 O74 157.2(4) . . ?
O52 Mo1 O74 83.4(4) . . ?
O73 Mo1 O74 84.5(4) . . ?
O72 Mo1 O19 169.2(4) . . ?
O36 Mo1 O19 74.3(4) . . ?
O52 Mo1 O19 87.9(4) . . ?
O73 Mo1 O19 73.7(4) . . ?
O74 Mo1 O19 82.9(4) . . ?
O78 Mo2 O6 104.9(5) . . ?
O78 Mo2 O22 105.6(5) . . ?
O6 Mo2 O22 96.1(4) . . ?
O78 Mo2 O43 93.9(5) . . ?
O6 Mo2 O43 158.8(4) . . ?
O22 Mo2 O43 87.9(4) . . ?
O78 Mo2 O10 92.1(5) . . ?
O6 Mo2 O10 86.4(4) . . ?
O22 Mo2 O10 160.7(4) . . ?
O43 Mo2 O10 83.3(4) . . ?
O78 Mo2 O41 158.5(4) . . ?
O6 Mo2 O41 88.3(4) . . ?
O22 Mo2 O41 89.3(4) . . ?
O43 Mo2 O41 70.9(3) . . ?
O10 Mo2 O41 71.6(3) . . ?
O51 Mo3 O15 104.2(5) . . ?
O51 Mo3 O37 105.3(5) . . ?
O15 Mo3 O37 98.4(5) . . ?
O51 Mo3 O18 91.8(4) . . ?
O15 Mo3 O18 89.6(4) . . ?
O37 Mo3 O18 158.6(4) . . ?
O51 Mo3 O36 92.7(5) . . ?
O15 Mo3 O36 160.0(4) . . ?
O37 Mo3 O36 87.1(4) . . ?
O18 Mo3 O36 79.1(4) . . ?
O51 Mo3 O19 157.7(4) . . ?
O15 Mo3 O19 90.8(4) . . ?
O37 Mo3 O19 88.4(4) . . ?
O18 Mo3 O19 71.5(3) . . ?
O36 Mo3 O19 70.1(3) . . ?
O31 Mo4 O32 102.2(5) . . ?
O31 Mo4 O33 103.9(5) . . ?
O32 Mo4 O33 96.9(4) . . ?
O31 Mo4 O5 98.8(5) . . ?
O32 Mo4 O5 155.0(4) . . ?
O33 Mo4 O5 91.0(4) . . ?
O31 Mo4 O4 96.8(5) . . ?
O32 Mo4 O4 83.8(4) . . ?
O33 Mo4 O4 158.6(4) . . ?
O5 Mo4 O4 80.3(4) . . ?
O31 Mo4 O20 170.6(5) . . ?
O32 Mo4 O20 87.1(4) . . ?
O33 Mo4 O20 75.9(4) . . ?
O5 Mo4 O20 71.9(4) . . ?
O4 Mo4 O20 82.8(3) . . ?
O21 Mo5 O2 104.2(5) . . ?
O21 Mo5 O3 100.2(5) . . ?
O2 Mo5 O3 95.2(4) . . ?
O21 Mo5 O44 100.8(5) . . ?
O2 Mo5 O44 95.8(4) . . ?
O3 Mo5 O44 153.1(4) . . ?
O21 Mo5 O22 94.8(4) . . ?
O2 Mo5 O22 161.0(4) . . ?
O3 Mo5 O22 82.0(4) . . ?
O44 Mo5 O22 79.6(4) . . ?
O21 Mo5 O29 174.5(4) . . ?
O2 Mo5 O29 77.0(4) . . ?
O3 Mo5 O29 74.3(4) . . ?
O44 Mo5 O29 84.3(4) . . ?
O22 Mo5 O29 84.2(3) . . ?
O45 Mo6 O46 104.1(5) . . ?
O45 Mo6 O44 102.8(5) . . ?
O46 Mo6 O44 95.1(5) . . ?
O45 Mo6 O23 98.3(5) . . ?
O46 Mo6 O23 94.7(4) . . ?
O44 Mo6 O23 153.8(4) . . ?
O45 Mo6 O6 95.7(5) . . ?
O46 Mo6 O6 160.2(4) . . ?
O44 Mo6 O6 81.2(4) . . ?
O23 Mo6 O6 81.4(4) . . ?
O45 Mo6 O7 172.1(4) . . ?
O46 Mo6 O7 77.5(4) . . ?
O44 Mo6 O7 84.7(4) . . ?
O23 Mo6 O7 73.8(3) . . ?
O6 Mo6 O7 82.8(3) . . ?
O68 Mo7 O13 102.7(5) . . ?
O68 Mo7 O16 96.7(5) . . ?
O13 Mo7 O16 96.5(4) . . ?
O68 Mo7 O54 101.0(5) . . ?
O13 Mo7 O54 95.0(4) . . ?
O16 Mo7 O54 156.2(4) . . ?
O68 Mo7 O32 90.4(5) . . ?
O13 Mo7 O32 166.7(4) . . ?
O16 Mo7 O32 84.5(4) . . ?
O54 Mo7 O32 79.6(4) . . ?
O68 Mo7 O39 167.7(5) . . ?
O13 Mo7 O39 85.7(4) . . ?
O16 Mo7 O39 73.1(3) . . ?
O54 Mo7 O39 87.1(3) . . ?
O32 Mo7 O39 81.9(4) . . ?
O61 Mo8 O24 103.3(5) . . ?
O61 Mo8 O40 102.1(5) . . ?
O24 Mo8 O40 89.1(4) . . ?
O61 Mo8 O47 98.2(5) . . ?
O24 Mo8 O47 90.6(4) . . ?
O40 Mo8 O47 159.2(4) . . ?
O61 Mo8 O23 96.8(4) . . ?
O24 Mo8 O23 159.9(4) . . ?
O40 Mo8 O23 86.8(4) . . ?
O47 Mo8 O23 86.4(4) . . ?
O61 Mo8 O7 167.8(4) . . ?
O24 Mo8 O7 85.6(4) . . ?
O40 Mo8 O7 86.2(4) . . ?
O47 Mo8 O7 73.0(4) . . ?
O23 Mo8 O7 74.6(4) . . ?
O77 Mo9 O60 104.2(5) . . ?
O77 Mo9 O1 104.6(5) . . ?
O60 Mo9 O1 97.1(5) . . ?
O77 Mo9 O48 96.1(5) . . ?
O60 Mo9 O48 92.4(4) . . ?
O1 Mo9 O48 154.3(4) . . ?
O77 Mo9 O2 91.5(5) . . ?
O60 Mo9 O2 163.4(4) . . ?
O1 Mo9 O2 83.9(4) . . ?
O48 Mo9 O2 80.4(4) . . ?
O77 Mo9 O29 159.7(5) . . ?
O60 Mo9 O29 92.6(4) . . ?
O1 Mo9 O29 84.1(4) . . ?
O48 Mo9 O29 71.5(4) . . ?
O2 Mo9 O29 71.0(3) . . ?
O28 Mo10 O27 105.2(5) . . ?
O28 Mo10 O47 101.0(5) . . ?
O27 Mo10 O47 99.1(4) . . ?
O28 Mo10 O1 100.8(5) . . ?
O27 Mo10 O1 90.6(4) . . ?
O47 Mo10 O1 152.8(4) . . ?
O28 Mo10 O46 91.8(5) . . ?
O27 Mo10 O46 162.4(4) . . ?
O47 Mo10 O46 81.6(4) . . ?
O1 Mo10 O46 81.7(4) . . ?
O28 Mo10 O7 161.5(5) . . ?
O27 Mo10 O7 92.9(4) . . ?
O47 Mo10 O7 71.9(3) . . ?
O1 Mo10 O7 82.3(4) . . ?
O46 Mo10 O7 70.5(3) . . ?
O65 Mo11 O25 103.5(5) . . ?
O65 Mo11 O66 100.5(5) . . ?
O25 Mo11 O66 98.3(4) . . ?
O65 Mo11 O40 100.9(5) . . ?
O25 Mo11 O40 89.7(4) . . ?
O66 Mo11 O40 154.7(4) . . ?
O65 Mo11 O10 96.0(4) . . ?
O25 Mo11 O10 159.5(4) . . ?
O66 Mo11 O10 84.3(4) . . ?
O40 Mo11 O10 80.1(4) . . ?
O65 Mo11 O41 165.8(4) . . ?
O25 Mo11 O41 90.5(4) . . ?
O66 Mo11 O41 74.6(4) . . ?
O40 Mo11 O41 81.4(4) . . ?
O10 Mo11 O41 70.5(3) . . ?
O62 Mo12 O12 103.9(5) . . ?
O62 Mo12 O26 98.3(4) . . ?
O12 Mo12 O26 97.4(4) . . ?
O62 Mo12 O24 98.4(4) . . ?
O12 Mo12 O24 97.0(4) . . ?
O26 Mo12 O24 154.6(4) . . ?
O62 Mo12 O25 90.7(4) . . ?
O12 Mo12 O25 165.3(4) . . ?
O26 Mo12 O25 82.3(4) . . ?
O24 Mo12 O25 78.5(4) . . ?
O62 Mo12 O8 168.0(4) . . ?
O12 Mo12 O8 86.1(4) . . ?
O26 Mo12 O8 73.4(4) . . ?
O24 Mo12 O8 86.9(4) . . ?
O25 Mo12 O8 79.8(3) . . ?
O76 Mo13 O75 105.0(5) . . ?
O76 Mo13 O34 105.2(5) . . ?
O75 Mo13 O34 96.5(4) . . ?
O76 Mo13 O58 95.0(5) . . ?
O75 Mo13 O58 157.8(4) . . ?
O34 Mo13 O58 87.4(4) . . ?
O76 Mo13 O33 92.9(4) . . ?
O75 Mo13 O33 86.8(4) . . ?
O34 Mo13 O33 160.0(4) . . ?
O58 Mo13 O33 82.4(4) . . ?
O76 Mo13 O20 160.4(4) . . ?
O75 Mo13 O20 87.6(4) . . ?
O34 Mo13 O20 87.9(4) . . ?
O58 Mo13 O20 70.7(4) . . ?
O33 Mo13 O20 72.5(3) . . ?
O71 Mo14 O50 103.6(5) . . ?
O71 Mo14 O52 100.9(5) . . ?
O50 Mo14 O52 92.8(5) . . ?
O71 Mo14 O70 100.5(5) . . ?
O50 Mo14 O70 93.2(4) . . ?
O52 Mo14 O70 155.7(4) . . ?
O71 Mo14 O56 98.9(5) . . ?
O50 Mo14 O56 157.4(4) . . ?
O52 Mo14 O56 82.0(4) . . ?
O70 Mo14 O56 83.4(4) . . ?
O71 Mo14 O53 173.1(4) . . ?
O50 Mo14 O53 75.8(4) . . ?
O52 Mo14 O53 86.0(4) . . ?
O70 Mo14 O53 72.7(4) . . ?
O56 Mo14 O53 81.9(4) . . ?
O67 Mo15 O64 105.5(5) . . ?
O67 Mo15 O42 105.1(5) . . ?
O64 Mo15 O42 93.2(4) . . ?
O67 Mo15 O66 96.4(5) . . ?
O64 Mo15 O66 91.9(4) . . ?
O42 Mo15 O66 155.7(4) . . ?
O67 Mo15 O43 94.9(5) . . ?
O64 Mo15 O43 159.2(4) . . ?
O42 Mo15 O43 85.0(4) . . ?
O66 Mo15 O43 81.9(4) . . ?
O67 Mo15 O41 162.0(4) . . ?
O64 Mo15 O41 89.0(4) . . ?
O42 Mo15 O41 84.2(4) . . ?
O66 Mo15 O41 72.1(3) . . ?
O43 Mo15 O41 70.1(3) . . ?
O35 Mo16 O18 101.7(5) . . ?
O35 Mo16 O73 100.8(5) . . ?
O18 Mo16 O73 92.6(4) . . ?
O35 Mo16 O17 100.8(5) . . ?
O18 Mo16 O17 94.2(4) . . ?
O73 Mo16 O17 155.6(4) . . ?
O35 Mo16 O34 96.9(5) . . ?
O18 Mo16 O34 161.4(4) . . ?
O73 Mo16 O34 84.4(4) . . ?
O17 Mo16 O34 81.7(4) . . ?
O35 Mo16 O19 174.7(4) . . ?
O18 Mo16 O19 75.1(4) . . ?
O73 Mo16 O19 75.3(4) . . ?
O17 Mo16 O19 83.8(4) . . ?
O34 Mo16 O19 86.4(4) . . ?
O30 Mo17 O48 101.3(5) . . ?
O30 Mo17 O9 104.3(5) . . ?
O48 Mo17 O9 93.6(4) . . ?
O30 Mo17 O3 97.5(5) . . ?
O48 Mo17 O3 89.8(4) . . ?
O9 Mo17 O3 156.9(4) . . ?
O30 Mo17 O42 98.6(5) . . ?
O48 Mo17 O42 159.8(4) . . ?
O9 Mo17 O42 84.2(4) . . ?
O3 Mo17 O42 84.7(4) . . ?
O30 Mo17 O29 170.5(4) . . ?
O48 Mo17 O29 74.6(4) . . ?
O9 Mo17 O29 84.7(4) . . ?
O3 Mo17 O29 74.1(4) . . ?
O42 Mo17 O29 85.2(4) . . ?
O63 Mo18 O11 103.5(5) . . ?
O63 Mo18 O26 97.9(4) . . ?
O11 Mo18 O26 96.0(4) . . ?
O63 Mo18 O9 99.1(4) . . ?
O11 Mo18 O9 98.2(4) . . ?
O26 Mo18 O9 154.6(4) . . ?
O63 Mo18 O8 167.1(4) . . ?
O11 Mo18 O8 87.5(4) . . ?
O26 Mo18 O8 73.9(4) . . ?
O9 Mo18 O8 85.7(4) . . ?
O63 Mo18 O64 89.3(5) . . ?
O11 Mo18 O64 167.1(4) . . ?
O26 Mo18 O64 83.3(4) . . ?
O9 Mo18 O64 78.2(4) . . ?
O8 Mo18 O64 80.0(4) . . ?
O57 Mo19 O56 104.6(5) . . ?
O57 Mo19 O74 104.3(5) . . ?
O56 Mo19 O74 91.1(4) . . ?
O57 Mo19 O5 97.5(5) . . ?
O56 Mo19 O5 94.1(4) . . ?
O74 Mo19 O5 155.5(4) . . ?
O57 Mo19 O58 93.8(5) . . ?
O56 Mo19 O58 161.7(4) . . ?
O74 Mo19 O58 83.8(4) . . ?
O5 Mo19 O58 83.8(4) . . ?
O57 Mo19 O20 160.8(4) . . ?
O56 Mo19 O20 92.9(4) . . ?
O74 Mo19 O20 83.0(4) . . ?
O5 Mo19 O20 72.8(4) . . ?
O58 Mo19 O20 69.0(4) . . ?
O69 Mo20 O4 102.4(5) . . ?
O69 Mo20 O54 102.2(5) . . ?
O4 Mo20 O54 90.9(4) . . ?
O69 Mo20 O70 97.6(5) . . ?
O4 Mo20 O70 93.4(4) . . ?
O54 Mo20 O70 158.4(4) . . ?
O69 Mo20 O38 96.9(5) . . ?
O4 Mo20 O38 160.6(4) . . ?
O54 Mo20 O38 85.8(4) . . ?
O70 Mo20 O38 83.1(4) . . ?
O69 Mo20 O53 166.6(5) . . ?
O4 Mo20 O53 88.9(4) . . ?
O54 Mo20 O53 84.6(4) . . ?
O70 Mo20 O53 74.4(4) . . ?
O38 Mo20 O53 71.8(4) . . ?
O55 Mo21 O14 102.7(5) . . ?
O55 Mo21 O17 100.3(4) . . ?
O14 Mo21 O17 98.8(4) . . ?
O55 Mo21 O16 97.7(4) . . ?
O14 Mo21 O16 94.4(4) . . ?
O17 Mo21 O16 154.7(4) . . ?
O55 Mo21 O75 89.1(4) . . ?
O14 Mo21 O75 168.0(4) . . ?
O17 Mo21 O75 80.5(4) . . ?
O16 Mo21 O75 82.1(4) . . ?
O55 Mo21 O39 168.2(4) . . ?
O14 Mo21 O39 86.0(4) . . ?
O17 Mo21 O39 86.1(4) . . ?
O16 Mo21 O39 73.3(3) . . ?
O75 Mo21 O39 82.1(4) . . ?
O49 Mo22 O59 104.5(5) . . ?
O49 Mo22 O38 102.1(5) . . ?
O59 Mo22 O38 99.9(4) . . ?
O49 Mo22 O37 98.0(5) . . ?
O59 Mo22 O37 89.8(4) . . ?
O38 Mo22 O37 154.6(4) . . ?
O49 Mo22 O50 92.4(5) . . ?
O59 Mo22 O50 160.4(4) . . ?
O38 Mo22 O50 85.8(4) . . ?
O37 Mo22 O50 78.0(4) . . ?
O49 Mo22 O53 163.0(5) . . ?
O59 Mo22 O53 92.4(4) . . ?
O38 Mo22 O53 73.3(4) . . ?
O37 Mo22 O53 83.0(4) . . ?
O50 Mo22 O53 71.2(3) . . ?
O59 Gd1 O13 75.8(3) . . ?
O59 Gd1 O15 70.9(3) . . ?
O13 Gd1 O15 118.7(3) . . ?
O59 Gd1 O14 119.5(3) . . ?
O13 Gd1 O14 77.0(3) . . ?
O15 Gd1 O14 76.9(3) . . ?
O59 Gd1 O12 149.6(3) . . ?
O13 Gd1 O12 134.0(3) . . ?
O15 Gd1 O12 86.0(3) . . ?
O14 Gd1 O12 71.6(3) . . ?
O59 Gd1 O27 81.1(3) . . ?
O13 Gd1 O27 148.5(3) . . ?
O15 Gd1 O27 72.0(3) . . ?
O14 Gd1 O27 133.8(3) . . ?
O12 Gd1 O27 72.9(3) . . ?
O59 Gd1 O60 71.8(3) . . ?
O13 Gd1 O60 83.1(3) . . ?
O15 Gd1 O60 129.3(3) . . ?
O14 Gd1 O60 153.0(3) . . ?
O12 Gd1 O60 111.9(3) . . ?
O27 Gd1 O60 69.4(4) . . ?
O59 Gd1 O11 133.4(3) . . ?
O13 Gd1 O11 70.8(3) . . ?
O15 Gd1 O11 155.0(3) . . ?
O14 Gd1 O11 83.5(3) . . ?
O12 Gd1 O11 73.0(3) . . ?
O27 Gd1 O11 113.0(3) . . ?
O60 Gd1 O11 72.8(3) . . ?
C10 C12 O81 113.8(19) . . ?

_refine_diff_density_max         0.938
_refine_diff_density_min         -0.872
_refine_diff_density_rms         0.154

_shelxl_version_number           2014-3


_vrf_CHEMW03_2_sq                
;
CHEMW03_ALERT_2_B

RESPONSE: Use of Platon SQUEEZE to remove disordered solvent. The accessible
solvent void in the crystal structure indicates that some more water molecules
and morpholine should exist in the structure, but cannot be found from the
weak residual electron peaks. Based on the TG analyses and elemental analysis,
13 water molecules and 8 morpholine were included in the sum formula.
;
_vrf_PLAT342_2_sq                
;
PLAT342_ALERT_3_B Low Bond Precision on C-C Bonds .............. 0.035 Ang.

RESPONSE: The low bond distance precision is likely due to the low data to
parameter ratio. There is a large amount of disorder in the structure. This is
common in high nuclearity polyoxometalate cluster . (such as Angew. Chem. Int.
Ed, 2010, 49, 6984; Angew. Chem. Int. Ed, 2008, 47, 6881, J. Am. Chem. Soc,
2004, 126, 13880.)
;
_vrf_PLAT430_2_sq                
;
PLAT430_ALERT_2_B Short Inter D...A Contact O10...O35 ......2.80 Ang.

RESPONSE: The structure contains a high degree of disorder.
;

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_3_sq
_database_code_depnum_ccdc_archive 'CCDC 991334'
_audit_update_record             
;
2017-10-04 deposited with the CCDC.
2017-10-09 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C32 H115 Dy Ge2 Mo22 N8 O101'
_chemical_formula_weight         4646.67

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           7
_space_group_name_H-M_alt        'P n'
_space_group_name_Hall           'P -2yac'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'x+1/2, -y, z+1/2'

_cell_length_a                   13.2127(3)
_cell_length_b                   12.7291(3)
_cell_length_c                   32.5182(10)
_cell_angle_alpha                90
_cell_angle_beta                 96.158(2)
_cell_angle_gamma                90
_cell_volume                     5437.5(2)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    9769
_cell_measurement_theta_min      3.0216
_cell_measurement_theta_max      29.1969

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_density_diffrn    2.838
_exptl_crystal_F_000             4450
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.420
_exptl_crystal_size_mid          0.340
_exptl_crystal_size_min          0.300
_exptl_absorpt_coefficient_mu    3.790
_shelx_estimated_absorpt_T_min   0.299
_shelx_estimated_absorpt_T_max   0.396
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.69195
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   ?

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Enhance (Mo) X-ray Source'
_diffrn_measurement_device_type  'Xcalibur, Ruby, Gemini ultra'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            20012
_diffrn_reflns_av_unetI/netI     0.0494
_diffrn_reflns_av_R_equivalents  0.0305
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -24
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_theta_min         3.028
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measured_fraction_theta_full 0.971
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_Laue_measured_fraction_full 0.971
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_point_group_measured_fraction_full 0.972
_reflns_number_total             14249
_reflns_number_gt                13731
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.999
_reflns_Friedel_fraction_max     0.996
_reflns_Friedel_fraction_full    0.972

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_cell_refinement       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction        
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXTL

_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0789P)²+1.5808P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.804(12)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         14249
_refine_ls_number_parameters     1243
_refine_ls_number_restraints     107
_refine_ls_R_factor_all          0.0417
_refine_ls_R_factor_gt           0.0399
_refine_ls_wR_factor_ref         0.1129
_refine_ls_wR_factor_gt          0.1110
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_restrained_S_all      9.738
_refine_ls_shift/su_max          0.007
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.0196(7) 0.2513(8) 0.9163(3) 0.021(2) Uani 1 1 d . U . . .
O2 O 0.0593(7) 0.1958(8) 0.8394(3) 0.020(2) Uani 1 1 d . . . . .
O3 O -0.1185(7) 0.2434(8) 0.8547(3) 0.017(2) Uani 1 1 d . . . . .
O4 O -0.0694(8) 0.0297(8) 0.8464(3) 0.021(2) Uani 1 1 d . . . . .
O5 O -0.3279(7) -0.0791(8) 0.8011(3) 0.020(2) Uani 1 1 d . . . . .
O6 O -0.0804(8) 0.1923(8) 0.7719(3) 0.020(2) Uani 1 1 d . . . . .
O7 O -0.1389(8) 0.3912(8) 0.7875(4) 0.026(3) Uani 1 1 d . . . . .
O8 O -0.0444(7) 0.0226(8) 0.7008(3) 0.018(2) Uani 1 1 d . . . . .
O9 O -0.2530(8) -0.0281(8) 0.6721(3) 0.021(2) Uani 1 1 d . U . . .
O10 O -0.1227(7) 0.0576(7) 0.6219(3) 0.014(2) Uani 1 1 d . U . . .
O11 O -0.3274(8) 0.0147(8) 0.5902(3) 0.021(2) Uani 1 1 d . . . . .
O12 O -0.4220(7) 0.2034(8) 0.5908(3) 0.023(2) Uani 1 1 d . . . . .
O13 O -0.3767(8) 0.2309(8) 0.5122(3) 0.022(2) Uani 1 1 d . . . . .
O14 O -0.3194(8) 0.4315(9) 0.4881(3) 0.028(3) Uani 1 1 d . . . . .
O15 O -0.1949(8) 0.3643(8) 0.6346(3) 0.022(2) Uani 1 1 d . . . . .
O16 O -0.0356(7) 0.2538(7) 0.6006(3) 0.013(2) Uani 1 1 d . . . . .
O17 O -0.0839(7) 0.0988(8) 0.5387(3) 0.018(2) Uani 1 1 d . . . . .
O18 O 0.0004(8) 0.2898(8) 0.5148(3) 0.020(2) Uani 1 1 d . . . . .
O19 O 0.0584(8) 0.0981(8) 0.4919(3) 0.021(2) Uani 1 1 d D . . . .
O20 O -0.4295(8) 0.2183(8) 0.9364(3) 0.023(2) Uani 1 1 d . . . . .
O21 O -0.5763(8) 0.0780(9) 0.9015(4) 0.031(3) Uani 1 1 d D . . . .
O22 O -0.4446(8) 0.0510(8) 0.8442(4) 0.026(2) Uani 1 1 d . . . . .
O23 O -0.1423(8) -0.1751(8) 0.8265(3) 0.027(3) Uani 1 1 d . . . . .
O24 O -0.4918(8) 0.2434(8) 0.8577(3) 0.024(2) Uani 1 1 d . . . . .
O25 O -0.2622(7) 0.1032(7) 0.8105(3) 0.017(2) Uani 1 1 d . . . . .
O26 O -0.4258(8) 0.3855(8) 0.7622(3) 0.024(2) Uani 1 1 d . . . . .
O27 O -0.2932(7) 0.1687(7) 0.8918(3) 0.016(2) Uani 1 1 d . . . . .
O28 O -0.0972(7) 0.0839(8) 0.9217(3) 0.022(2) Uani 1 1 d . . . . .
O29 O 0.1027(8) 0.0555(8) 0.9032(4) 0.029(3) Uani 1 1 d . . . . .
O30 O 0.0037(7) 0.3957(8) 0.8553(3) 0.022(2) Uani 1 1 d . . . . .
O31 O -0.0935(7) -0.1290(7) 0.6416(3) 0.017(2) Uani 1 1 d . . . . .
O32 O -0.0903(7) 0.2380(8) 0.6873(3) 0.020(2) Uani 1 1 d . . . . .
O33 O -0.0450(9) 0.4456(9) 0.6964(3) 0.031(3) Uani 1 1 d . . . . .
O34 O 0.0844(8) 0.1048(8) 0.6473(3) 0.023(2) Uani 1 1 d . . . . .
O35 O -0.2339(8) -0.0418(8) 0.8783(3) 0.026(2) Uani 1 1 d . . . . .
O36 O 0.1250(7) 0.3395(8) 0.5808(3) 0.022(2) Uani 1 1 d . . . . .
O37 O 0.0344(10) 0.5035(8) 0.5355(4) 0.034(3) Uani 1 1 d . . . . .
O38 O 0.0406(7) -0.0454(8) 0.5930(3) 0.019(2) Uani 1 1 d . . . . .
O39 O -0.3368(7) 0.3875(7) 0.5698(3) 0.020(2) Uani 1 1 d . . . . .
O40 O -0.0212(8) 0.4552(8) 0.6110(3) 0.024(2) Uani 1 1 d . . . . .
O41 O 0.0637(8) 0.3414(8) 0.7782(4) 0.026(2) Uani 1 1 d . . . . .
O42 O -0.3414(8) 0.3949(8) 0.9077(3) 0.026(2) Uani 1 1 d . . . . .
O43 O -0.1782(8) 0.4571(8) 0.8772(3) 0.027(2) Uani 1 1 d . . . . .
O44 O -0.3100(8) 0.3428(9) 0.9903(3) 0.026(2) Uani 1 1 d . . . . .
O45 O -0.2443(8) 0.1446(8) 0.9666(3) 0.026(2) Uani 1 1 d D . . . .
O46 O -0.3775(8) 0.0133(8) 0.9246(3) 0.025(2) Uani 1 1 d D . . . .
O47 O -0.3134(7) 0.3200(7) 0.8254(3) 0.017(2) Uani 1 1 d . . . . .
O48 O -0.1547(7) -0.0253(8) 0.7665(3) 0.020(2) Uani 1 1 d . . . . .
O49 O -0.3562(7) 0.0576(8) 0.7341(3) 0.023(2) Uani 1 1 d . . . . .
O50 O 0.0878(7) 0.3134(8) 0.6596(3) 0.019(2) Uani 1 1 d . U . . .
O51 O 0.1021(8) -0.1010(9) 0.6756(3) 0.028(3) Uani 1 1 d . . . . .
O52 O 0.1210(8) 0.1320(8) 0.5702(3) 0.022(2) Uani 1 1 d . U . . .
O53 O 0.1749(8) -0.0601(9) 0.5363(3) 0.027(3) Uani 1 1 d D . . . .
O54 O -0.1819(8) -0.0951(8) 0.5616(3) 0.024(2) Uani 1 1 d . . . . .
O55 O -0.1443(8) 0.0549(8) 0.4643(3) 0.023(2) Uani 1 1 d D . . . .
O56 O -0.1932(7) 0.2506(8) 0.4870(3) 0.021(2) Uani 1 1 d . . . . .
O57 O -0.0451(9) 0.2272(9) 0.4339(3) 0.031(3) Uani 1 1 d . U . . .
O58 O -0.2408(7) 0.2105(7) 0.5729(3) 0.014(2) Uani 1 1 d . . . . .
O59 O -0.1465(8) 0.3945(8) 0.5428(3) 0.021(2) Uani 1 1 d . . . . .
O60 O -0.6075(9) 0.3381(10) 0.7940(4) 0.039(3) Uani 1 1 d . . . . .
O61 O -0.0051(9) 0.4570(10) 0.9356(4) 0.034(3) Uani 1 1 d . . . . .
O62 O -0.3338(9) 0.6041(9) 0.8783(4) 0.036(3) Uani 1 1 d . . . . .
O63 O -0.2878(8) 0.5144(8) 0.8053(3) 0.025(2) Uani 1 1 d . . . . .
O64 O -0.4536(8) 0.4493(9) 0.8392(3) 0.028(3) Uani 1 1 d . . . . .
O65 O -0.2732(9) 0.4752(9) 0.7226(4) 0.034(3) Uani 1 1 d . . . . .
O66 O -0.1656(8) 0.3135(8) 0.9336(3) 0.023(2) Uani 1 1 d . . . . .
O67 O -0.2004(8) -0.0704(9) 0.9620(3) 0.030(3) Uani 1 1 d . . . . .
O68 O -0.4589(7) 0.1847(8) 0.7831(3) 0.021(2) Uani 1 1 d . . . . .
O69 O -0.2672(8) 0.2655(8) 0.7406(3) 0.022(2) Uani 1 1 d . . . . .
O70 O -0.5188(8) -0.0224(9) 0.7663(4) 0.033(3) Uani 1 1 d . . . . .
O71 O 0.2561(8) 0.2207(9) 0.6327(3) 0.029(3) Uani 1 1 d . . . . .
O72 O -0.2899(8) -0.1898(8) 0.6194(4) 0.029(3) Uani 1 1 d . . . . .
O73 O -0.2878(8) 0.1919(8) 0.6590(3) 0.023(2) Uani 1 1 d . . . . .
O74 O -0.4025(9) 0.3640(9) 0.6475(4) 0.030(3) Uani 1 1 d . . . . .
O75 O -0.4908(8) 0.0604(10) 0.5304(4) 0.035(3) Uani 1 1 d . . . . .
O76 O -0.2900(7) 0.0433(8) 0.5142(3) 0.023(2) Uani 1 1 d . . . . .
O77 O -0.2225(9) -0.1427(10) 0.4788(4) 0.035(3) Uani 1 1 d . . . . .
O78 O -0.0293(8) -0.0794(8) 0.5121(3) 0.023(2) Uani 1 1 d . . . . .
O79 O 0.2248(11) 0.2539(11) 0.5118(4) 0.048(3) Uani 1 1 d . . . . .
O80 O 0.2118(10) 0.1608(12) 0.7843(5) 0.052(4) Uani 1 1 d . . . . .
O82 O 0.0344(14) 0.7186(12) 0.7350(5) 0.070(5) Uani 1 1 d . . . . .
O84 O 0.9217(17) 0.2540(19) 0.0487(7) 0.100(7) Uani 1 1 d . . . . .
C1 C 0.1705(15) 0.7992(19) 0.8952(7) 0.052(6) Uani 1 1 d . . . . .
H1A H 0.1490 0.8380 0.8701 0.063 Uiso 1 1 calc R U . . .
H1B H 0.2440 0.8041 0.9005 0.063 Uiso 1 1 calc R U . . .
C2 C 0.140(2) 0.689(2) 0.8900(8) 0.075(8) Uani 1 1 d . . . . .
H2A H 0.1742 0.6578 0.8680 0.090 Uiso 1 1 calc R U . . .
H2B H 0.1604 0.6508 0.9153 0.090 Uiso 1 1 calc R U . . .
C3 C 0.0066(13) 0.8307(14) 0.9230(6) 0.036(4) Uani 1 1 d . . . . .
H3A H -0.0262 0.8525 0.9469 0.043 Uiso 1 1 calc R U . . .
H3B H -0.0204 0.8727 0.8995 0.043 Uiso 1 1 calc R U . . .
C4 C -0.0131(18) 0.7185(18) 0.9145(7) 0.058(6) Uani 1 1 d . . . . .
H4A H 0.0130 0.6779 0.9386 0.070 Uiso 1 1 calc R U . . .
H4B H -0.0860 0.7072 0.9100 0.070 Uiso 1 1 calc R U . . .
C5 C 0.3002(12) 0.1084(15) 0.8064(7) 0.046(5) Uani 1 1 d . . . . .
H5A H 0.3339 0.1550 0.8271 0.055 Uiso 1 1 calc R U . . .
H5B H 0.3485 0.0892 0.7872 0.055 Uiso 1 1 calc R U . . .
C6 C 0.2617(17) 0.0091(18) 0.8271(8) 0.059(6) Uani 1 1 d . . . . .
H6A H 0.3186 -0.0278 0.8420 0.070 Uiso 1 1 calc R U . . .
H6B H 0.2146 0.0287 0.8467 0.070 Uiso 1 1 calc R U . . .
C7 C 0.1535(14) 0.0934(15) 0.7543(7) 0.042(5) Uani 1 1 d . . . . .
H7A H 0.1930 0.0778 0.7316 0.051 Uiso 1 1 calc R U . . .
H7B H 0.0913 0.1285 0.7433 0.051 Uiso 1 1 calc R U . . .
C8 C 0.1284(15) -0.0074(17) 0.7758(7) 0.049(5) Uani 1 1 d . . . . .
H8A H 0.0806 0.0083 0.7956 0.059 Uiso 1 1 calc R U . . .
H8B H 0.0951 -0.0553 0.7555 0.059 Uiso 1 1 calc R U . . .
C9 C 0.3805(15) 0.3417(15) 0.5426(7) 0.044(5) Uani 1 1 d . . . . .
H9A H 0.3439 0.3802 0.5621 0.052 Uiso 1 1 calc R U . . .
H9B H 0.4500 0.3317 0.5549 0.052 Uiso 1 1 calc R U . . .
C10 C 0.3306(12) 0.2368(14) 0.5334(6) 0.036(4) Uani 1 1 d . . . . .
H10A H 0.3268 0.1983 0.5589 0.044 Uiso 1 1 calc R U . . .
H10B H 0.3706 0.1959 0.5158 0.044 Uiso 1 1 calc R U . . .
C11 C 0.2808(18) 0.4200(16) 0.4834(8) 0.060(7) Uani 1 1 d . . . . .
H11A H 0.2885 0.4562 0.4577 0.072 Uiso 1 1 calc R U . . .
H11B H 0.2426 0.4653 0.5001 0.072 Uiso 1 1 calc R U . . .
C12 C 0.2236(16) 0.3205(16) 0.4744(7) 0.048(5) Uani 1 1 d . . . . .
H12A H 0.1538 0.3367 0.4641 0.057 Uiso 1 1 calc R U . . .
H12B H 0.2538 0.2821 0.4531 0.057 Uiso 1 1 calc R U . . .
C13 C 0.074(2) 0.689(2) 0.7750(10) 0.089(9) Uani 1 1 d . U . . .
H13A H 0.0676 0.7469 0.7939 0.107 Uiso 1 1 calc R U . . .
H13B H 0.1451 0.6714 0.7754 0.107 Uiso 1 1 calc R U . . .
C14 C 0.014(2) 0.593(2) 0.7889(10) 0.081(8) Uani 1 1 d . U . . .
H14A H 0.0147 0.5378 0.7684 0.097 Uiso 1 1 calc R U . . .
H14B H 0.0477 0.5666 0.8148 0.097 Uiso 1 1 calc R U . . .
C15 C -0.0674(17) 0.749(2) 0.7378(8) 0.065(7) Uani 1 1 d . . . . .
H15A H -0.0977 0.7743 0.7112 0.078 Uiso 1 1 calc R U . . .
H15B H -0.0692 0.8050 0.7578 0.078 Uiso 1 1 calc R U . . .
C16 C -0.128(2) 0.655(2) 0.7512(9) 0.078(8) Uani 1 1 d . U . . .
H16A H -0.1986 0.6746 0.7524 0.094 Uiso 1 1 calc R U . . .
H16B H -0.1261 0.5979 0.7314 0.094 Uiso 1 1 calc R U . . .
C17 C 0.371(3) 0.515(3) 0.9256(12) 0.108(11) Uani 1 1 d . U . . .
H17A H 0.3381 0.5360 0.9497 0.130 Uiso 1 1 calc R U . . .
H17B H 0.4077 0.5758 0.9170 0.130 Uiso 1 1 calc R U . . .
C18 C 0.447(2) 0.428(2) 0.9382(9) 0.076(8) Uani 1 1 d . U . . .
H18A H 0.4940 0.4196 0.9176 0.092 Uiso 1 1 calc R U . . .
H18B H 0.4852 0.4442 0.9645 0.092 Uiso 1 1 calc R U . . .
C19 C 0.301(2) 0.313(2) 0.9094(10) 0.079(8) Uani 1 1 d . U . . .
H19A H 0.3282 0.2915 0.8841 0.095 Uiso 1 1 calc R U . . .
H19B H 0.2583 0.2567 0.9176 0.095 Uiso 1 1 calc R U . . .
C20 C 0.242(2) 0.402(2) 0.9013(11) 0.087(9) Uani 1 1 d . U . . .
H20A H 0.1925 0.3883 0.8776 0.105 Uiso 1 1 calc R U . . .
H20B H 0.2044 0.4157 0.9248 0.105 Uiso 1 1 calc R U . . .
C21 C 1.052(2) 0.385(2) 0.0384(10) 0.086(9) Uani 1 1 d . U . . .
H21A H 1.0598 0.4545 0.0269 0.103 Uiso 1 1 calc R U . . .
H21B H 1.0866 0.3842 0.0663 0.103 Uiso 1 1 calc R U . . .
C22 C 0.937(2) 0.358(2) 0.0391(9) 0.073(7) Uani 1 1 d . U . . .
H22A H 0.9090 0.4027 0.0594 0.088 Uiso 1 1 calc R U . . .
H22B H 0.9009 0.3740 0.0123 0.088 Uiso 1 1 calc R U . . .
C23 C 1.065(2) 0.1973(19) 0.0180(8) 0.062(7) Uani 1 1 d . . . . .
H23A H 1.0875 0.1507 -0.0029 0.075 Uiso 1 1 calc R U . . .
H23B H 1.0919 0.1713 0.0450 0.075 Uiso 1 1 calc R U . . .
C24 C 0.962(2) 0.202(2) 0.0147(10) 0.084(8) Uani 1 1 d . U . . .
H24A H 0.9354 0.1309 0.0126 0.101 Uiso 1 1 calc R U . . .
H24B H 0.9382 0.2383 -0.0107 0.101 Uiso 1 1 calc R U . . .
N1 N 0.0313(12) 0.6816(11) 0.8800(5) 0.039(4) Uani 1 1 d . . . . .
H1C H 0.0113 0.7204 0.8578 0.047 Uiso 1 1 calc R U . . .
H1D H 0.0132 0.6152 0.8746 0.047 Uiso 1 1 calc R U . . .
N2 N 0.3796(12) 0.3996(12) 0.5050(6) 0.046(4) Uani 1 1 d . . . . .
H2C H 0.4162 0.3644 0.4881 0.055 Uiso 1 1 calc R U . . .
H2D H 0.4105 0.4608 0.5106 0.055 Uiso 1 1 calc R U . . .
N3 N 0.2124(13) -0.0568(13) 0.7962(5) 0.043(4) Uani 1 1 d . . . . .
H3C H 0.2557 -0.0735 0.7780 0.051 Uiso 1 1 calc R U . . .
H3D H 0.1931 -0.1159 0.8077 0.051 Uiso 1 1 calc R U . . .
N4 N -0.0808(14) 0.6194(14) 0.7935(6) 0.054(5) Uani 1 1 d . U . . .
N5 N 0.2939(15) 0.4895(16) 0.8935(9) 0.079(7) Uani 1 1 d . . . . .
N6 N 1.101(3) 0.303(3) 0.0120(10) 0.145(15) Uani 1 1 d . . . . .
H6C H 1.0868 0.3204 -0.0146 0.174 Uiso 1 1 calc R U . . .
H6D H 1.1679 0.3050 0.0180 0.174 Uiso 1 1 calc R U . . .
Ge1 Ge -0.24833(11) 0.20754(11) 0.84467(5) 0.0134(3) Uani 1 1 d . . . . .
Ge2 Ge -0.12100(11) 0.15373(11) 0.58428(5) 0.0120(3) Uani 1 1 d . . . . .
Mo1 Mo -0.22853(10) -0.07339(10) 0.62353(4) 0.0188(3) Uani 1 1 d . . . . .
Mo2 Mo 0.12941(9) 0.21829(11) 0.61821(4) 0.0217(3) Uani 1 1 d . . . . .
Mo3 Mo -0.37897(10) 0.11363(10) 0.55071(4) 0.0229(3) Uani 1 1 d . . . . .
Mo4 Mo -0.45717(9) 0.10964(10) 0.89321(4) 0.0194(3) Uani 1 1 d . . . . .
Mo5 Mo -0.00530(10) 0.40106(10) 0.56212(4) 0.0202(3) Uani 1 1 d . . . . .
Mo6 Mo -0.07002(9) 0.19655(10) 0.48185(4) 0.0184(3) Uani 1 1 d . . . . .
Mo7 Mo -0.29982(10) 0.28951(11) 0.94310(4) 0.0221(3) Uani 1 1 d . . . . .
Mo8 Mo -0.03435(9) 0.29707(10) 0.80192(4) 0.0187(3) Uani 1 1 d . . . . .
Mo9 Mo -0.22293(10) 0.02654(10) 0.92609(4) 0.0202(3) Uani 1 1 d . . . . .
Mo10 Mo -0.31790(10) 0.29128(11) 0.62497(4) 0.0227(3) Uani 1 1 d . . . . .
Mo11 Mo -0.28057(10) 0.34292(10) 0.52535(4) 0.0206(3) Uani 1 1 d . . . . .
Mo12 Mo -0.48470(10) 0.31363(11) 0.81046(4) 0.0223(3) Uani 1 1 d . . . . .
Mo13 Mo -0.17704(10) -0.04441(10) 0.51103(4) 0.0217(3) Uani 1 1 d . . . . .
Mo14 Mo -0.28502(10) 0.38945(10) 0.76145(4) 0.0202(3) Uani 1 1 d . . . . .
Mo15 Mo 0.00569(9) -0.02148(10) 0.65655(4) 0.0188(3) Uani 1 1 d . . . . .
Mo16 Mo 0.00353(10) 0.13011(10) 0.88222(4) 0.0217(3) Uani 1 1 d . . . . .
Mo17 Mo -0.05456(10) 0.34730(10) 0.66088(4) 0.0217(3) Uani 1 1 d . . . . .
Mo18 Mo -0.06388(10) 0.37669(11) 0.89989(4) 0.0233(3) Uani 1 1 d . . . . .
Mo19 Mo 0.06697(10) 0.00194(10) 0.54448(4) 0.0202(3) Uani 1 1 d . . . . .
Mo20 Mo -0.31706(11) 0.48413(10) 0.85744(5) 0.0245(3) Uani 1 1 d . . . . .
Mo21 Mo -0.18260(10) -0.04742(10) 0.81707(4) 0.0207(3) Uani 1 1 d . . . . .
Mo22 Mo -0.40798(9) 0.04289(11) 0.78120(4) 0.0205(3) Uani 1 1 d . . . . .
Dy1 Dy -0.19164(5) 0.11234(5) 0.71886(2) 0.01969(17) Uani 1 1 d . . . . .
O85 O 0.1214(13) 0.8460(14) 0.9313(6) 0.070(5) Uiso 1 1 d . . . . .
O81 O 0.3863(16) 0.3272(17) 0.9417(7) 0.092(6) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 Mo16 1.898(10) . ?
O1 Mo18 1.981(11) . ?
O2 Mo16 1.844(10) . ?
O2 Mo8 2.087(10) . ?
O3 Ge1 1.772(9) . ?
O3 Mo8 2.250(10) . ?
O3 Mo16 2.274(9) . ?
O3 Mo18 2.308(10) . ?
O4 Mo16 1.919(10) . ?
O4 Mo21 1.950(10) . ?
O5 Mo22 1.950(10) . ?
O5 Mo21 1.976(10) . ?
O6 Mo8 1.725(10) . ?
O6 Dy1 2.372(10) . ?
O7 Mo8 1.851(10) . ?
O7 Mo14 2.023(10) . ?
O8 Mo15 1.740(10) . ?
O8 Dy1 2.384(9) . ?
O9 Mo1 1.743(10) . ?
O9 Dy1 2.430(10) . ?
O10 Ge2 1.732(9) . ?
O10 Mo15 2.180(9) . ?
O10 Mo1 2.180(9) . ?
O11 Mo3 1.873(10) . ?
O11 Mo1 1.959(10) . ?
O12 Mo3 1.868(10) . ?
O12 Mo10 2.012(10) . ?
O13 Mo11 1.926(10) . ?
O13 Mo3 1.952(11) . ?
O14 Mo11 1.692(11) . ?
O15 Mo10 1.869(10) . ?
O15 Mo17 1.968(10) . ?
O16 Ge2 1.747(9) . ?
O16 Mo2 2.240(9) . ?
O16 Mo5 2.312(9) . ?
O16 Mo17 2.329(10) . ?
O17 Ge2 1.754(10) . ?
O17 Mo6 2.253(10) . ?
O17 Mo13 2.327(10) . ?
O17 Mo19 2.334(10) . ?
O18 Mo6 1.791(10) . ?
O18 Mo5 2.099(10) . ?
O19 Mo19 2.097(10) . ?
O19 Mo6 2.107(9) . ?
O20 Mo7 1.930(10) . ?
O20 Mo4 1.977(10) . ?
O21 Mo4 1.675(10) . ?
O22 Mo4 1.784(11) . ?
O22 Mo22 2.157(11) . ?
O23 Mo21 1.727(10) . ?
O24 Mo12 1.789(11) . ?
O24 Mo4 2.080(11) . ?
O25 Ge1 1.729(9) . ?
O25 Mo21 2.186(10) . ?
O25 Mo22 2.194(9) . ?
O26 Mo14 1.863(10) . ?
O26 Mo12 2.041(11) . ?
O27 Ge1 1.771(10) . ?
O27 Mo9 2.272(9) . ?
O27 Mo7 2.279(10) . ?
O27 Mo4 2.298(9) . ?
O28 Mo9 1.834(10) . ?
O28 Mo16 2.032(10) . ?
O29 Mo16 1.701(9) . ?
O30 Mo18 1.800(11) . ?
O30 Mo8 2.157(10) . ?
O31 Mo15 1.921(10) . ?
O31 Mo1 1.951(9) . ?
O32 Mo17 1.728(9) . ?
O32 Dy1 2.387(9) . ?
O33 Mo17 1.697(11) . ?
O34 Mo2 1.858(11) . ?
O34 Mo15 1.956(10) . ?
O35 Mo9 1.774(11) . ?
O35 Mo21 2.171(11) . ?
O36 Mo5 1.930(10) . ?
O36 Mo2 1.961(10) . ?
O37 Mo5 1.680(11) . ?
O38 Mo19 1.757(10) . ?
O38 Mo15 2.187(10) . ?
O39 Mo11 1.785(11) . ?
O39 Mo10 2.165(10) . ?
O40 Mo5 1.765(11) . ?
O40 Mo17 2.206(11) . ?
O41 Mo8 1.676(10) . ?
O42 Mo7 1.815(11) . ?
O42 Mo20 2.043(11) . ?
O43 Mo18 1.907(11) . ?
O43 Mo20 1.908(10) . ?
O44 Mo7 1.697(11) . ?
O45 Mo9 2.039(11) . ?
O45 Mo7 2.099(10) . ?
O46 Mo4 1.851(10) . ?
O46 Mo9 2.044(11) . ?
O47 Ge1 1.750(9) . ?
O47 Mo12 2.265(9) . ?
O47 Mo14 2.327(10) . ?
O47 Mo20 2.338(10) . ?
O48 Mo21 1.745(11) . ?
O48 Dy1 2.356(11) . ?
O49 Mo22 1.754(11) . ?
O49 Dy1 2.385(10) . ?
O50 Mo2 1.933(10) . ?
O50 Mo17 1.935(10) . ?
O51 Mo15 1.691(10) . ?
O52 Mo2 1.903(10) . ?
O52 Mo19 1.955(10) . ?
O53 Mo19 1.677(10) . ?
O54 Mo13 1.773(12) . ?
O54 Mo1 2.187(11) . ?
O55 Mo13 2.058(10) . ?
O55 Mo6 2.103(10) . ?
O56 Mo6 1.791(10) . ?
O56 Mo11 2.140(10) . ?
O57 Mo6 1.675(11) . ?
O58 Ge2 1.743(9) . ?
O58 Mo3 2.257(9) . ?
O58 Mo10 2.308(9) . ?
O58 Mo11 2.310(9) . ?
O59 Mo5 1.906(10) . ?
O59 Mo11 1.917(10) . ?
O60 Mo12 1.682(12) . ?
O61 Mo18 1.673(11) . ?
O62 Mo20 1.695(11) . ?
O63 Mo20 1.820(11) . ?
O63 Mo14 2.139(10) . ?
O64 Mo20 1.890(11) . ?
O64 Mo12 1.986(11) . ?
O65 Mo14 1.691(11) . ?
O66 Mo7 1.858(11) . ?
O66 Mo18 1.993(11) . ?
O67 Mo9 1.703(11) . ?
O68 Mo12 1.916(10) . ?
O68 Mo22 1.929(10) . ?
O69 Mo14 1.744(10) . ?
O69 Dy1 2.334(10) . ?
O70 Mo22 1.708(10) . ?
O71 Mo2 1.690(11) . ?
O72 Mo1 1.687(10) . ?
O73 Mo10 1.700(11) . ?
O73 Dy1 2.428(10) . ?
O74 Mo10 1.679(10) . ?
O75 Mo3 1.694(11) . ?
O76 Mo13 1.875(10) . ?
O76 Mo3 1.974(10) . ?
O77 Mo13 1.699(11) . ?
O78 Mo19 1.873(10) . ?
O78 Mo13 1.999(10) . ?
O79 C12 1.48(2) . ?
O79 C10 1.51(2) . ?
O80 C7 1.46(2) . ?
O80 C5 1.46(2) . ?
O82 C13 1.40(3) . ?
O82 C15 1.41(3) . ?
O84 C22 1.39(3) . ?
O84 C24 1.44(3) . ?
C1 C2 1.46(3) . ?
C1 O85 1.52(3) . ?
C2 N1 1.44(3) . ?
C3 C4 1.47(3) . ?
C3 O85 1.52(2) . ?
C4 N1 1.40(3) . ?
C5 C6 1.54(3) . ?
C6 N3 1.41(3) . ?
C7 C8 1.52(3) . ?
C8 N3 1.38(2) . ?
C9 N2 1.43(3) . ?
C9 C10 1.51(2) . ?
C11 N2 1.44(3) . ?
C11 C12 1.49(3) . ?
C13 C14 1.54(4) . ?
C14 N4 1.33(3) . ?
C15 C16 1.53(3) . ?
C16 N4 1.52(3) . ?
C17 N5 1.41(4) . ?
C17 C18 1.53(4) . ?
C18 O81 1.52(3) . ?
C19 C20 1.39(4) . ?
C19 O81 1.46(3) . ?
C20 N5 1.34(4) . ?
C21 N6 1.53(4) . ?
C21 C22 1.57(4) . ?
C23 C24 1.36(4) . ?
C23 N6 1.45(4) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Mo16 O1 Mo18 118.2(5) . . ?
Mo16 O2 Mo8 117.5(5) . . ?
Ge1 O3 Mo8 119.0(5) . . ?
Ge1 O3 Mo16 122.7(5) . . ?
Mo8 O3 Mo16 96.0(3) . . ?
Ge1 O3 Mo18 122.5(5) . . ?
Mo8 O3 Mo18 96.7(4) . . ?
Mo16 O3 Mo18 93.2(4) . . ?
Mo16 O4 Mo21 160.2(6) . . ?
Mo22 O5 Mo21 113.7(5) . . ?
Mo8 O6 Dy1 153.7(6) . . ?
Mo8 O7 Mo14 138.7(6) . . ?
Mo15 O8 Dy1 138.7(5) . . ?
Mo1 O9 Dy1 136.8(5) . . ?
Ge2 O10 Mo15 128.5(5) . . ?
Ge2 O10 Mo1 127.9(5) . . ?
Mo15 O10 Mo1 95.7(3) . . ?
Mo3 O11 Mo1 159.4(6) . . ?
Mo3 O12 Mo10 119.0(5) . . ?
Mo11 O13 Mo3 118.6(5) . . ?
Mo10 O15 Mo17 141.3(6) . . ?
Ge2 O16 Mo2 120.6(5) . . ?
Ge2 O16 Mo5 124.8(5) . . ?
Mo2 O16 Mo5 94.7(3) . . ?
Ge2 O16 Mo17 120.3(5) . . ?
Mo2 O16 Mo17 94.5(3) . . ?
Mo5 O16 Mo17 94.7(3) . . ?
Ge2 O17 Mo6 121.9(5) . . ?
Ge2 O17 Mo13 117.1(5) . . ?
Mo6 O17 Mo13 101.6(4) . . ?
Ge2 O17 Mo19 117.2(5) . . ?
Mo6 O17 Mo19 102.3(4) . . ?
Mo13 O17 Mo19 91.6(4) . . ?
Mo6 O18 Mo5 145.9(6) . . ?
Mo19 O19 Mo6 116.4(5) . . ?
Mo7 O20 Mo4 120.2(5) . . ?
Mo4 O22 Mo22 157.0(6) . . ?
Mo12 O24 Mo4 148.9(6) . . ?
Ge1 O25 Mo21 126.5(5) . . ?
Ge1 O25 Mo22 125.1(5) . . ?
Mo21 O25 Mo22 97.3(4) . . ?
Mo14 O26 Mo12 119.1(5) . . ?
Ge1 O27 Mo9 119.3(5) . . ?
Ge1 O27 Mo7 119.2(5) . . ?
Mo9 O27 Mo7 102.9(4) . . ?
Ge1 O27 Mo4 120.9(5) . . ?
Mo9 O27 Mo4 93.8(3) . . ?
Mo7 O27 Mo4 95.5(4) . . ?
Mo9 O28 Mo16 145.6(6) . . ?
Mo18 O30 Mo8 118.5(5) . . ?
Mo15 O31 Mo1 113.2(5) . . ?
Mo17 O32 Dy1 161.7(6) . . ?
Mo2 O34 Mo15 157.2(6) . . ?
Mo9 O35 Mo21 144.6(6) . . ?
Mo5 O36 Mo2 118.7(5) . . ?
Mo19 O38 Mo15 152.0(6) . . ?
Mo11 O39 Mo10 118.0(5) . . ?
Mo5 O40 Mo17 118.1(5) . . ?
Mo7 O42 Mo20 148.8(6) . . ?
Mo18 O43 Mo20 156.9(6) . . ?
Mo9 O45 Mo7 118.6(5) . . ?
Mo4 O46 Mo9 117.8(5) . . ?
Ge1 O47 Mo12 119.3(5) . . ?
Ge1 O47 Mo14 120.7(5) . . ?
Mo12 O47 Mo14 94.3(4) . . ?
Ge1 O47 Mo20 127.2(5) . . ?
Mo12 O47 Mo20 93.4(3) . . ?
Mo14 O47 Mo20 94.1(3) . . ?
Mo21 O48 Dy1 133.6(5) . . ?
Mo22 O49 Dy1 131.4(5) . . ?
Mo2 O50 Mo17 120.3(5) . . ?
Mo2 O52 Mo19 145.7(6) . . ?
Mo13 O54 Mo1 148.2(6) . . ?
Mo13 O55 Mo6 117.1(5) . . ?
Mo6 O56 Mo11 144.9(5) . . ?
Ge2 O58 Mo3 121.7(5) . . ?
Ge2 O58 Mo10 119.5(5) . . ?
Mo3 O58 Mo10 94.2(3) . . ?
Ge2 O58 Mo11 125.5(5) . . ?
Mo3 O58 Mo11 93.8(3) . . ?
Mo10 O58 Mo11 94.6(3) . . ?
Mo5 O59 Mo11 162.4(6) . . ?
Mo20 O63 Mo14 118.9(5) . . ?
Mo20 O64 Mo12 119.6(5) . . ?
Mo7 O66 Mo18 150.5(6) . . ?
Mo12 O68 Mo22 153.7(6) . . ?
Mo14 O69 Dy1 162.5(6) . . ?
Mo10 O73 Dy1 153.9(6) . . ?
Mo13 O76 Mo3 146.3(6) . . ?
Mo19 O78 Mo13 119.3(5) . . ?
C12 O79 C10 113.1(14) . . ?
C7 O80 C5 113.3(14) . . ?
C13 O82 C15 106(2) . . ?
C22 O84 C24 101(2) . . ?
C2 C1 O85 109.3(19) . . ?
N1 C2 C1 110.1(18) . . ?
C4 C3 O85 108.0(15) . . ?
N1 C4 C3 113.3(17) . . ?
O80 C5 C6 107.7(15) . . ?
N3 C6 C5 109(2) . . ?
O80 C7 C8 108.4(16) . . ?
N3 C8 C7 113.6(16) . . ?
N2 C9 C10 108.9(16) . . ?
C9 C10 O79 109.1(14) . . ?
N2 C11 C12 110.9(17) . . ?
O79 C12 C11 111.5(17) . . ?
O82 C13 C14 110(2) . . ?
N4 C14 C13 111(2) . . ?
O82 C15 C16 110(2) . . ?
N4 C16 C15 108(2) . . ?
N5 C17 C18 115(3) . . ?
O81 C18 C17 107(2) . . ?
C20 C19 O81 114(3) . . ?
N5 C20 C19 115(3) . . ?
N6 C21 C22 109(2) . . ?
O84 C22 C21 112(2) . . ?
C24 C23 N6 107(2) . . ?
C23 C24 O84 114(3) . . ?
C4 N1 C2 106.8(17) . . ?
C9 N2 C11 115.8(16) . . ?
C8 N3 C6 110.9(17) . . ?
C14 N4 C16 106(2) . . ?
C20 N5 C17 113(3) . . ?
C23 N6 C21 113(2) . . ?
O25 Ge1 O47 112.6(5) . . ?
O25 Ge1 O27 108.6(5) . . ?
O47 Ge1 O27 109.9(5) . . ?
O25 Ge1 O3 110.5(4) . . ?
O47 Ge1 O3 106.5(5) . . ?
O27 Ge1 O3 108.7(4) . . ?
O10 Ge2 O58 111.2(5) . . ?
O10 Ge2 O16 111.0(4) . . ?
O58 Ge2 O16 107.7(4) . . ?
O10 Ge2 O17 109.9(5) . . ?
O58 Ge2 O17 108.4(4) . . ?
O16 Ge2 O17 108.5(5) . . ?
O72 Mo1 O9 103.2(5) . . ?
O72 Mo1 O31 97.0(5) . . ?
O9 Mo1 O31 95.8(5) . . ?
O72 Mo1 O11 99.9(5) . . ?
O9 Mo1 O11 97.7(5) . . ?
O31 Mo1 O11 155.3(4) . . ?
O72 Mo1 O10 166.8(5) . . ?
O9 Mo1 O10 87.2(4) . . ?
O31 Mo1 O10 73.6(4) . . ?
O11 Mo1 O10 86.6(4) . . ?
O72 Mo1 O54 89.8(5) . . ?
O9 Mo1 O54 167.0(4) . . ?
O31 Mo1 O54 83.8(4) . . ?
O11 Mo1 O54 78.4(4) . . ?
O10 Mo1 O54 80.2(4) . . ?
O71 Mo2 O34 103.6(5) . . ?
O71 Mo2 O52 102.0(5) . . ?
O34 Mo2 O52 88.6(5) . . ?
O71 Mo2 O50 98.2(5) . . ?
O34 Mo2 O50 90.1(4) . . ?
O52 Mo2 O50 159.5(4) . . ?
O71 Mo2 O36 96.9(5) . . ?
O34 Mo2 O36 159.5(4) . . ?
O52 Mo2 O36 87.1(4) . . ?
O50 Mo2 O36 87.0(4) . . ?
O71 Mo2 O16 167.3(5) . . ?
O34 Mo2 O16 86.0(4) . . ?
O52 Mo2 O16 86.4(4) . . ?
O50 Mo2 O16 73.1(4) . . ?
O36 Mo2 O16 73.7(4) . . ?
O75 Mo3 O12 101.5(5) . . ?
O75 Mo3 O11 103.7(5) . . ?
O12 Mo3 O11 92.8(5) . . ?
O75 Mo3 O13 97.4(5) . . ?
O12 Mo3 O13 90.4(5) . . ?
O11 Mo3 O13 157.6(4) . . ?
O75 Mo3 O76 97.8(5) . . ?
O12 Mo3 O76 160.6(4) . . ?
O11 Mo3 O76 84.9(4) . . ?
O13 Mo3 O76 84.8(4) . . ?
O75 Mo3 O58 170.1(5) . . ?
O12 Mo3 O58 74.8(4) . . ?
O11 Mo3 O58 85.7(4) . . ?
O13 Mo3 O58 73.7(4) . . ?
O76 Mo3 O58 85.8(4) . . ?
O21 Mo4 O22 102.9(5) . . ?
O21 Mo4 O46 103.9(5) . . ?
O22 Mo4 O46 96.5(5) . . ?
O21 Mo4 O20 99.1(5) . . ?
O22 Mo4 O20 154.1(5) . . ?
O46 Mo4 O20 91.2(5) . . ?
O21 Mo4 O24 97.6(5) . . ?
O22 Mo4 O24 83.3(4) . . ?
O46 Mo4 O24 158.0(4) . . ?
O20 Mo4 O24 80.5(4) . . ?
O21 Mo4 O27 170.5(5) . . ?
O22 Mo4 O27 86.6(4) . . ?
O46 Mo4 O27 75.3(4) . . ?
O20 Mo4 O27 71.5(4) . . ?
O24 Mo4 O27 82.7(4) . . ?
O37 Mo5 O40 103.6(5) . . ?
O37 Mo5 O59 102.3(5) . . ?
O40 Mo5 O59 96.2(5) . . ?
O37 Mo5 O36 99.2(5) . . ?
O40 Mo5 O36 93.7(5) . . ?
O59 Mo5 O36 153.5(4) . . ?
O37 Mo5 O18 96.2(5) . . ?
O40 Mo5 O18 160.2(4) . . ?
O59 Mo5 O18 80.8(4) . . ?
O36 Mo5 O18 81.7(4) . . ?
O37 Mo5 O16 171.8(5) . . ?
O40 Mo5 O16 77.6(4) . . ?
O59 Mo5 O16 85.6(4) . . ?
O36 Mo5 O16 72.6(4) . . ?
O18 Mo5 O16 82.7(4) . . ?
O57 Mo6 O56 105.6(5) . . ?
O57 Mo6 O18 105.1(5) . . ?
O56 Mo6 O18 96.2(5) . . ?
O57 Mo6 O55 94.6(5) . . ?
O56 Mo6 O55 87.3(4) . . ?
O18 Mo6 O55 158.2(4) . . ?
O57 Mo6 O19 92.7(5) . . ?
O56 Mo6 O19 159.9(4) . . ?
O18 Mo6 O19 86.8(4) . . ?
O55 Mo6 O19 82.9(4) . . ?
O57 Mo6 O17 159.2(5) . . ?
O56 Mo6 O17 88.9(4) . . ?
O18 Mo6 O17 87.6(4) . . ?
O55 Mo6 O17 70.9(4) . . ?
O19 Mo6 O17 71.3(4) . . ?
O44 Mo7 O42 103.3(5) . . ?
O44 Mo7 O66 104.8(5) . . ?
O42 Mo7 O66 90.1(5) . . ?
O44 Mo7 O20 97.7(5) . . ?
O42 Mo7 O20 94.1(5) . . ?
O66 Mo7 O20 155.5(4) . . ?
O44 Mo7 O45 94.6(5) . . ?
O42 Mo7 O45 162.1(5) . . ?
O66 Mo7 O45 84.4(4) . . ?
O20 Mo7 O45 84.3(4) . . ?
O44 Mo7 O27 161.0(5) . . ?
O42 Mo7 O27 93.8(4) . . ?
O66 Mo7 O27 82.9(4) . . ?
O20 Mo7 O27 72.7(4) . . ?
O45 Mo7 O27 68.6(4) . . ?
O41 Mo8 O6 104.1(5) . . ?
O41 Mo8 O7 105.0(5) . . ?
O6 Mo8 O7 98.5(5) . . ?
O41 Mo8 O2 92.2(5) . . ?
O6 Mo8 O2 90.2(4) . . ?
O7 Mo8 O2 158.1(5) . . ?
O41 Mo8 O30 92.8(5) . . ?
O6 Mo8 O30 160.6(4) . . ?
O7 Mo8 O30 86.0(5) . . ?
O2 Mo8 O30 79.5(4) . . ?
O41 Mo8 O3 157.5(5) . . ?
O6 Mo8 O3 91.4(4) . . ?
O7 Mo8 O3 88.5(4) . . ?
O2 Mo8 O3 71.2(4) . . ?
O30 Mo8 O3 69.8(4) . . ?
O67 Mo9 O35 103.7(5) . . ?
O67 Mo9 O28 104.4(5) . . ?
O35 Mo9 O28 96.6(5) . . ?
O67 Mo9 O45 96.7(5) . . ?
O35 Mo9 O45 157.6(4) . . ?
O28 Mo9 O45 87.0(4) . . ?
O67 Mo9 O46 93.3(5) . . ?
O35 Mo9 O46 87.2(5) . . ?
O28 Mo9 O46 160.3(4) . . ?
O45 Mo9 O46 82.5(4) . . ?
O67 Mo9 O27 161.1(5) . . ?
O35 Mo9 O27 88.2(4) . . ?
O28 Mo9 O27 88.3(4) . . ?
O45 Mo9 O27 69.7(4) . . ?
O46 Mo9 O27 72.5(4) . . ?
O74 Mo10 O73 104.2(5) . . ?
O74 Mo10 O15 105.1(5) . . ?
O73 Mo10 O15 97.0(5) . . ?
O74 Mo10 O12 95.7(5) . . ?
O73 Mo10 O12 92.5(5) . . ?
O15 Mo10 O12 154.2(5) . . ?
O74 Mo10 O39 91.6(5) . . ?
O73 Mo10 O39 163.5(4) . . ?
O15 Mo10 O39 83.1(4) . . ?
O12 Mo10 O39 81.1(4) . . ?
O74 Mo10 O58 158.8(5) . . ?
O73 Mo10 O58 93.2(4) . . ?
O15 Mo10 O58 84.3(4) . . ?
O12 Mo10 O58 71.2(4) . . ?
O39 Mo10 O58 70.4(4) . . ?
O14 Mo11 O39 104.2(5) . . ?
O14 Mo11 O59 100.5(5) . . ?
O39 Mo11 O59 95.9(4) . . ?
O14 Mo11 O13 101.0(5) . . ?
O39 Mo11 O13 95.4(5) . . ?
O59 Mo11 O13 152.3(4) . . ?
O14 Mo11 O56 95.2(5) . . ?
O39 Mo11 O56 160.6(4) . . ?
O59 Mo11 O56 79.7(4) . . ?
O13 Mo11 O56 81.3(4) . . ?
O14 Mo11 O58 174.0(5) . . ?
O39 Mo11 O58 77.0(4) . . ?
O59 Mo11 O58 85.2(4) . . ?
O13 Mo11 O58 72.9(4) . . ?
O56 Mo11 O58 83.8(4) . . ?
O60 Mo12 O24 103.2(6) . . ?
O60 Mo12 O68 103.0(5) . . ?
O24 Mo12 O68 90.0(5) . . ?
O60 Mo12 O64 97.6(5) . . ?
O24 Mo12 O64 93.3(5) . . ?
O68 Mo12 O64 157.8(4) . . ?
O60 Mo12 O26 96.1(5) . . ?
O24 Mo12 O26 160.7(4) . . ?
O68 Mo12 O26 85.7(4) . . ?
O64 Mo12 O26 84.0(5) . . ?
O60 Mo12 O47 165.8(5) . . ?
O24 Mo12 O47 88.7(4) . . ?
O68 Mo12 O47 84.6(4) . . ?
O64 Mo12 O47 73.5(4) . . ?
O26 Mo12 O47 72.2(4) . . ?
O77 Mo13 O54 104.9(5) . . ?
O77 Mo13 O76 103.9(5) . . ?
O54 Mo13 O76 93.3(5) . . ?
O77 Mo13 O78 97.3(5) . . ?
O54 Mo13 O78 92.0(5) . . ?
O76 Mo13 O78 155.9(4) . . ?
O77 Mo13 O55 94.9(5) . . ?
O54 Mo13 O55 159.9(4) . . ?
O76 Mo13 O55 84.6(4) . . ?
O78 Mo13 O55 82.4(4) . . ?
O77 Mo13 O17 162.4(5) . . ?
O54 Mo13 O17 89.8(4) . . ?
O76 Mo13 O17 84.4(4) . . ?
O78 Mo13 O17 72.1(4) . . ?
O55 Mo13 O17 70.1(4) . . ?
O65 Mo14 O69 105.4(5) . . ?
O65 Mo14 O26 101.5(5) . . ?
O69 Mo14 O26 99.1(5) . . ?
O65 Mo14 O7 98.4(5) . . ?
O69 Mo14 O7 90.6(5) . . ?
O26 Mo14 O7 154.6(5) . . ?
O65 Mo14 O63 91.6(5) . . ?
O69 Mo14 O63 160.9(5) . . ?
O26 Mo14 O63 85.6(4) . . ?
O7 Mo14 O63 78.3(4) . . ?
O65 Mo14 O47 161.9(5) . . ?
O69 Mo14 O47 92.6(4) . . ?
O26 Mo14 O47 73.8(4) . . ?
O7 Mo14 O47 82.4(4) . . ?
O63 Mo14 O47 70.8(4) . . ?
O51 Mo15 O8 103.2(5) . . ?
O51 Mo15 O31 97.6(5) . . ?
O8 Mo15 O31 97.5(5) . . ?
O51 Mo15 O34 99.0(5) . . ?
O8 Mo15 O34 96.8(5) . . ?
O31 Mo15 O34 155.0(4) . . ?
O51 Mo15 O10 168.3(5) . . ?
O8 Mo15 O10 86.3(4) . . ?
O31 Mo15 O10 74.1(4) . . ?
O34 Mo15 O10 86.4(4) . . ?
O51 Mo15 O38 92.1(5) . . ?
O8 Mo15 O38 164.6(4) . . ?
O31 Mo15 O38 82.4(4) . . ?
O34 Mo15 O38 78.4(4) . . ?
O10 Mo15 O38 78.8(4) . . ?
O29 Mo16 O2 101.7(5) . . ?
O29 Mo16 O1 100.7(5) . . ?
O2 Mo16 O1 92.5(5) . . ?
O29 Mo16 O4 100.8(5) . . ?
O2 Mo16 O4 93.3(5) . . ?
O1 Mo16 O4 156.0(4) . . ?
O29 Mo16 O28 96.5(5) . . ?
O2 Mo16 O28 161.8(4) . . ?
O1 Mo16 O28 84.7(4) . . ?
O4 Mo16 O28 82.5(4) . . ?
O29 Mo16 O3 174.4(5) . . ?
O2 Mo16 O3 74.9(4) . . ?
O1 Mo16 O3 75.2(4) . . ?
O4 Mo16 O3 84.0(4) . . ?
O28 Mo16 O3 87.0(4) . . ?
O33 Mo17 O32 105.0(5) . . ?
O33 Mo17 O50 100.2(5) . . ?
O32 Mo17 O50 98.6(4) . . ?
O33 Mo17 O15 102.2(5) . . ?
O32 Mo17 O15 90.5(5) . . ?
O50 Mo17 O15 152.6(4) . . ?
O33 Mo17 O40 92.0(5) . . ?
O32 Mo17 O40 162.6(4) . . ?
O50 Mo17 O40 81.4(4) . . ?
O15 Mo17 O40 82.3(4) . . ?
O33 Mo17 O16 160.3(5) . . ?
O32 Mo17 O16 93.9(4) . . ?
O50 Mo17 O16 71.0(4) . . ?
O15 Mo17 O16 82.7(4) . . ?
O40 Mo17 O16 69.6(4) . . ?
O61 Mo18 O30 104.1(6) . . ?
O61 Mo18 O43 103.3(5) . . ?
O30 Mo18 O43 93.2(5) . . ?
O61 Mo18 O1 95.9(5) . . ?
O30 Mo18 O1 90.9(5) . . ?
O43 Mo18 O1 158.8(4) . . ?
O61 Mo18 O66 99.0(5) . . ?
O30 Mo18 O66 156.9(4) . . ?
O43 Mo18 O66 82.9(5) . . ?
O1 Mo18 O66 85.1(4) . . ?
O61 Mo18 O3 168.6(5) . . ?
O30 Mo18 O3 74.6(4) . . ?
O43 Mo18 O3 88.1(4) . . ?
O1 Mo18 O3 72.9(4) . . ?
O66 Mo18 O3 82.5(4) . . ?
O53 Mo19 O38 103.6(5) . . ?
O53 Mo19 O78 100.9(5) . . ?
O38 Mo19 O78 97.2(5) . . ?
O53 Mo19 O52 100.9(5) . . ?
O38 Mo19 O52 90.3(5) . . ?
O78 Mo19 O52 154.6(4) . . ?
O53 Mo19 O19 96.7(5) . . ?
O38 Mo19 O19 159.0(4) . . ?
O78 Mo19 O19 83.7(4) . . ?
O52 Mo19 O19 80.7(4) . . ?
O53 Mo19 O17 165.9(4) . . ?
O38 Mo19 O17 90.2(4) . . ?
O78 Mo19 O17 74.0(4) . . ?
O52 Mo19 O17 81.7(4) . . ?
O19 Mo19 O17 69.9(4) . . ?
O62 Mo20 O63 103.4(6) . . ?
O62 Mo20 O64 100.1(5) . . ?
O63 Mo20 O64 92.8(5) . . ?
O62 Mo20 O43 100.9(5) . . ?
O63 Mo20 O43 93.4(5) . . ?
O64 Mo20 O43 156.0(5) . . ?
O62 Mo20 O42 98.2(6) . . ?
O63 Mo20 O42 158.4(4) . . ?
O64 Mo20 O42 83.9(5) . . ?
O43 Mo20 O42 81.9(4) . . ?
O62 Mo20 O47 173.5(5) . . ?
O63 Mo20 O47 76.0(4) . . ?
O64 Mo20 O47 73.5(4) . . ?
O43 Mo20 O47 85.6(4) . . ?
O42 Mo20 O47 82.6(4) . . ?
O23 Mo21 O48 103.0(5) . . ?
O23 Mo21 O4 100.5(4) . . ?
O48 Mo21 O4 98.6(4) . . ?
O23 Mo21 O5 97.3(5) . . ?
O48 Mo21 O5 94.7(4) . . ?
O4 Mo21 O5 154.7(4) . . ?
O23 Mo21 O35 89.4(5) . . ?
O48 Mo21 O35 167.4(4) . . ?
O4 Mo21 O35 80.5(4) . . ?
O5 Mo21 O35 81.8(4) . . ?
O23 Mo21 O25 168.1(5) . . ?
O48 Mo21 O25 85.1(4) . . ?
O4 Mo21 O25 86.7(4) . . ?
O5 Mo21 O25 73.1(4) . . ?
O35 Mo21 O25 82.3(4) . . ?
O70 Mo22 O49 101.9(5) . . ?
O70 Mo22 O68 100.0(5) . . ?
O49 Mo22 O68 95.6(5) . . ?
O70 Mo22 O5 97.2(5) . . ?
O49 Mo22 O5 97.2(5) . . ?
O68 Mo22 O5 155.9(4) . . ?
O70 Mo22 O22 91.1(5) . . ?
O49 Mo22 O22 166.6(4) . . ?
O68 Mo22 O22 79.1(4) . . ?
O5 Mo22 O22 83.8(4) . . ?
O70 Mo22 O25 168.4(5) . . ?
O49 Mo22 O25 86.3(4) . . ?
O68 Mo22 O25 87.2(4) . . ?
O5 Mo22 O25 73.4(4) . . ?
O22 Mo22 O25 81.2(4) . . ?
O69 Dy1 O48 119.2(4) . . ?
O69 Dy1 O6 70.9(4) . . ?
O48 Dy1 O6 76.8(4) . . ?
O69 Dy1 O8 149.5(4) . . ?
O48 Dy1 O8 71.9(3) . . ?
O6 Dy1 O8 85.8(3) . . ?
O69 Dy1 O49 75.6(4) . . ?
O48 Dy1 O49 77.0(4) . . ?
O6 Dy1 O49 118.8(4) . . ?
O8 Dy1 O49 134.2(4) . . ?
O69 Dy1 O32 81.3(4) . . ?
O48 Dy1 O32 134.0(3) . . ?
O6 Dy1 O32 72.1(4) . . ?
O8 Dy1 O32 72.8(4) . . ?
O49 Dy1 O32 148.3(4) . . ?
O69 Dy1 O73 72.0(3) . . ?
O48 Dy1 O73 153.0(4) . . ?
O6 Dy1 O73 129.3(3) . . ?
O8 Dy1 O73 111.9(3) . . ?
O49 Dy1 O73 83.0(4) . . ?
O32 Dy1 O73 69.3(4) . . ?
O69 Dy1 O9 132.8(4) . . ?
O48 Dy1 O9 84.1(3) . . ?
O6 Dy1 O9 155.5(3) . . ?
O8 Dy1 O9 73.7(3) . . ?
O49 Dy1 O9 70.4(3) . . ?
O32 Dy1 O9 112.9(3) . . ?
O73 Dy1 O9 72.2(3) . . ?
C1 O85 C3 108.2(15) . . ?
C19 O81 C18 115(2) . . ?

_refine_diff_density_max         1.368
_refine_diff_density_min         -1.399
_refine_diff_density_rms         0.176

_shelxl_version_number           2014-3


_vrf_CHEMW03_3_sq                
;
CHEMW03_ALERT_2_A

RESPONSE: Use of Platon SQUEEZE to remove disordered solvent. The accessible
solvent void in the crystal structure indicates that some more water molecules
and morpholine should exist in the structure, but cannot be found from the
weak residual electron peaks. Based on the TG analyses and elemental analysis,
15 water molecules and 8 morpholine were included in the sum formula.
;
_vrf_PLAT342_3_sq                
;
PLAT342_ALERT_3_B Low Bond Precision on C-C Bonds .............. 0.03583 Ang.

RESPONSE: The low bond distance precision is likely due to the low data to
parameter ratio. There is a large amount of disorder in the structure. This is
common in high nuclearity polyoxometalate cluster . (such as Angew. Chem. Int.
Ed, 2010, 49, 6984; Angew. Chem. Int. Ed, 2008, 47, 6881, J. Am. Chem. Soc,
2004, 126, 13880.)
;
_vrf_PLAT430_3_sq                
;
PLAT430_ALERT_2_B Short Inter D...A Contact O13...O855 ......2.81 Ang.

RESPONSE: The structure contains a high degree of disorder.
;

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_4_sq
_database_code_depnum_ccdc_archive 'CCDC 991335'
_audit_update_record             
;
2017-10-04 deposited with the CCDC.
2017-10-09 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014
_chemical_name_systematic        
;
 ?
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C32 H113 Ge2 Mo22 N8 O100 Tb'
_chemical_formula_weight         4625.08

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tb Tb -0.1723 4.1537 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           7
_space_group_name_H-M_alt        'P n'
_space_group_name_Hall           'P -2yac'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'x+1/2, -y, z+1/2'

_cell_length_a                   13.2174(6)
_cell_length_b                   12.7175(6)
_cell_length_c                   32.4095(14)
_cell_angle_alpha                90
_cell_angle_beta                 96.294(4)
_cell_angle_gamma                90
_cell_volume                     5414.9(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    11230
_cell_measurement_theta_min      3.0900
_cell_measurement_theta_max      29.2409

_exptl_crystal_description       block
_exptl_crystal_colour            green
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.837
_exptl_crystal_F_000             4428
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.46
_exptl_crystal_size_mid          0.35
_exptl_crystal_size_min          0.30
_exptl_absorpt_coefficient_mu    3.768
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.74450
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_process_details   ?

_exptl_special_details           
;
 ?
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'Enhance (Mo) X-ray Source'
_diffrn_measurement_device_type  'Xcalibur, Ruby, Gemini ultra'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            19326
_diffrn_reflns_av_unetI/netI     0.0503
_diffrn_reflns_av_R_equivalents  0.0297
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -38
_diffrn_reflns_limit_l_max       38
_diffrn_reflns_theta_min         3.101
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measured_fraction_theta_full 0.969
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_Laue_measured_fraction_full 0.969
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_point_group_measured_fraction_full 0.970
_reflns_number_total             13826
_reflns_number_gt                13310
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.999
_reflns_Friedel_fraction_max     0.996
_reflns_Friedel_fraction_full    0.970

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_cell_refinement       
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction        
;
CrysAlisPro, Oxford Diffraction Ltd.,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  SHELXTL

_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0640P)²+2.8297P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.574(11)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         13826
_refine_ls_number_parameters     1307
_refine_ls_number_restraints     102
_refine_ls_R_factor_all          0.0382
_refine_ls_R_factor_gt           0.0363
_refine_ls_wR_factor_ref         0.0977
_refine_ls_wR_factor_gt          0.0962
_refine_ls_goodness_of_fit_ref   1.023
_refine_ls_restrained_S_all      9.733
_refine_ls_shift/su_max          0.008
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
O1 O 0.7511(7) 0.9415(7) 0.6403(3) 0.0152(19) Uani 1 1 d . . . . .
O2 O 0.5472(7) 0.9846(7) 0.6085(3) 0.022(2) Uani 1 1 d . . . . .
O3 O 0.4969(7) 0.7674(7) 0.5308(3) 0.023(2) Uani 1 1 d . . . . .
O4 O 0.5362(7) 0.6124(7) 0.5877(3) 0.023(2) Uani 1 1 d . . . . .
O5 O 0.9348(7) 0.9014(7) 0.5101(3) 0.021(2) Uani 1 1 d D . . . .
O6 O 0.6801(8) 0.6346(7) 0.6535(3) 0.024(2) Uani 1 1 d . . . . .
O7 O 0.8368(7) 0.7459(7) 0.6191(3) 0.0157(19) Uani 1 1 d . . . . .
O8 O 0.7898(7) 0.9015(7) 0.5576(3) 0.018(2) Uani 1 1 d . . . . .
O9 O 0.8746(7) 0.7085(8) 0.5333(3) 0.024(2) Uani 1 1 d . . . . .
O10 O 0.7349(7) 0.6106(8) 0.8054(3) 0.023(2) Uani 1 1 d . . . . .
O11 O 0.9994(7) 0.6590(7) 0.5990(3) 0.021(2) Uani 1 1 d . . . . .
O12 O 0.9589(7) 0.8962(7) 0.6659(3) 0.018(2) Uani 1 1 d . . . . .
O13 O 0.7806(7) 1.1305(7) 0.6593(3) 0.018(2) Uani 1 1 d . . . . .
O14 O 0.5544(8) 0.5685(8) 0.5067(3) 0.030(2) Uani 1 1 d . . . . .
O15 O 0.6345(7) 0.7880(7) 0.5927(3) 0.0160(19) Uani 1 1 d . U . . .
O16 O 0.3848(8) 0.9408(9) 0.5497(3) 0.033(3) Uani 1 1 d . . . . .
O17 O 0.6201(8) 1.0302(7) 0.6906(3) 0.022(2) Uani 1 1 d . . . . .
O18 O 0.8308(7) 0.9783(7) 0.7194(3) 0.020(2) Uani 1 1 d . . . . .
O19 O 0.7841(7) 0.7621(8) 0.7060(3) 0.024(2) Uani 1 1 d . . . . .
O20 O 0.7940(7) 0.8079(8) 0.7902(3) 0.022(2) Uani 1 1 d . . . . .
O21 O 0.9150(7) 1.0457(7) 0.6114(3) 0.019(2) Uani 1 1 d . . . . .
O22 O 0.6499(8) 1.1413(8) 0.4974(3) 0.031(2) Uani 1 1 d . . . . .
O23 O 0.4513(7) 0.7970(8) 0.6091(3) 0.024(2) Uani 1 1 d . . . . .
O24 O 0.9384(8) 0.6594(8) 0.7968(3) 0.029(2) Uani 1 1 d . . . . .
O25 O 0.5181(7) 0.9413(7) 0.7529(3) 0.020(2) Uani 1 1 d . . . . .
O26 O 0.8768(8) 0.6047(8) 0.8740(3) 0.028(2) Uani 1 1 d . . . . .
O27 O 0.9319(7) 0.8051(7) 0.8584(3) 0.021(2) Uani 1 1 d . . . . .
O28 O 0.7191(7) 1.0268(7) 0.7855(3) 0.021(2) Uani 1 1 d . . . . .
O29 O 0.7549(7) 0.7570(7) 0.8731(3) 0.0158(19) Uani 1 1 d . . . . .
O30 O 0.6947(7) 0.5424(7) 0.8965(3) 0.023(2) Uani 1 1 d . . . . .
O31 O 0.6806(7) 0.7481(8) 0.5060(3) 0.020(2) Uani 1 1 d . . . . .
O32 O 0.5848(7) 0.9561(7) 0.5329(3) 0.020(2) Uani 1 1 d . . . . .
O33 O 0.8298(8) 0.7719(8) 0.4520(3) 0.032(2) Uani 1 1 d . . . . .
O34 O 0.9934(7) 0.8675(7) 0.5888(3) 0.019(2) Uani 1 1 d . . . . .
O35 O 0.9608(7) 0.6856(8) 0.6778(3) 0.024(2) Uani 1 1 d . . . . .
O36 O 0.8519(8) 0.5449(7) 0.6296(3) 0.025(2) Uani 1 1 d . . . . .
O37 O 0.7253(7) 0.6052(7) 0.5613(3) 0.019(2) Uani 1 1 d . . . . .
O38 O 0.7302(8) 1.1748(8) 0.8454(3) 0.031(2) Uani 1 1 d . . . . .
O39 O 0.5468(7) 1.0789(7) 0.8193(3) 0.019(2) Uani 1 1 d . . . . .
O40 O 0.6124(6) 0.8958(7) 0.8293(3) 0.0142(19) Uani 1 1 d . . . . .
O41 O 0.7305(8) 0.9445(7) 0.4822(3) 0.024(2) Uani 1 1 d D . . . .
O42 O 0.6911(7) 1.0936(7) 0.5798(3) 0.024(2) Uani 1 1 d . . . . .
O43 O 0.8442(7) 1.0792(7) 0.5302(3) 0.021(2) Uani 1 1 d . . . . .
O44 O 0.4133(7) 0.8168(7) 0.8014(3) 0.021(2) Uani 1 1 d . . . . .
O45 O 0.4292(7) 0.9495(8) 0.8627(3) 0.026(2) Uani 1 1 d . . . . .
O46 O 0.5986(9) 0.5259(9) 0.7410(3) 0.035(3) Uani 1 1 d . . . . .
O47 O 0.2653(8) 0.6648(9) 0.8122(3) 0.032(3) Uani 1 1 d . . . . .
O48 O 0.5596(7) 0.6812(7) 0.8439(3) 0.0157(19) Uani 1 1 d . . . . .
O49 O 0.3818(7) 0.7573(7) 0.8768(3) 0.023(2) Uani 1 1 d . . . . .
O50 O 0.5863(8) 0.4850(7) 0.8247(3) 0.025(2) Uani 1 1 d . . . . .
O51 O 0.9762(8) 0.9428(9) 0.9213(3) 0.032(2) Uani 1 1 d . . . . .
O52 O 0.8033(7) 0.9716(7) 0.8645(3) 0.022(2) Uani 1 1 d . . . . .
O53 O 0.7765(7) 0.9165(7) 0.9397(3) 0.020(2) Uani 1 1 d . . . . .
O54 O 0.8678(8) 0.5421(9) 0.9547(3) 0.032(2) Uani 1 1 d . . . . .
O55 O 0.9779(7) 1.1004(8) 0.6937(3) 0.028(2) Uani 1 1 d . . . . .
O56 O 0.6283(8) 0.8575(8) 0.9862(3) 0.026(2) Uani 1 1 d D . . . .
O57 O 0.4946(8) 0.9872(8) 0.9434(3) 0.027(2) Uani 1 1 d D . . . .
O58 O 0.5802(7) 0.8316(7) 0.9098(3) 0.019(2) Uani 1 1 d . . . . .
O59 O 0.2974(7) 0.9213(9) 0.9203(3) 0.031(2) Uani 1 1 d D . . . .
O60 O 0.4441(7) 0.7833(8) 0.9551(3) 0.027(2) Uani 1 1 d D . . . .
O61 O 0.5395(9) 0.3962(8) 0.8970(3) 0.036(3) Uani 1 1 d . . . . .
O62 O 0.4182(8) 0.5512(8) 0.8575(3) 0.026(2) Uani 1 1 d . . . . .
O63 O 0.5317(8) 0.6072(7) 0.9257(3) 0.026(2) Uani 1 1 d . . . . .
O64 O 0.6738(8) 1.0689(8) 0.9804(3) 0.027(2) Uani 1 1 d . . . . .
O65 O 0.6399(8) 1.0418(8) 0.8968(3) 0.025(2) Uani 1 1 d . . . . .
O66 O 0.5647(8) 0.6604(8) 1.0086(3) 0.027(2) Uani 1 1 d . . . . .
O67 O 0.7079(7) 0.6869(7) 0.9525(3) 0.024(2) Uani 1 1 d . . . . .
O68 O 0.8938(7) 0.7501(8) 0.9351(3) 0.025(2) Uani 1 1 d . . . . .
O69 O 0.6073(8) 0.7347(8) 0.7597(3) 0.023(2) Uani 1 1 d . . . . .
O70 O 0.4472(7) 0.6139(8) 0.7812(3) 0.024(2) Uani 1 1 d . . . . .
O71 O 0.9073(9) 0.4960(8) 0.5539(3) 0.031(2) Uani 1 1 d . . . . .
O72 O 1.0495(7) 1.0614(9) 0.5543(3) 0.029(2) Uani 1 1 d D . . . .
O73 O 1.1310(7) 0.7791(8) 0.6513(3) 0.028(2) Uani 1 1 d . . . . .
O74 O 0.8285(9) 0.5547(8) 0.7142(3) 0.033(3) Uani 1 1 d . . . . .
O75 O 0.5820(8) 1.1888(8) 0.6365(3) 0.033(3) Uani 1 1 d . . . . .
O76 O 0.3551(8) 1.0245(8) 0.7854(3) 0.031(2) Uani 1 1 d . . . . .
O77 O 0.5876(8) 0.8078(8) 0.6780(3) 0.023(2) Uani 1 1 d . . . . .
O78 O 0.4707(9) 0.6341(9) 0.6660(3) 0.035(3) Uani 1 1 d . . . . .
O79 O 0.0838(9) 0.8373(11) 0.8028(4) 0.053(3) Uani 1 1 d . . . . .
O80 O 0.0973(10) 0.7456(11) 0.5305(4) 0.050(3) Uani 1 1 d . . . . .
O81 O 0.7914(14) 0.3802(14) 0.8114(6) 0.081(5) Uani 1 1 d . . . . .
O82 O 0.9949(12) 0.1529(12) 0.9484(4) 0.066(4) Uani 1 1 d . U . . .
O83 O 0.7986(16) 0.7489(17) 0.0670(7) 0.106(7) Uani 1 1 d . . . . .
O84 O 0.289(2) 0.959(2) 0.6798(9) 0.149(10) Uani 1 1 d . U . . .
O85 O 0.2564(13) 0.6713(16) 0.9611(6) 0.093(6) Uani 1 1 d D U . . .
Ge1 Ge 0.75302(10) 0.84614(10) 0.60284(4) 0.0126(3) Uani 1 1 d . . . . .
Ge2 Ge 0.62552(10) 0.79288(10) 0.86323(4) 0.0133(3) Uani 1 1 d . . . . .
Mo1 Mo 0.38891(9) 0.68671(10) 0.82919(4) 0.0227(3) Uani 1 1 d . . . . .
Mo2 Mo 0.80388(9) 0.80302(9) 0.50061(3) 0.0188(3) Uani 1 1 d . . . . .
Mo3 Mo 0.49459(9) 0.88604(10) 0.56943(4) 0.0231(3) Uani 1 1 d . . . . .
Mo4 Mo 0.41643(9) 0.89091(9) 0.91186(4) 0.0196(3) Uani 1 1 d . . . . .
Mo5 Mo 0.59325(9) 0.65698(9) 0.54399(4) 0.0210(3) Uani 1 1 d . . . . .
Mo6 Mo 0.83922(9) 0.70264(9) 0.82075(4) 0.0187(3) Uani 1 1 d . . . . .
Mo7 Mo 0.80952(10) 0.62389(10) 0.91862(4) 0.0239(3) Uani 1 1 d . . . . .
Mo8 Mo 0.86861(9) 0.59894(9) 0.58077(4) 0.0205(3) Uani 1 1 d . . . . .
Mo9 Mo 0.55614(10) 0.70807(10) 0.64352(4) 0.0228(3) Uani 1 1 d . . . . .
Mo10 Mo 0.87714(9) 0.87039(10) 0.90086(4) 0.0222(3) Uani 1 1 d . . . . .
Mo11 Mo 0.65092(9) 0.97378(9) 0.94466(4) 0.0203(3) Uani 1 1 d . . . . .
Mo12 Mo 0.69639(9) 1.04395(9) 0.52950(4) 0.0211(3) Uani 1 1 d . . . . .
Mo13 Mo 0.57346(9) 0.71112(10) 0.96162(4) 0.0223(3) Uani 1 1 d . . . . .
Mo14 Mo 0.87971(9) 1.02173(9) 0.67500(4) 0.0193(3) Uani 1 1 d . . . . .
Mo15 Mo 0.69100(10) 1.04786(9) 0.83574(4) 0.0213(3) Uani 1 1 d . . . . .
Mo16 Mo 0.94070(9) 0.99787(10) 0.56294(4) 0.0208(3) Uani 1 1 d . . . . .
Mo17 Mo 0.46537(9) 0.95761(10) 0.79982(4) 0.0214(3) Uani 1 1 d . . . . .
Mo18 Mo 0.64544(9) 1.07355(9) 0.64193(4) 0.0192(3) Uani 1 1 d . . . . .
Mo19 Mo 1.00345(9) 0.78190(10) 0.63671(4) 0.0218(3) Uani 1 1 d . . . . .
Mo20 Mo 0.58830(9) 0.61041(9) 0.78025(4) 0.0203(3) Uani 1 1 d . . . . .
Mo21 Mo 0.81976(10) 0.65269(9) 0.67950(4) 0.0221(3) Uani 1 1 d . . . . .
Mo22 Mo 0.55661(10) 0.51617(9) 0.87623(4) 0.0245(3) Uani 1 1 d . . . . .
Tb1 Tb 0.68200(5) 0.88801(5) 0.73750(2) 0.01989(15) Uani 1 1 d . . . . .
N1 N 0.0857(12) 1.0583(11) 0.8158(4) 0.040(4) Uani 1 1 d . . . . .
H01A H 0.1284 1.0768 0.7977 0.048 Uiso 1 1 calc R U . . .
H01B H 0.0667 1.1165 0.8282 0.048 Uiso 1 1 calc R U . . .
N2 N 0.2559(10) 0.5983(11) 0.5226(5) 0.037(3) Uani 1 1 d . U . . .
N3 N 0.9095(13) 0.2798(11) 0.7551(5) 0.048(4) Uani 1 1 d . . . . .
H03A H 0.9454 0.2272 0.7458 0.057 Uiso 1 1 calc R U . . .
H03B H 0.9112 0.3339 0.7377 0.057 Uiso 1 1 calc R U . . .
N4 N 0.9042(11) 0.3172(10) 0.8993(4) 0.036(3) Uani 1 1 d . . . . .
H04A H 0.8877 0.3841 0.8941 0.044 Uiso 1 1 calc R U . . .
H04B H 0.8840 0.2796 0.8767 0.044 Uiso 1 1 calc R U . . .
N5 N 0.1713(15) 0.5083(15) 0.9105(7) 0.073(6) Uani 1 1 d . . . . .
N6 N 0.244(3) 1.143(3) 0.6419(12) 0.162(16) Uani 1 1 d . . . . .
N7 N 0.9722(17) 0.698(3) 0.0287(7) 0.112(10) Uani 1 1 d . . . . .
H07A H 1.0398 0.6954 0.0334 0.134 Uiso 1 1 calc R U . . .
H07B H 0.9549 0.6833 0.0020 0.134 Uiso 1 1 calc R U . . .
C1 C 0.1358(14) 0.9921(15) 0.8456(6) 0.045(5) Uani 1 1 d . . . . .
H1A H 0.0896 0.9723 0.8655 0.054 Uiso 1 1 calc R U . . .
H1B H 0.1928 1.0292 0.8603 0.054 Uiso 1 1 calc R U . . .
C2 C 0.1751(12) 0.8917(14) 0.8255(5) 0.040(4) Uani 1 1 d . . . . .
H2A H 0.2236 0.9101 0.8063 0.047 Uiso 1 1 calc R U . . .
H2B H 0.2085 0.8458 0.8467 0.047 Uiso 1 1 calc R U . . .
C3 C -0.0023(14) 1.0097(16) 0.7940(6) 0.048(5) Uani 1 1 d . . . . .
H3A H -0.0341 1.0582 0.7734 0.057 Uiso 1 1 calc R U . . .
H3B H -0.0511 0.9937 0.8133 0.057 Uiso 1 1 calc R U . . .
C4 C 0.0256(13) 0.9105(15) 0.7729(6) 0.046(5) Uani 1 1 d . . . . .
H4A H -0.0359 0.8759 0.7607 0.055 Uiso 1 1 calc R U . . .
H4B H 0.0665 0.9277 0.7508 0.055 Uiso 1 1 calc R U . . .
C5 C 0.2031(12) 0.7615(12) 0.5524(5) 0.031(3) Uani 1 1 d . . . . .
H5A H 0.2429 0.8047 0.5355 0.037 Uiso 1 1 calc R U . . .
H5B H 0.1995 0.7970 0.5787 0.037 Uiso 1 1 calc R U . . .
C6 C 0.2529(15) 0.6556(15) 0.5598(6) 0.048(5) Uani 1 1 d . . . . .
H6A H 0.3218 0.6654 0.5729 0.058 Uiso 1 1 calc R U . . .
H6B H 0.2158 0.6154 0.5786 0.058 Uiso 1 1 calc R U . . .
C7 C 0.0982(14) 0.6844(14) 0.4928(6) 0.043(4) Uani 1 1 d . . . . .
H7A H 0.1314 0.7240 0.4725 0.052 Uiso 1 1 calc R U . . .
H7B H 0.0290 0.6695 0.4811 0.052 Uiso 1 1 calc R U . . .
C8 C 0.1565(17) 0.5797(16) 0.5031(7) 0.056(5) Uani 1 1 d . . . . .
H8A H 0.1191 0.5375 0.5212 0.068 Uiso 1 1 calc R U . . .
H8B H 0.1605 0.5405 0.4776 0.068 Uiso 1 1 calc R U . . .
C9 C 0.8072(18) 0.2475(17) 0.7572(8) 0.073(7) Uani 1 1 d . . . . .
H9A H 0.8052 0.1913 0.7773 0.087 Uiso 1 1 calc R U . . .
H9B H 0.7780 0.2215 0.7304 0.087 Uiso 1 1 calc R U . . .
C10 C 0.7448(19) 0.3433(19) 0.7703(8) 0.074(7) Uani 1 1 d . . . . .
H10A H 0.7457 0.3993 0.7500 0.089 Uiso 1 1 calc R U . . .
H10B H 0.6746 0.3229 0.7719 0.089 Uiso 1 1 calc R U . . .
C11 C 0.890(2) 0.407(2) 0.8085(9) 0.083(8) Uani 1 1 d . U . . .
H11A H 0.9207 0.4328 0.8351 0.100 Uiso 1 1 calc R U . . .
H11B H 0.8923 0.4631 0.7883 0.100 Uiso 1 1 calc R U . . .
C12 C 0.950(3) 0.309(3) 0.7949(10) 0.107(10) Uani 1 1 d . U . . .
H12A H 1.0219 0.3265 0.7950 0.128 Uiso 1 1 calc R U . . .
H12B H 0.9446 0.2513 0.8141 0.128 Uiso 1 1 calc R U . . .
C13 C 1.0431(14) 0.2008(18) 0.9143(6) 0.057(6) Uani 1 1 d . . . . .
H13A H 1.1166 0.1971 0.9203 0.068 Uiso 1 1 calc R U . . .
H13B H 1.0239 0.1621 0.8888 0.068 Uiso 1 1 calc R U . . .
C14 C 1.012(2) 0.3081(19) 0.9089(7) 0.072(6) Uani 1 1 d . U . . .
H14A H 1.0459 0.3389 0.8866 0.086 Uiso 1 1 calc R U . . .
H14B H 1.0337 0.3470 0.9341 0.086 Uiso 1 1 calc R U . . .
C15 C 0.8826(15) 0.1693(14) 0.9403(6) 0.046(5) Uani 1 1 d . . . . .
H15A H 0.8560 0.1270 0.9167 0.056 Uiso 1 1 calc R U . . .
H15B H 0.8504 0.1460 0.9642 0.056 Uiso 1 1 calc R U . . .
C16 C 0.8567(17) 0.2820(17) 0.9317(6) 0.059(6) Uani 1 1 d . . . . .
H16A H 0.7836 0.2895 0.9253 0.070 Uiso 1 1 calc R U . . .
H16B H 0.8778 0.3239 0.9562 0.070 Uiso 1 1 calc R U . . .
C17 C 0.3177(19) 0.5746(19) 0.9569(8) 0.076(7) Uani 1 1 d . U . . .
H17A H 0.3599 0.5820 0.9344 0.091 Uiso 1 1 calc R U . . .
H17B H 0.3613 0.5606 0.9824 0.091 Uiso 1 1 calc R U . . .
C18 C 0.244(3) 0.490(3) 0.9482(11) 0.111(11) Uani 1 1 d . U . . .
H18A H 0.2064 0.4818 0.9719 0.134 Uiso 1 1 calc R U . . .
H18B H 0.2809 0.4254 0.9447 0.134 Uiso 1 1 calc R U . . .
C19 C 0.175(2) 0.690(2) 0.9277(7) 0.081(8) Uani 1 1 d . . . . .
H19A H 0.1318 0.7474 0.9352 0.098 Uiso 1 1 calc R U . . .
H19B H 0.2032 0.7091 0.9024 0.098 Uiso 1 1 calc R U . . .
C20 C 0.118(2) 0.599(3) 0.9215(10) 0.099(9) Uani 1 1 d . U . . .
H20A H 0.0626 0.6120 0.8998 0.119 Uiso 1 1 calc R U . . .
H20B H 0.0873 0.5836 0.9468 0.119 Uiso 1 1 calc R U . . .
C21 C 0.346(3) 1.112(4) 0.6458(14) 0.147(15) Uani 1 1 d . U . . .
H21A H 0.3883 1.1718 0.6542 0.177 Uiso 1 1 calc R U . . .
H21B H 0.3628 1.0887 0.6189 0.177 Uiso 1 1 calc R U . . .
C22 C 0.369(3) 1.019(4) 0.6786(14) 0.153(16) Uani 1 1 d . U . . .
H22A H 0.4257 0.9778 0.6711 0.184 Uiso 1 1 calc R U . . .
H22B H 0.3881 1.0490 0.7059 0.184 Uiso 1 1 calc R U . . .
C23 C 0.171(3) 1.087(4) 0.6468(13) 0.135(17) Uani 1 1 d . . . . .
H23A H 0.1555 1.0433 0.6225 0.162 Uiso 1 1 calc R U . . .
H23B H 0.1126 1.1310 0.6499 0.162 Uiso 1 1 calc R U . . .
C24 C 0.193(3) 1.020(3) 0.6840(13) 0.132(13) Uani 1 1 d . U . . .
H24A H 0.1365 0.9716 0.6861 0.158 Uiso 1 1 calc R U . . .
H24B H 0.2010 1.0627 0.7089 0.158 Uiso 1 1 calc R U . . .
C25 C 0.9400(19) 0.8022(18) 0.0365(7) 0.062(6) Uani 1 1 d . . . . .
C26 C 0.835(2) 0.801(2) 0.0314(9) 0.082(7) Uani 1 1 d . U . . .
C27 C 0.808(2) 0.638(2) 0.0565(8) 0.075(7) Uani 1 1 d . . . . .
C28 C 0.928(2) 0.614(2) 0.0547(9) 0.092(8) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
O1 Ge1 1.719(8) . ?
O1 Mo14 2.185(8) . ?
O1 Mo18 2.188(9) . ?
O2 Mo3 1.861(9) . ?
O2 Mo18 1.958(9) . ?
O3 Mo5 1.913(10) . ?
O3 Mo3 1.964(9) . ?
O4 Mo5 1.769(9) . ?
O4 Mo9 2.173(9) . ?
O5 Mo16 2.101(9) . ?
O5 Mo2 2.130(9) . ?
O6 Mo9 1.882(10) . ?
O6 Mo21 1.958(10) . ?
O7 Ge1 1.733(9) . ?
O7 Mo19 2.261(9) . ?
O7 Mo8 2.308(9) . ?
O7 Mo21 2.319(9) . ?
O8 Ge1 1.743(9) . ?
O8 Mo2 2.255(9) . ?
O8 Mo12 2.322(9) . ?
O8 Mo16 2.331(10) . ?
O9 Mo2 1.796(10) . ?
O9 Mo8 2.084(10) . ?
O10 Mo6 1.835(10) . ?
O10 Mo20 2.018(9) . ?
O11 Mo8 1.922(9) . ?
O11 Mo19 1.982(9) . ?
O12 Mo19 1.865(9) . ?
O12 Mo14 1.949(9) . ?
O13 Mo14 1.934(9) . ?
O13 Mo18 1.952(9) . ?
O14 Mo5 1.690(10) . ?
O15 Ge1 1.731(8) . ?
O15 Mo9 2.279(8) . ?
O15 Mo3 2.288(9) . ?
O15 Mo5 2.319(8) . ?
O16 Mo3 1.672(10) . ?
O17 Mo18 1.738(8) . ?
O17 Tb1 2.444(9) . ?
O18 Mo14 1.730(9) . ?
O18 Tb1 2.405(9) . ?
O19 Mo21 1.728(10) . ?
O19 Tb1 2.393(10) . ?
O20 Mo6 1.731(9) . ?
O20 Tb1 2.366(9) . ?
O21 Mo16 1.750(9) . ?
O21 Mo14 2.185(9) . ?
O22 Mo12 1.689(10) . ?
O23 Mo3 1.851(9) . ?
O23 Mo9 2.026(10) . ?
O24 Mo6 1.686(9) . ?
O25 Mo17 1.753(9) . ?
O25 Tb1 2.374(9) . ?
O26 Mo7 1.795(10) . ?
O26 Mo6 2.143(10) . ?
O27 Mo10 1.825(8) . ?
O27 Mo6 2.087(10) . ?
O28 Mo15 1.730(9) . ?
O28 Tb1 2.369(9) . ?
O29 Ge2 1.765(9) . ?
O29 Mo6 2.239(8) . ?
O29 Mo10 2.276(9) . ?
O29 Mo7 2.308(9) . ?
O30 Mo22 1.900(10) . ?
O30 Mo7 1.911(10) . ?
O31 Mo2 1.798(9) . ?
O31 Mo5 2.123(9) . ?
O32 Mo12 1.863(9) . ?
O32 Mo3 1.982(9) . ?
O33 Mo2 1.696(10) . ?
O34 Mo19 1.890(9) . ?
O34 Mo16 1.951(9) . ?
O35 Mo21 1.917(10) . ?
O35 Mo19 1.937(9) . ?
O36 Mo8 1.761(9) . ?
O36 Mo21 2.197(9) . ?
O37 Mo5 1.892(9) . ?
O37 Mo8 1.931(9) . ?
O38 Mo15 1.713(10) . ?
O39 Mo17 1.945(9) . ?
O39 Mo15 1.962(9) . ?
O40 Ge2 1.707(8) . ?
O40 Mo15 2.195(8) . ?
O40 Mo17 2.213(9) . ?
O41 Mo12 2.074(9) . ?
O41 Mo2 2.099(9) . ?
O42 Mo12 1.757(10) . ?
O42 Mo18 2.179(10) . ?
O43 Mo16 1.876(9) . ?
O43 Mo12 2.002(9) . ?
O44 Mo17 1.921(9) . ?
O44 Mo1 1.928(9) . ?
O45 Mo4 1.784(10) . ?
O45 Mo17 2.146(10) . ?
O46 Mo20 1.682(10) . ?
O47 Mo1 1.690(10) . ?
O48 Ge2 1.747(9) . ?
O48 Mo1 2.255(9) . ?
O48 Mo20 2.320(9) . ?
O48 Mo22 2.347(8) . ?
O49 Mo1 1.797(9) . ?
O49 Mo4 2.067(9) . ?
O50 Mo22 1.801(9) . ?
O50 Mo20 2.151(9) . ?
O51 Mo10 1.677(10) . ?
O52 Mo15 1.925(10) . ?
O52 Mo10 1.936(10) . ?
O53 Mo11 1.836(9) . ?
O53 Mo10 2.016(8) . ?
O54 Mo7 1.686(10) . ?
O55 Mo14 1.697(10) . ?
O56 Mo11 2.044(10) . ?
O56 Mo13 2.121(10) . ?
O57 Mo4 1.839(10) . ?
O57 Mo11 2.068(10) . ?
O58 Ge2 1.756(8) . ?
O58 Mo11 2.278(9) . ?
O58 Mo13 2.281(9) . ?
O58 Mo4 2.300(9) . ?
O59 Mo4 1.672(10) . ?
O60 Mo13 1.932(10) . ?
O60 Mo4 1.963(10) . ?
O61 Mo22 1.693(10) . ?
O62 Mo22 1.916(10) . ?
O62 Mo1 1.971(10) . ?
O63 Mo13 1.807(10) . ?
O63 Mo22 2.034(10) . ?
O64 Mo11 1.680(9) . ?
O65 Mo11 1.769(9) . ?
O65 Mo15 2.160(9) . ?
O66 Mo13 1.670(9) . ?
O67 Mo13 1.858(10) . ?
O67 Mo7 1.994(9) . ?
O68 Mo10 1.889(10) . ?
O68 Mo7 1.994(10) . ?
O69 Mo20 1.745(10) . ?
O69 Tb1 2.334(10) . ?
O70 Mo20 1.870(10) . ?
O70 Mo1 2.033(9) . ?
O71 Mo8 1.683(10) . ?
O72 Mo16 1.700(9) . ?
O73 Mo19 1.700(10) . ?
O74 Mo21 1.674(10) . ?
O75 Mo18 1.688(9) . ?
O76 Mo17 1.708(11) . ?
O77 Mo9 1.711(10) . ?
O77 Tb1 2.406(10) . ?
O78 Mo9 1.695(10) . ?
O79 C4 1.49(2) . ?
O79 C2 1.51(2) . ?
O80 C7 1.45(2) . ?
O80 C5 1.512(19) . ?
O81 C11 1.36(3) . ?
O81 C10 1.48(3) . ?
O82 C13 1.47(2) . ?
O82 C15 1.49(2) . ?
O83 C27 1.46(3) . ?
O83 C26 1.46(3) . ?
O84 C22 1.31(4) . ?
O84 C24 1.51(4) . ?
O85 C19 1.46(3) . ?
O85 C17 1.49(3) . ?
N1 C1 1.39(2) . ?
N1 C3 1.43(2) . ?
N2 C6 1.41(2) . ?
N2 C8 1.41(3) . ?
N3 C12 1.40(3) . ?
N3 C9 1.42(3) . ?
N4 C16 1.36(2) . ?
N4 C14 1.44(3) . ?
N5 C20 1.42(4) . ?
N5 C18 1.49(4) . ?
N6 C23 1.22(5) . ?
N6 C21 1.39(5) . ?
N7 C25 1.42(3) . ?
N7 C28 1.52(4) . ?
C1 C2 1.55(3) . ?
C3 C4 1.50(3) . ?
C5 C6 1.51(2) . ?
C7 C8 1.56(3) . ?
C9 C10 1.56(3) . ?
C11 C12 1.57(4) . ?
C13 C14 1.43(3) . ?
C15 C16 1.49(3) . ?
C17 C18 1.45(4) . ?
C19 C20 1.39(4) . ?
C21 C22 1.59(5) . ?
C23 C24 1.48(5) . ?
C25 C26 1.38(3) . ?
C27 C28 1.63(4) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ge1 O1 Mo14 128.5(5) . . ?
Ge1 O1 Mo18 128.1(5) . . ?
Mo14 O1 Mo18 95.3(3) . . ?
Mo3 O2 Mo18 160.3(6) . . ?
Mo5 O3 Mo3 118.5(5) . . ?
Mo5 O4 Mo9 117.7(4) . . ?
Mo16 O5 Mo2 114.7(4) . . ?
Mo9 O6 Mo21 141.0(5) . . ?
Ge1 O7 Mo19 120.0(4) . . ?
Ge1 O7 Mo8 125.4(4) . . ?
Mo19 O7 Mo8 94.0(3) . . ?
Ge1 O7 Mo21 121.0(4) . . ?
Mo19 O7 Mo21 94.2(3) . . ?
Mo8 O7 Mo21 94.7(3) . . ?
Ge1 O8 Mo2 121.4(5) . . ?
Ge1 O8 Mo12 117.3(4) . . ?
Mo2 O8 Mo12 101.5(3) . . ?
Ge1 O8 Mo16 117.7(5) . . ?
Mo2 O8 Mo16 101.9(3) . . ?
Mo12 O8 Mo16 91.9(3) . . ?
Mo2 O9 Mo8 145.4(5) . . ?
Mo6 O10 Mo20 140.4(5) . . ?
Mo8 O11 Mo19 117.7(4) . . ?
Mo19 O12 Mo14 156.9(5) . . ?
Mo14 O13 Mo18 112.5(4) . . ?
Ge1 O15 Mo9 121.8(4) . . ?
Ge1 O15 Mo3 120.8(4) . . ?
Mo9 O15 Mo3 93.8(3) . . ?
Ge1 O15 Mo5 125.2(5) . . ?
Mo9 O15 Mo5 94.6(3) . . ?
Mo3 O15 Mo5 92.6(3) . . ?
Mo18 O17 Tb1 135.6(5) . . ?
Mo14 O18 Tb1 138.2(5) . . ?
Mo21 O19 Tb1 161.5(5) . . ?
Mo6 O20 Tb1 153.5(5) . . ?
Mo16 O21 Mo14 151.6(5) . . ?
Mo3 O23 Mo9 118.6(5) . . ?
Mo17 O25 Tb1 132.4(5) . . ?
Mo7 O26 Mo6 118.5(5) . . ?
Mo10 O27 Mo6 118.0(5) . . ?
Mo15 O28 Tb1 133.1(5) . . ?
Ge2 O29 Mo6 119.7(4) . . ?
Ge2 O29 Mo10 122.7(4) . . ?
Mo6 O29 Mo10 96.0(3) . . ?
Ge2 O29 Mo7 122.3(4) . . ?
Mo6 O29 Mo7 96.4(3) . . ?
Mo10 O29 Mo7 93.1(3) . . ?
Mo22 O30 Mo7 156.6(6) . . ?
Mo2 O31 Mo5 145.5(5) . . ?
Mo12 O32 Mo3 146.8(5) . . ?
Mo19 O34 Mo16 146.3(5) . . ?
Mo21 O35 Mo19 121.0(5) . . ?
Mo8 O36 Mo21 118.1(5) . . ?
Mo5 O37 Mo8 162.0(5) . . ?
Mo17 O39 Mo15 114.5(4) . . ?
Ge2 O40 Mo15 126.9(5) . . ?
Ge2 O40 Mo17 125.0(4) . . ?
Mo15 O40 Mo17 96.4(3) . . ?
Mo12 O41 Mo2 116.4(4) . . ?
Mo12 O42 Mo18 149.2(6) . . ?
Mo16 O43 Mo12 119.0(5) . . ?
Mo17 O44 Mo1 153.0(5) . . ?
Mo4 O45 Mo17 157.0(6) . . ?
Ge2 O48 Mo1 119.9(4) . . ?
Ge2 O48 Mo20 120.7(4) . . ?
Mo1 O48 Mo20 94.7(3) . . ?
Ge2 O48 Mo22 126.8(4) . . ?
Mo1 O48 Mo22 93.3(3) . . ?
Mo20 O48 Mo22 93.6(3) . . ?
Mo1 O49 Mo4 148.6(5) . . ?
Mo22 O50 Mo20 118.5(5) . . ?
Mo15 O52 Mo10 160.0(6) . . ?
Mo11 O53 Mo10 146.6(5) . . ?
Mo11 O56 Mo13 117.2(4) . . ?
Mo4 O57 Mo11 117.1(5) . . ?
Ge2 O58 Mo11 119.2(5) . . ?
Ge2 O58 Mo13 119.3(4) . . ?
Mo11 O58 Mo13 102.5(3) . . ?
Ge2 O58 Mo4 121.8(5) . . ?
Mo11 O58 Mo4 93.5(3) . . ?
Mo13 O58 Mo4 95.0(3) . . ?
Mo13 O60 Mo4 120.2(5) . . ?
Mo22 O62 Mo1 118.9(5) . . ?
Mo13 O63 Mo22 149.3(6) . . ?
Mo11 O65 Mo15 144.8(6) . . ?
Mo13 O67 Mo7 150.2(5) . . ?
Mo10 O68 Mo7 117.9(5) . . ?
Mo20 O69 Tb1 163.3(6) . . ?
Mo20 O70 Mo1 119.1(5) . . ?
Mo9 O77 Tb1 154.8(5) . . ?
C4 O79 C2 110.9(13) . . ?
C7 O80 C5 112.0(12) . . ?
C11 O81 C10 109(2) . . ?
C13 O82 C15 108.2(14) . . ?
C27 O83 C26 102.3(19) . . ?
C22 O84 C24 113(4) . . ?
C19 O85 C17 115.6(19) . . ?
O1 Ge1 O15 110.6(4) . . ?
O1 Ge1 O7 111.2(4) . . ?
O15 Ge1 O7 106.2(4) . . ?
O1 Ge1 O8 109.7(4) . . ?
O15 Ge1 O8 110.1(4) . . ?
O7 Ge1 O8 109.0(4) . . ?
O40 Ge2 O48 112.4(4) . . ?
O40 Ge2 O58 108.7(4) . . ?
O48 Ge2 O58 109.4(4) . . ?
O40 Ge2 O29 110.1(4) . . ?
O48 Ge2 O29 106.9(4) . . ?
O58 Ge2 O29 109.4(4) . . ?
O47 Mo1 O49 102.9(5) . . ?
O47 Mo1 O44 101.2(5) . . ?
O49 Mo1 O44 90.0(4) . . ?
O47 Mo1 O62 98.1(5) . . ?
O49 Mo1 O62 93.6(4) . . ?
O44 Mo1 O62 159.0(4) . . ?
O47 Mo1 O70 96.3(5) . . ?
O49 Mo1 O70 160.9(4) . . ?
O44 Mo1 O70 86.4(4) . . ?
O62 Mo1 O70 83.4(4) . . ?
O47 Mo1 O48 166.7(4) . . ?
O49 Mo1 O48 88.8(4) . . ?
O44 Mo1 O48 84.9(4) . . ?
O62 Mo1 O48 74.5(4) . . ?
O70 Mo1 O48 72.2(4) . . ?
O33 Mo2 O9 104.3(5) . . ?
O33 Mo2 O31 106.0(5) . . ?
O9 Mo2 O31 95.8(4) . . ?
O33 Mo2 O41 94.0(4) . . ?
O9 Mo2 O41 159.4(4) . . ?
O31 Mo2 O41 88.0(4) . . ?
O33 Mo2 O5 91.6(4) . . ?
O9 Mo2 O5 86.9(4) . . ?
O31 Mo2 O5 160.8(4) . . ?
O41 Mo2 O5 83.1(4) . . ?
O33 Mo2 O8 159.0(4) . . ?
O9 Mo2 O8 88.5(4) . . ?
O31 Mo2 O8 88.8(4) . . ?
O41 Mo2 O8 71.3(3) . . ?
O5 Mo2 O8 72.2(3) . . ?
O16 Mo3 O23 101.5(5) . . ?
O16 Mo3 O2 102.9(5) . . ?
O23 Mo3 O2 93.5(4) . . ?
O16 Mo3 O3 98.6(5) . . ?
O23 Mo3 O3 90.1(4) . . ?
O2 Mo3 O3 157.0(4) . . ?
O16 Mo3 O32 97.9(5) . . ?
O23 Mo3 O32 160.5(4) . . ?
O2 Mo3 O32 84.2(4) . . ?
O3 Mo3 O32 84.9(4) . . ?
O16 Mo3 O15 171.5(4) . . ?
O23 Mo3 O15 74.8(4) . . ?
O2 Mo3 O15 85.1(4) . . ?
O3 Mo3 O15 73.9(4) . . ?
O32 Mo3 O15 85.7(3) . . ?
O59 Mo4 O45 103.5(5) . . ?
O59 Mo4 O57 103.7(5) . . ?
O45 Mo4 O57 96.6(4) . . ?
O59 Mo4 O60 98.6(5) . . ?
O45 Mo4 O60 154.2(4) . . ?
O57 Mo4 O60 91.1(4) . . ?
O59 Mo4 O49 97.2(5) . . ?
O45 Mo4 O49 83.7(4) . . ?
O57 Mo4 O49 158.4(4) . . ?
O60 Mo4 O49 80.3(4) . . ?
O59 Mo4 O58 170.4(4) . . ?
O45 Mo4 O58 86.0(4) . . ?
O57 Mo4 O58 76.2(4) . . ?
O60 Mo4 O58 71.9(4) . . ?
O49 Mo4 O58 82.4(3) . . ?
O14 Mo5 O4 103.7(5) . . ?
O14 Mo5 O37 100.3(5) . . ?
O4 Mo5 O37 96.4(4) . . ?
O14 Mo5 O3 100.7(5) . . ?
O4 Mo5 O3 94.7(4) . . ?
O37 Mo5 O3 153.1(4) . . ?
O14 Mo5 O31 95.2(4) . . ?
O4 Mo5 O31 161.1(4) . . ?
O37 Mo5 O31 79.6(4) . . ?
O3 Mo5 O31 82.0(4) . . ?
O14 Mo5 O15 174.8(4) . . ?
O4 Mo5 O15 77.0(4) . . ?
O37 Mo5 O15 84.7(4) . . ?
O3 Mo5 O15 74.1(4) . . ?
O31 Mo5 O15 84.3(3) . . ?
O24 Mo6 O20 103.1(5) . . ?
O24 Mo6 O10 105.4(5) . . ?
O20 Mo6 O10 97.8(4) . . ?
O24 Mo6 O27 92.0(4) . . ?
O20 Mo6 O27 89.7(4) . . ?
O10 Mo6 O27 158.7(4) . . ?
O24 Mo6 O26 93.3(5) . . ?
O20 Mo6 O26 160.9(4) . . ?
O10 Mo6 O26 87.1(4) . . ?
O27 Mo6 O26 79.8(4) . . ?
O24 Mo6 O29 157.7(5) . . ?
O20 Mo6 O29 91.5(4) . . ?
O10 Mo6 O29 88.9(4) . . ?
O27 Mo6 O29 71.0(3) . . ?
O26 Mo6 O29 70.1(3) . . ?
O54 Mo7 O26 104.2(5) . . ?
O54 Mo7 O30 102.1(5) . . ?
O26 Mo7 O30 93.8(4) . . ?
O54 Mo7 O68 96.4(5) . . ?
O26 Mo7 O68 90.8(4) . . ?
O30 Mo7 O68 159.2(4) . . ?
O54 Mo7 O67 98.7(5) . . ?
O26 Mo7 O67 157.1(4) . . ?
O30 Mo7 O67 82.5(4) . . ?
O68 Mo7 O67 85.4(4) . . ?
O54 Mo7 O29 169.2(5) . . ?
O26 Mo7 O29 74.5(4) . . ?
O30 Mo7 O29 88.7(4) . . ?
O68 Mo7 O29 73.0(4) . . ?
O67 Mo7 O29 82.8(4) . . ?
O71 Mo8 O36 103.7(5) . . ?
O71 Mo8 O11 98.9(5) . . ?
O36 Mo8 O11 94.4(4) . . ?
O71 Mo8 O37 101.8(5) . . ?
O36 Mo8 O37 95.4(4) . . ?
O11 Mo8 O37 154.2(4) . . ?
O71 Mo8 O9 95.7(4) . . ?
O36 Mo8 O9 160.6(4) . . ?
O11 Mo8 O9 81.7(4) . . ?
O37 Mo8 O9 81.2(4) . . ?
O71 Mo8 O7 172.8(4) . . ?
O36 Mo8 O7 77.5(4) . . ?
O11 Mo8 O7 74.0(3) . . ?
O37 Mo8 O7 85.0(3) . . ?
O9 Mo8 O7 83.1(3) . . ?
O78 Mo9 O77 104.8(5) . . ?
O78 Mo9 O6 105.0(5) . . ?
O77 Mo9 O6 96.4(4) . . ?
O78 Mo9 O23 95.7(5) . . ?
O77 Mo9 O23 92.8(4) . . ?
O6 Mo9 O23 154.3(4) . . ?
O78 Mo9 O4 91.3(5) . . ?
O77 Mo9 O4 163.3(4) . . ?
O6 Mo9 O4 83.6(4) . . ?
O23 Mo9 O4 80.8(4) . . ?
O78 Mo9 O15 159.3(4) . . ?
O77 Mo9 O15 92.6(4) . . ?
O6 Mo9 O15 83.7(4) . . ?
O23 Mo9 O15 72.0(3) . . ?
O4 Mo9 O15 70.8(3) . . ?
O51 Mo10 O27 101.0(5) . . ?
O51 Mo10 O68 100.2(5) . . ?
O27 Mo10 O68 92.6(4) . . ?
O51 Mo10 O52 101.2(5) . . ?
O27 Mo10 O52 93.3(4) . . ?
O68 Mo10 O52 156.2(4) . . ?
O51 Mo10 O53 97.7(5) . . ?
O27 Mo10 O53 161.3(4) . . ?
O68 Mo10 O53 84.9(4) . . ?
O52 Mo10 O53 82.2(4) . . ?
O51 Mo10 O29 173.7(4) . . ?
O27 Mo10 O29 74.7(4) . . ?
O68 Mo10 O29 75.6(4) . . ?
O52 Mo10 O29 83.8(4) . . ?
O53 Mo10 O29 86.7(4) . . ?
O64 Mo11 O65 104.2(5) . . ?
O64 Mo11 O53 104.5(5) . . ?
O65 Mo11 O53 96.1(4) . . ?
O64 Mo11 O56 95.4(5) . . ?
O65 Mo11 O56 158.1(4) . . ?
O53 Mo11 O56 88.3(4) . . ?
O64 Mo11 O57 93.3(4) . . ?
O65 Mo11 O57 87.5(4) . . ?
O53 Mo11 O57 160.3(4) . . ?
O56 Mo11 O57 81.7(4) . . ?
O64 Mo11 O58 161.2(4) . . ?
O65 Mo11 O58 87.9(4) . . ?
O53 Mo11 O58 88.1(4) . . ?
O56 Mo11 O58 70.7(3) . . ?
O57 Mo11 O58 72.6(4) . . ?
O22 Mo12 O42 105.0(5) . . ?
O22 Mo12 O32 103.8(5) . . ?
O42 Mo12 O32 92.8(4) . . ?
O22 Mo12 O43 97.6(5) . . ?
O42 Mo12 O43 92.7(4) . . ?
O32 Mo12 O43 155.7(4) . . ?
O22 Mo12 O41 94.9(4) . . ?
O42 Mo12 O41 159.8(4) . . ?
O32 Mo12 O41 85.2(4) . . ?
O43 Mo12 O41 81.6(4) . . ?
O22 Mo12 O8 162.9(4) . . ?
O42 Mo12 O8 89.4(4) . . ?
O32 Mo12 O8 84.2(4) . . ?
O43 Mo12 O8 72.1(3) . . ?
O41 Mo12 O8 70.4(3) . . ?
O66 Mo13 O63 104.9(5) . . ?
O66 Mo13 O67 104.1(5) . . ?
O63 Mo13 O67 90.4(4) . . ?
O66 Mo13 O60 97.8(5) . . ?
O63 Mo13 O60 94.2(4) . . ?
O67 Mo13 O60 155.7(4) . . ?
O66 Mo13 O56 93.0(4) . . ?
O63 Mo13 O56 162.1(4) . . ?
O67 Mo13 O56 84.9(4) . . ?
O60 Mo13 O56 83.4(4) . . ?
O66 Mo13 O58 160.5(4) . . ?
O63 Mo13 O58 92.9(4) . . ?
O67 Mo13 O58 83.1(4) . . ?
O60 Mo13 O58 72.9(4) . . ?
O56 Mo13 O58 69.4(3) . . ?
O55 Mo14 O18 103.5(4) . . ?
O55 Mo14 O13 98.1(5) . . ?
O18 Mo14 O13 98.2(4) . . ?
O55 Mo14 O12 97.7(5) . . ?
O18 Mo14 O12 96.9(4) . . ?
O13 Mo14 O12 154.9(4) . . ?
O55 Mo14 O1 168.6(4) . . ?
O18 Mo14 O1 86.4(4) . . ?
O13 Mo14 O1 74.5(4) . . ?
O12 Mo14 O1 86.6(4) . . ?
O55 Mo14 O21 91.2(4) . . ?
O18 Mo14 O21 165.2(4) . . ?
O13 Mo14 O21 82.0(3) . . ?
O12 Mo14 O21 78.3(4) . . ?
O1 Mo14 O21 79.3(3) . . ?
O38 Mo15 O28 103.1(5) . . ?
O38 Mo15 O52 100.6(5) . . ?
O28 Mo15 O52 98.2(4) . . ?
O38 Mo15 O39 97.2(5) . . ?
O28 Mo15 O39 94.5(4) . . ?
O52 Mo15 O39 155.1(4) . . ?
O38 Mo15 O65 89.1(4) . . ?
O28 Mo15 O65 167.7(4) . . ?
O52 Mo15 O65 80.9(4) . . ?
O39 Mo15 O65 82.2(4) . . ?
O38 Mo15 O40 168.0(4) . . ?
O28 Mo15 O40 85.5(4) . . ?
O52 Mo15 O40 86.2(4) . . ?
O39 Mo15 O40 73.5(3) . . ?
O65 Mo15 O40 82.2(3) . . ?
O72 Mo16 O21 103.5(5) . . ?
O72 Mo16 O43 100.4(5) . . ?
O21 Mo16 O43 97.4(4) . . ?
O72 Mo16 O34 101.9(5) . . ?
O21 Mo16 O34 90.3(4) . . ?
O43 Mo16 O34 154.0(4) . . ?
O72 Mo16 O5 95.7(4) . . ?
O21 Mo16 O5 160.0(4) . . ?
O43 Mo16 O5 84.2(4) . . ?
O34 Mo16 O5 80.4(4) . . ?
O72 Mo16 O8 166.0(4) . . ?
O21 Mo16 O8 90.1(4) . . ?
O43 Mo16 O8 74.0(4) . . ?
O34 Mo16 O8 81.2(4) . . ?
O5 Mo16 O8 71.2(3) . . ?
O76 Mo17 O25 103.4(5) . . ?
O76 Mo17 O44 100.0(5) . . ?
O25 Mo17 O44 95.2(4) . . ?
O76 Mo17 O39 96.8(5) . . ?
O25 Mo17 O39 96.7(4) . . ?
O44 Mo17 O39 156.5(4) . . ?
O76 Mo17 O45 90.6(4) . . ?
O25 Mo17 O45 165.7(4) . . ?
O44 Mo17 O45 79.2(4) . . ?
O39 Mo17 O45 84.4(4) . . ?
O76 Mo17 O40 167.8(4) . . ?
O25 Mo17 O40 85.3(4) . . ?
O44 Mo17 O40 87.6(4) . . ?
O39 Mo17 O40 73.4(3) . . ?
O45 Mo17 O40 81.4(3) . . ?
O75 Mo18 O17 103.2(5) . . ?
O75 Mo18 O13 97.9(5) . . ?
O17 Mo18 O13 96.7(4) . . ?
O75 Mo18 O2 98.7(5) . . ?
O17 Mo18 O2 97.9(4) . . ?
O13 Mo18 O2 154.7(4) . . ?
O75 Mo18 O42 89.2(5) . . ?
O17 Mo18 O42 167.4(4) . . ?
O13 Mo18 O42 83.5(4) . . ?
O2 Mo18 O42 77.9(4) . . ?
O75 Mo18 O1 167.1(5) . . ?
O17 Mo18 O1 88.0(4) . . ?
O13 Mo18 O1 74.1(3) . . ?
O2 Mo18 O1 86.0(4) . . ?
O42 Mo18 O1 80.0(3) . . ?
O73 Mo19 O12 103.5(5) . . ?
O73 Mo19 O34 102.6(4) . . ?
O12 Mo19 O34 88.3(4) . . ?
O73 Mo19 O35 98.6(4) . . ?
O12 Mo19 O35 90.7(4) . . ?
O34 Mo19 O35 158.3(4) . . ?
O73 Mo19 O11 96.6(4) . . ?
O12 Mo19 O11 159.9(4) . . ?
O34 Mo19 O11 87.3(4) . . ?
O35 Mo19 O11 86.3(4) . . ?
O73 Mo19 O7 167.1(4) . . ?
O12 Mo19 O7 86.2(4) . . ?
O34 Mo19 O7 86.1(4) . . ?
O35 Mo19 O7 72.3(4) . . ?
O11 Mo19 O7 74.0(3) . . ?
O46 Mo20 O69 105.2(5) . . ?
O46 Mo20 O70 101.0(5) . . ?
O69 Mo20 O70 99.8(4) . . ?
O46 Mo20 O10 98.8(5) . . ?
O69 Mo20 O10 88.9(4) . . ?
O70 Mo20 O10 155.4(4) . . ?
O46 Mo20 O50 92.4(5) . . ?
O69 Mo20 O50 160.2(4) . . ?
O70 Mo20 O50 85.5(4) . . ?
O10 Mo20 O50 79.2(4) . . ?
O46 Mo20 O48 162.8(5) . . ?
O69 Mo20 O48 91.9(4) . . ?
O70 Mo20 O48 73.5(4) . . ?
O10 Mo20 O48 83.3(4) . . ?
O50 Mo20 O48 71.1(3) . . ?
O74 Mo21 O19 105.5(5) . . ?
O74 Mo21 O35 100.8(5) . . ?
O19 Mo21 O35 99.1(4) . . ?
O74 Mo21 O6 101.2(5) . . ?
O19 Mo21 O6 90.7(4) . . ?
O35 Mo21 O6 152.5(4) . . ?
O74 Mo21 O36 91.5(4) . . ?
O19 Mo21 O36 162.5(4) . . ?
O35 Mo21 O36 81.2(4) . . ?
O6 Mo21 O36 81.9(4) . . ?
O74 Mo21 O7 160.2(4) . . ?
O19 Mo21 O7 93.7(4) . . ?
O35 Mo21 O7 71.3(3) . . ?
O6 Mo21 O7 82.6(4) . . ?
O36 Mo21 O7 69.7(3) . . ?
O61 Mo22 O50 102.9(5) . . ?
O61 Mo22 O30 100.7(5) . . ?
O50 Mo22 O30 93.4(4) . . ?
O61 Mo22 O62 99.9(5) . . ?
O50 Mo22 O62 93.1(4) . . ?
O30 Mo22 O62 156.4(4) . . ?
O61 Mo22 O63 99.1(5) . . ?
O50 Mo22 O63 158.0(4) . . ?
O30 Mo22 O63 82.0(4) . . ?
O62 Mo22 O63 83.5(4) . . ?
O61 Mo22 O48 173.0(5) . . ?
O50 Mo22 O48 76.5(4) . . ?
O30 Mo22 O48 86.3(4) . . ?
O62 Mo22 O48 73.3(4) . . ?
O63 Mo22 O48 81.7(3) . . ?
O69 Tb1 O20 70.7(3) . . ?
O69 Tb1 O28 119.0(3) . . ?
O20 Tb1 O28 77.2(3) . . ?
O69 Tb1 O25 75.4(3) . . ?
O20 Tb1 O25 119.0(3) . . ?
O28 Tb1 O25 77.1(3) . . ?
O69 Tb1 O19 81.4(3) . . ?
O20 Tb1 O19 71.5(3) . . ?
O28 Tb1 O19 133.9(3) . . ?
O25 Tb1 O19 148.3(3) . . ?
O69 Tb1 O18 149.2(3) . . ?
O20 Tb1 O18 85.3(3) . . ?
O28 Tb1 O18 71.9(3) . . ?
O25 Tb1 O18 134.8(3) . . ?
O19 Tb1 O18 72.6(3) . . ?
O69 Tb1 O77 72.1(3) . . ?
O20 Tb1 O77 128.7(3) . . ?
O28 Tb1 O77 153.4(3) . . ?
O25 Tb1 O77 83.4(3) . . ?
O19 Tb1 O77 69.0(3) . . ?
O18 Tb1 O77 111.9(3) . . ?
O69 Tb1 O17 133.2(3) . . ?
O20 Tb1 O17 155.2(3) . . ?
O28 Tb1 O17 83.6(3) . . ?
O25 Tb1 O17 70.7(3) . . ?
O19 Tb1 O17 113.3(3) . . ?
O18 Tb1 O17 73.8(3) . . ?
O77 Tb1 O17 72.9(3) . . ?
C1 N1 C3 112.3(15) . . ?
C6 N2 C8 110.9(14) . . ?
C12 N3 C9 108(2) . . ?
C16 N4 C14 109.9(16) . . ?
C20 N5 C18 102(2) . . ?
C23 N6 C21 126(4) . . ?
C25 N7 C28 115(2) . . ?
N1 C1 C2 111.4(15) . . ?
O79 C2 C1 107.1(13) . . ?
N1 C3 C4 111.2(15) . . ?
O79 C4 C3 111.4(15) . . ?
C6 C5 O80 108.7(13) . . ?
N2 C6 C5 112.3(15) . . ?
O80 C7 C8 109.2(15) . . ?
N2 C8 C7 111.5(16) . . ?
N3 C9 C10 108.8(19) . . ?
O81 C10 C9 108.2(19) . . ?
O81 C11 C12 110(2) . . ?
N3 C12 C11 108(2) . . ?
C14 C13 O82 110.4(18) . . ?
C13 C14 N4 111.5(18) . . ?
C16 C15 O82 111.8(16) . . ?
N4 C16 C15 110.1(16) . . ?
C18 C17 O85 106(2) . . ?
C17 C18 N5 114(3) . . ?
C20 C19 O85 108(2) . . ?
C19 C20 N5 116(3) . . ?
N6 C21 C22 113(4) . . ?
O84 C22 C21 111(4) . . ?
N6 C23 C24 111(4) . . ?
C23 C24 O84 108(3) . . ?
C26 C25 N7 107(2) . . ?
C25 C26 O83 109(2) . . ?
O83 C27 C28 107(2) . . ?
N7 C28 C27 109(2) . . ?

_refine_diff_density_max         0.948
_refine_diff_density_min         -1.068
_refine_diff_density_rms         0.156

_shelxl_version_number           2014-3


_vrf_CHEMW03_4_sq                
;
CHEMW03_ALERT_2_B

RESPONSE: Use of Platon SQUEEZE to remove disordered solvent. The accessible
solvent void in the crystal structure indicates that some more water molecules
and morpholine should exist in the structure, but cannot be found from the
weak residual electron peaks. Based on the TG analyses and elemental analysis,
14 water molecules and 8 morpholine were included in the sum formula.
;
_vrf_PLAT342_4_sq                
;
PLAT342_ALERT_3_B Low Bond Precision on C-C Bonds .............. 0.03929 Ang.

RESPONSE: The low bond distance precision is likely due to the low data to
parameter ratio. There is a large amount of disorder in the structure. This is
common in high nuclearity polyoxometalate cluster . (such as Angew. Chem. Int.
Ed, 2010, 49, 6984; Angew. Chem. Int. Ed, 2008, 47, 6881, J. Am. Chem. Soc,
2004, 126, 13880.)
;
_vrf_PLAT430_4_sq                
;
PLAT430_ALERT_2_B Short Inter D...A Contact O5...O57 ......2.77 Ang.

RESPONSE: The structure contains a high degree of disorder.
;

